164 Advances in Polymer Science
Editorial Board: A. Abe · A.-C. Albertsson · H.-J. Cantow K. Dusek · S. Edwards · H. H...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

164 Advances in Polymer Science

Editorial Board: A. Abe · A.-C. Albertsson · H.-J. Cantow K. Dusek · S. Edwards · H. Hcker J. F. Joanny · H.-H. Kausch · S. Kobayashi K.-S. Lee · I. Manners · O. Nuyken S. I. Stupp · U. W. Suter · G. Wegner

D Berlin Heidelberg New York Hong Kong London Milan Paris Tokyo

Filler-Reinforced Elastomers Scanning Force Microscopy

With contributions by B. Cappella · M. Geuss · M. Klppel M. Munz · E. Schulz · H. Sturm

BD

The series presents critical reviews of the present and future trends in polymer and biopolymer science including chemistry, physical chemistry, physics and material science. It is addressed to all scientists at universities and in industry who wish to keep abreast of advances in the topics covered. As a rule, contributions are specially commissioned. The editors and publishers will, however, always be pleased to receive suggestions and supplementary information. Papers are accepted for “Advances in Polymer Science” in English. In references Advances in Polymer Science is abbreviated Adv Polym Sci and is cited as a journal. The electronic content of APS may be found at http://www.SpringerLink.com

ISSN 0065-3195 ISBN 3-540-00530-7 DOI 10.1007/b10953 Springer-Verlag Berlin Heidelberg New York

Library of Congress Catalog Card Number 61642 This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, re-use of illustrations, recitation, broadcasting, reproduction on microfilms or in other ways, and storage in data banks. Duplication of this publication or parts thereof is only permitted under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer-Verlag. Violations are liable for prosecution under the German Copyright Law. Springer-Verlag Berlin Heidelberg New York a member of BertelsmannSpringer Science+Business Media GmbH http://www.springer.de Springer-Verlag Berlin Heidelberg 2003 Printed in Germany The use of registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Typesetting: Strtz AG, 97080 Wrzburg Cover: Design & Production, Heidelberg Printed on acid-free paper 02/3020/kk – 5 4 3 2 1 0

Editorial Board Prof. Akihiro Abe

Prof. Hans-Henning Kausch

Department of Industrial Chemistry Tokyo Institute of Polytechnics 1583 Iiyama, Atsugi-shi 243-02, Japan E-mail: [email protected]

c/o IGC I, Lab. of Polyelectrolytes and Biomacromolecules EPFL-Ecublens CH-1015 Lausanne, Switzerland E-mail: [email protected]

Prof. Ann-Christine Albertsson Department of Polymer Technology The Royal Institute of Technology S-10044 Stockholm, Sweden E-mail: [email protected]

Prof. Hans-Joachim Cantow Freiburger Materialforschungszentrum Stefan Meier-Str. 21 79104 Freiburg i. Br., Germany E-mail: [email protected]

Prof. Karel Dusek Institute of Macromolecular Chemistry, Czech Academy of Sciences of the Czech Republic Heyrovsky´ Sq. 2 16206 Prague 6, Czech Republic E-mail: [email protected]

Prof. Sam Edwards Department of Physics Cavendish Laboratory University of Cambridge Madingley Road Cambridge CB3 OHE, UK E-mail: [email protected]

Prof. Hartwig Hcker Lehrstuhl fr Textilchemie und Makromolekulare Chemie RWTH Aachen Veltmanplatz 8 52062 Aachen, Germany E-mail: [email protected]

Prof. Jean-Franois Joanny Institute Charles Sadron 6, rue Boussingault F-67083 Strasbourg Cedex, France E-mail: [email protected]

Prof. S. Kobayashi Department of Materials Chemistry Graduate School of Engineering Kyoto University Kyoto 606-8501, Japan E-mail: [email protected]

Prof. Prof. Kwang-Sup Lee Department of Polymer Science & Engineering Hannam University 133 Ojung-Dong Teajon 300-791, Korea E-mail: [email protected]

Prof. Ian Manners Department of Chemistry University of Toronto 80 St. George St. M5S 3H6 Ontario, Canada E-mail: [email protected]

Prof. Oskar Nuyken Lehrstuhl fr Makromolekulare Stoffe TU Mnchen Lichtenbergstr. 4 85747 Garching E-mail: [email protected]

Prof. Samuel I. Stupp Department of Measurement Materials Science and Engineering Northwestern University 2225 North Campus Drive Evanston, IL 60208-3113, USA E-mail: [email protected]

VI

Editorial Board

Prof. Ulrich W. Suter

Prof. Gerhard Wegner

Vice President for Research ETH Zentrum, HG F 57 CH-8092 Zrich, Switzerland E-mail: [email protected]

Max-Planck-Institut fr Polymerforschung Ackermannweg 10 Postfach 3148 55128 Mainz, Germany E-mail: [email protected]

Advances in Polymer Science Available Electronically

For all customers with a standing order for Advances in Polymer Science we offer the electronic form via SpringerLink free of charge. Please contact your librarian who can receive a password for free access to the full articles. By registration at: http://www.SpringerLink.com If you do not have a standing order you can nevertheless browse through the table of contents of the volumes and the abstracts of each article by choosing Advances in Polymer Science within the Chemistry Online Library. You will find information about the – Editorial Board – Aims and Scope – Instructions for Authors – Sample Contribution at www.springeronline.com using the search function.

Contents

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales M. Klppel . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

1

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM) and their Application to Polymers and Polymer Composites M. Munz, B. Cappella, H. Sturm, M. Geuss, E. Schulz . . . . . . . . . . . . . . . .

87

Author Index Volumes 101–164 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 211 Subject Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 225

Adv Polym Sci (2003) 164:1–86 DOI 10.1007/b11054

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales Manfred Klppel Deutsches Institut fr Kautschuktechnologie e. V., Eupener Strasse 33, 30519 Hannover, Germany E-mail: [email protected] Abstract The chapter considers the disordered nature of filler networks on different length scales and relates it to the specific reinforcing properties of active fillers in elastomer composites. On nanoscopic length scales, the surface structure and primary aggregate morphology of carbon blacks, the most widely used filler in technical rubber goods, are analyzed by static gas adsorption and transmission electron microscopy (TEM) techniques, respectively. They are found to be closely related to two distinct disordered growth mechanisms during carbon black processing, surface growth and aggregate growth. The role of disorder becomes also apparent on mesoscopic length scales of elastomer composites, where a filler network in formed due to attractive filler-filler interactions. An analysis of the d.c.-conductivity and dielectric properties of conductive carbon black-rubber composites indicates that no universal percolation structure is realized, but a superimposed kinetic aggregation mechanism of the particles takes place. The assumed kinetic cluster-cluster aggregation (CCA) of filler particles in elastomers is confirmed by the predicted scaling behavior of the small strain elastic modulus. Based on the analysis of in-rubber morphology of filler particles and clusters on nanoscopic and mesoscopic length scales, a constitutive micro-mechanical model of stress softening and hysteresis of filler reinforced rubbers up to large strain is developed. It refers to a non-affine tube model of rubber elasticity, including hydrodynamic amplification of the rubber matrix by a fraction of rigid filler clusters with filler-filler bonds in the unbroken, virgin state. The filler-induced hysteresis is described by an anisotropic free energy density, considering the cyclic breakdown and re-aggregation of the residual fraction of more fragile filler clusters with already broken filler-filler bonds. Experimental investigations of the quasi-static stress-strain behavior of silica and carbon black filled rubbers up to large strain agree well with adaptations found by the developed model. Keywords Elastomer composites · Disordered structures · Filler networking · Reinforcement · Micro-mechanics · Constitutive material laws

1

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

2

2

Experimental Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . .

8

2.1 2.2 2.3 2.4 2.5

Materials and Sample Preparation Gas Adsorption Measurements . . Microscopic Techniques. . . . . . . Mechanical Analysis . . . . . . . . . Dielectric Measurements . . . . . .

. . . . .

8 9 10 11 11

3

The Disordered Structure of Carbon Black . . . . . . . . . . . . . . .

12

3.1

Surface Roughness and Activity on Atomic Length Scales . . . . . .

12

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

Springer-Verlag Berlin Heidelberg 2003

2

Manfred Klppel

3.1.1 3.1.2 3.2 3.2.1 3.2.2

Universality of Carbon Black Surface Roughness. . . . . . . . . . . . Energy Distribution of Carbon Black Surfaces . . . . . . . . . . . . . Morphology of Carbon Black Aggregates on Nanoscales . . . . . . . Fractal Analysis of Primary Carbon Black Aggregates . . . . . . . . Effect of Mixing on In-Rubber Morphology of Primary Aggregates

12 19 24 25 29

4

Carbon Black Networking on Mesoscopic Length Scales . . . . . .

33

4.1 4.2 4.2.1 4.2.2 4.3

Microscopic and Scattering Analysis . . . . . . . . . . . . . . . . Investigations of Electrical Properties . . . . . . . . . . . . . . . . Percolation Behavior of the d.c.-Conductivity. . . . . . . . . . . Dielectric Analysis of Carbon Black Networks . . . . . . . . . . Flocculation Dynamics and the Nature of Filler-Filler Bonds .

. . . . .

33 35 35 38 45

5

Rubber Reinforcement by Fractal Filler Networks . . . . . . . . . .

51

5.1 5.1.1 5.1.2 5.1.3 5.2 5.2.1 5.2.2 5.2.3

Structure and Elasticity of Filler Networks at Small Strain. . . . Cluster-Cluster Aggregation (CCA) in Elastomers . . . . . . . . . Elasticity of Flexible Chains of Filler Particles. . . . . . . . . . . . Scaling Behavior of the Small Strain Modulus. . . . . . . . . . . . Stress Softening and Filler-Induced Hysteresis at Large Strain . Strength and Fracture of Filler Clusters in Elastomers . . . . . . Free Energy Density of Reinforced Rubbers . . . . . . . . . . . . . Stress-Strain Cycles of Filled Rubbers in the Quasi-Static Limit

. . . . . . . .

52 52 53 56 59 59 62 69

6

Summary and Conclusions . . . . . . . . . . . . . . . . . . . . . . . . .

79

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

82

. . . . .

. . . . . . . . . . . . .

1 Introduction Since the development of fractal geometry by Mandelbrot [1, 2] it has been learned that the apparently random structure of many colloidal aggregates formed in disorderly growth processes is subject to strong statistical constraints [3–8]. It is now well known that the fractal structure of colloidal aggregates results from the random movement, e.g., diffusion, of the aggregating particles that may be represented in computer simulations of cluster growth processes via random walks of single particles [3, 9] or whole clusters [10, 11]. Thereby, different universality classes of fractal aggregates can be distinguished by characteristic fractal exponents, dependent on the conditions of cluster growth [12]. In these studies we are primary interested in two classes of disorderly grown colloidal aggregates:

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

3

1. Clusters that are build in a diffusion limited cluster-cluster aggregation (CCA) process, where particles and clusters diffuse across each other and stick upon contact, irreversibly. 2. Clusters resulting from a ballistic cluster-cluster aggregation process, where particles and clusters move on linear trajectories.

A physical realization of the CCA-process is found during fast gelation of colloids in solution, where physical (and not chemical) bonds between particles and clusters are formed. From light scattering data of corresponding gold-, silica-, and polystyrene clusters as well as from computer simulations of CCA-clusters the fractal dimension takes the universal values df1.8 in all these cases [3–8, 12, 13]. The size distribution of the clusters is typically found to be broadly peaked around a maximum cluster size. This is in contrast to percolation clusters, where the size distribution shows a characteristic scaling behavior implying that the number of clusters increases successively with decreasing cluster size [6, 7]. A physical realization of ballistic cluster-cluster aggregation is found during carbon black processing, where surface growth due to random deposition of carbon nuclei also takes place [14–18]. Corresponding computer simulations of primary aggregate formation under ballistic conditions yields for the mass fractal dimension df1.95 [11, 12]. The surface growth of carbon black appears to be governed by a random deposition mechanism that falls into a universality class with a surface fractal dimension ds2.6 [3, 6, 7, 19]. We will consider the simultaneous cluster and surface growth of carbon black more closely in Sect. 3, where the energetic surface structure is also analyzed [20]. Recently it has been argued that CCA-clusters are also built in elastomer composites. Accordingly, their particular structure can be used for the modeling of rubber reinforcement by active fillers like carbon blacks or silica [21–23]. This approach is not evident, because long range diffusion of filler particles or clusters, as assumed in the CCA-process, is strongly suppressed in high viscosity media. Instead, the polymeric structure of highly entangled rubbers give rise to fluctuations of colloidal particles around their mean position with a fluctuation length of the order of the entanglement length of the rubber [22–24]. For that reason the assumption of CCA-clusters in filler reinforced rubbers appears reasonable for sufficient large filler concentrations, only, where the mean trajectory length of aggregating particles or clusters becomes smaller than the fluctuation length. This condition is fulfilled for filler concentrations F above the gel point F* of the filler network if the gelation concept of Ball and Brown is applied [25]. Then, the mean trajectory length in gelling systems becomes small and the cluster size is governed by the available empty space only. However, due to the restricted mobility of filler particles in rubber the gel point is shifted to filler concentrations that are orders of magnitude larger than the critical concentration F* in solution [22, 23]. This is the main difference between the two systems that appears to be important for rubber reinforcement.

4

Manfred Klppel

Fig. 1 Schematic view of filler morphology in three concentration regimes. For FF+) with Feff=F or Feff=F/FA, respectively. For F>F* reinforcement is due to the deformation of a flexible filler network

Different concentration limits of the filler arise from the CCA concept [22]. With increasing filler concentration first an aggregation limit F+ is reached. For F>F+, the distance of neighboring filler particles becomes sufficiently small for the onset of flocculation and clusters with solid fraction FA are formed. Dependent on the concentration of filler particles, this flocculation process leads to spatially separated clusters or, for F>F*, a through going filler network that can be considered as a space-filling configuration of fractal CCA-clusters. The different cases for spherical filler particles are shown schematically in Fig. 1. So far, the formation and structure of filler networks in elastomers and the mechanical response, e.g., the pronounced dynamic amplitude dependence or stress softening, of reinforced rubbers, is not fully understood, though this question is of high technical interest. A deeper understanding of filler networking and reinforcement could provide a useful tool for the design, preparation, and testing of high performance elastomers, as applied in tires, seals, bearings, and other dynamically loaded elastomer components. Different attempts have been considered in the past that were primary focusing on the reinforcing mechanism of carbon black, the most widely used filler in rubber industry [26, 27]. The strongly non-linear dynamic-mechanical response of carbon black filled rubbers, reflected primarily by the amplitude dependence of the viscoelastic complex modulus, was brought into clear focus by the extensive work of Payne [28–35]. Therefore, this effect is often referred to as the Payne effect. As shown in Fig. 2a, for a specific frequency and temperature, the storage modulus G0 decreases from a small strain plateau value G0 o to an apparently high amplitude plateau value G0 1 with increasing strain amplitude. The loss modulus G00 shows a more or less pronounced peak. It can be evaluated from the tangent of the measured loss angle, tan d=G00 /G00 , as depicted in Fig. 2b. Obviously, the loss tangent shows a low plateau value at small strain amplitude, almost independent of filler concentration, and passes through a broad maximum with increasing strain.

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

5

Fig. 2 a Amplitude dependence of the storage modulus of Butyl/N330-samples. b Amplitude dependence of the loss tangent of the same Butyl/N330-samples at various carbon black concentrations [28]

The Payne effect of carbon black reinforced rubbers has also been investigated intensively by a number of different researchers [36–39]. In most cases, standard diene rubbers widely used in the tire industry, like SBR, NR, and BR, have been applied, but also carbon black filled bromobutyl rubbers [40–42] or functional rubbers containing tin end-modified polymers [43] were used. The Payne effect was described in the framework of various experimental procedures, including pre-conditioning-, recovery- and dynamic stress-softening studies [44]. The typically almost reversible, non-linear response found for carbon black composites has also been observed for silica filled rubbers [44–46]. The temperature dependence of the Payne effect has been studied by Payne and other authors [28, 32, 47]. With increasing temperature an Arrhenius-like drop of the moduli is found if the deformation amplitude is kept constant. Beside this effect, the impact of filler surface characteristics in the non-linear dynamic properties of filler reinforced rubbers has been discussed in a review of Wang [47], where basic theoretical interpretations and modeling is presented. The Payne effect has also been investigated in composites containing polymeric model fillers, like microgels of different particle size and surface chemistry, which could provide some more insight into the fundamental mechanisms of rubber reinforcement by colloidal fillers [48, 49]. The pronounced amplitude dependence of the complex modulus, referred to as the Payne effect, has also been observed in low viscosity media, e.g., composites of carbon black with decane and liquid paraffin [50], carbon black suspensions in ethylene vinylacetate copolymers [51], and clay/water suspensions [52, 53]. It was found that the storage modulus decreases with

6

Manfred Klppel

dynamic strain amplitude in a qualitative manner similar to that of carbon black filled rubbers. This emphasizes the role of a physically bonded filler network structure in the Payne effect, which governs the small strain dynamic properties even in absence of rubber. Further, these results indicate that the Payne effect is primarily determined by structure effects of the filler. The elastomer seems to act merely as a dispersing medium that influences the kinetics of filler aggregation, but does not have a pronounced influence on the overall mechanical behavior of three-dimensional filler networks. However, the critical strain amplitude where the Payne effect appears is found to be shifted to significantly smaller values, if the low viscosity composites are compared to corresponding rubber composites. This indicates a strong impact of the polymer-matrix on the stability and strength of filler networks. The strong non-linearity of the viscoelastic modulus with increasing dynamic strain amplitude has been related to a cyclic breakdown and re-aggregation of filler-filler bonds [21–23, 48, 54–57]. Thereby, different geometrical arrangements of particles in a particular filler network structure, resulting, e.g., from percolation as in the L-N-B-model of Lin and Lee [56] or kinetic cluster-cluster aggregation [21–23, 48], have been considered. Nevertheless, a full micro-mechanical description of energy storage and -dissipation in dynamically excited reinforced rubbers is still outstanding. A review of the different attempts is given by Heinrich and Klppel [57]. Beside the Payne effect, relevant for dynamical loading of filler reinforced rubbers, the pronounced stress softening, characteristic for quasi-static deformations up to large strain, is of major interest for technical applications. It is often referred to as the Mullins effect due to the extensive studies of Mullins and coworkers [58–60] on the stress softening phenomena. Dependent on the history of straining, e.g., the extent of previous stretching, the rubber material undergoes an almost permanent change that alters the elastic properties and increases hysteresis, drastically. Most of the softening occurs in the first deformation and after a few deformation cycles the rubber approaches a steady state with a constant stress-strain behavior. The softening is usually only present at deformations smaller than the previous maximum. An example of (discontinuous) stress softening is shown in Fig. 3, where the maximum strain is increased, successively, from one uniaxial stretching cycle to the next. So far the micro-mechanical origin of the Mullins effect is not totally understood [26, 36, 61]. Beside the action of the entropy elastic polymer network that is quite well understood on a molecular-statistical basis [24, 62], the impact of filler particles on stress-strain properties is of high importance. On the one hand the addition of hard filler particles leads to a stiffening of the rubber matrix that can be described by a hydrodynamic strain amplification factor [22, 63–65]. On the other, the constraints introduced into the system by filler-polymer bonds result in a decreased network entropy. Accordingly, the free energy that equals the negative entropy times the temperature increases linear with the effective number of network junctions [64–67]. A further effect is obtained from the formation of filler clusters or a

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

7

Fig. 3 Example of stress softening with successively increasing maximum strain for an E-SBR-sample filled with 80 phr N 339

filler network due to strong attractive filler-filler bonds [21, 22, 26, 36, 61, 64–67]. Stress softening is supposed to be affected by different influences and mechanisms that have been discussed by a variety of authors. In particular, it has been attributed to a breakdown or slippage [68–71] and disentanglements [72] of bonds between filler and rubber, a strain-induced crystallization-decrystallization [73, 74], or a rearrangement of network chain junctions in filled systems [60]. A model of stress-induced rupture or separation of network chains from the filler surface has been derived by Govindjee and Simo [69], who developed a complete macroscopic constitutive theory on the basis of statistical mechanics. A remarkable approach has been proposed by Witten et al. [21], who found a scaling law for the stress-strain behavior in the first stretching cycle by modeling the breakdown of a CCA-network of filler particles. They used purely geometrical arguments by referring to the available space for the filler clusters in strained samples, leading to universal scaling exponents that involve the characteristic fractal exponents of CCAclusters. However, they did not consider effects coming in from the rubber matrix or the polymer-filler interaction strength, though these are evident from experimental data, e.g., the impact of matrix cross-linking or filler surface treatment (graphitization) on stress-strain curves. It indicates that stress-induced breakdown of filler clusters takes place, where the stress on the filler clusters is transmitted by the rubber matrix. The above interpretations of the Mullins effect of stress softening ignore the important results of Haarwood et al. [73, 74], who showed that a plot of stress in second extension vs ratio between strain and pre-strain of natural rubber filled with a variety of carbon blacks yields a single master curve [60, 73]. This demonstrates that stress softening is related to hydrodynamic strain amplification due to the presence of the filler. Based on this observation a micro-mechanical model of stress softening has been developed by referring to hydrodynamic reinforcement of the rubber matrix by rigid filler

8

Manfred Klppel

clusters that are irreversibly broken during the first deformation cycle [75, 76]. Thereby, a non-Gaussian tube model of rubber elasticity has been applied [24, 62, 77, 78]. In the present chapter we will first focus on the specific morphology and energetic surface properties of carbon black (Sect. 3). In particular, we will consider the surface roughness and activity on atomic length scales as obtained by recent gas adsorption investigations [20, 79–82]. Then, we will concentrate on the primary aggregate structure that can be well characterized by TEM-measurements [83–85]. Both morphological characteristics of carbon black are compared to results of computer simulations and analytical models of disorderly growth processes under ballistic conditions [18, 84]. In Sect. 4, we will consider the structures involved in secondary aggregation and networking of carbon black in elastomers [22, 23] that has also been extended to elastomer blends [86, 87]. We will discuss the developed model in the framework of experimental results concerning filler flocculation and dielectric properties of carbon black reinforced rubbers. Based on the investigations of carbon black morphology and energetic surface structure we will then develop a model of rubber reinforcement by kinetically aggregated filler networks in Sect. 5. We will first consider the linear viscoelastic behavior by referring to the elasticity of the fractal CCA-unit cells of the filler network [22, 23, 48, 57, 85, 88]. Then, we will focus on a micro-mechanical concept of stress-induced filler cluster breakdown that combines the hyperelastic response of the hydrodynamically reinforced rubber matrix with the non-linear viscoelastic response of reversibly broken filler clusters [75, 76, 89]. It allows for an explanation of both, the Payne effect and the Mullins effect, by referring to a single micro-mechanical mechanism.

2 Experimental Methods 2.1 Materials and Sample Preparation

For the preparation of filler reinforced elastomer composites, most frequently commercial rubber grades with variable microstructure and broad molar mass distribution are applied. The typical rubber grades, considered in the present review, are as follows: 1. Natural rubber NR (SMR 5L; 99.9 vol.% cis) 2. Solution-styrene-butadiene rubber S-SBR (Buna VSL-2525–0; 25 vol.% vinyl, 25 vol.% styrene, Mw=206,600 g/mol, Mw/Mn=2.75) 3. Emulsion-styrene-butadiene rubber E-SBR (Intol 1524; 15 vol.% vinyl, 23.5 vol.% styrene, Mw=205,300 g/mol, Mw/Mn=2.12) 4. Ethylene-propylene-diene rubber EPDM (Keltan 512; 55 vol.% ethylene) 5. Nitrile-butadiene rubber NBR (Perbunan 3307; 33 vol.% acryl-nitrile)

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

9

In addition to the commercial rubber grades, model polymers with variable molar mass and narrow molecular weight distribution are often used for studying reinforcement mechanisms. (In Sect. 4.3 we consider a special S-SBR type with 29 vol.% vinyl and 25 vol.% styrene units; Mw/Mn=1.1). In general, furnace carbon blacks with different structure and specific surface area are employed as reinforcing fillers. Furthermore, commercial silica grades are applied, especially in the tire industry. In Sect. 5 we refer to a highly dispersive silica grade (Ultrasil 7000 GR) together with a bi-functional silane as coupling agent (Si 69).) The filler loading can range from very small amounts up to 100 phr. The notation “per hundred rubber” (phr), representing the mass (in grams) of an ingredient with respect to 100 g of rubber, is widely used in the rubber industry. The conversion to volume fraction F is obtained by the elementary formula F=phr/rCB (100 g/ rPol+phr/rCB)1, where phr is the mass of carbon black (in grams) per 100 g polymer, while rPol0.9 g/cm3 and rCB1.8 g/cm3 is the mass density of the pure polymer and carbon black, respectively. As polymeric model fillers with specific surface groups and narrow size distribution, different microgel types, e.g., poly(styrene)-microgel, PS(m), and poly(methoxy-styrene)-microgel, PMS(m), are applied. They can be prepared by emulsion polymerization techniques as described, e.g., in [48]. The rubber composites are in general processed in an interlocking mixer, as widely used in rubber industry, e.g., Werner & Pfleiderer GK 1.5 E with a mixing chamber of 1500 cm3. For obtaining a sufficient dispersion of the filler, at least 4 min mixing time are necessary. For the silica/silane systems, most frequently a two step mixing procedure is applied, for obtaining a reasonable coating reaction of the silane on the silica surface. Furthermore, a small amount of ZnO and stearinic acid is added to all compounds for supporting a fast filler dispersion and vulcanization. In general, the mixer is filled up to 75% of its capacity for the specimens with less than 40 phr filler, 70% for loading between 40 and 70 phr, and 60% for more than 70 phr filler. The cross-linking system is added on a roller mill in a separate mixing step (Here, 1.7 phr sulfur and 2.5 phr N-cyclohexylbenzothiazol-2-sulfenamide (CBS) is used). The composites with graphitized blacks are mixed on a roller mill for 20 min to ensure a sufficient dispersion. The composites are cured in a steam press, most frequently up to 90% of the rheometer optimum (T90 time) at 160 C. 2.2 Gas Adsorption Measurements

The morphological and energetic surface characterization of carbon black on atomic length scales can be performed by volumetric gas adsorption techniques. A schematic view of three different application regimes of this technique is shown in Fig. 4. According to this scheme, the surface roughness of particular fillers is estimated in the mono- and multi-layer regime. Furthermore, a characterization of the energy distribution of adsorption sites of carbon black and other colloids is obtained in the sub-layer regime.

10

Manfred Klppel

Fig. 4 Schematic representation of gas adsorption techniques in different layer regimes (decreasing pressure from top to bottom)

A classical volumetric adsorption apparatus equipped with absolute capacitance pressures transducers can be used for the estimation of adsorption isotherms in the pressure range 103 mbar

Editorial Board: A. Abe · A.-C. Albertsson · H.-J. Cantow K. Dusek · S. Edwards · H. Hcker J. F. Joanny · H.-H. Kausch · S. Kobayashi K.-S. Lee · I. Manners · O. Nuyken S. I. Stupp · U. W. Suter · G. Wegner

D Berlin Heidelberg New York Hong Kong London Milan Paris Tokyo

Filler-Reinforced Elastomers Scanning Force Microscopy

With contributions by B. Cappella · M. Geuss · M. Klppel M. Munz · E. Schulz · H. Sturm

BD

The series presents critical reviews of the present and future trends in polymer and biopolymer science including chemistry, physical chemistry, physics and material science. It is addressed to all scientists at universities and in industry who wish to keep abreast of advances in the topics covered. As a rule, contributions are specially commissioned. The editors and publishers will, however, always be pleased to receive suggestions and supplementary information. Papers are accepted for “Advances in Polymer Science” in English. In references Advances in Polymer Science is abbreviated Adv Polym Sci and is cited as a journal. The electronic content of APS may be found at http://www.SpringerLink.com

ISSN 0065-3195 ISBN 3-540-00530-7 DOI 10.1007/b10953 Springer-Verlag Berlin Heidelberg New York

Library of Congress Catalog Card Number 61642 This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, re-use of illustrations, recitation, broadcasting, reproduction on microfilms or in other ways, and storage in data banks. Duplication of this publication or parts thereof is only permitted under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer-Verlag. Violations are liable for prosecution under the German Copyright Law. Springer-Verlag Berlin Heidelberg New York a member of BertelsmannSpringer Science+Business Media GmbH http://www.springer.de Springer-Verlag Berlin Heidelberg 2003 Printed in Germany The use of registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Typesetting: Strtz AG, 97080 Wrzburg Cover: Design & Production, Heidelberg Printed on acid-free paper 02/3020/kk – 5 4 3 2 1 0

Editorial Board Prof. Akihiro Abe

Prof. Hans-Henning Kausch

Department of Industrial Chemistry Tokyo Institute of Polytechnics 1583 Iiyama, Atsugi-shi 243-02, Japan E-mail: [email protected]

c/o IGC I, Lab. of Polyelectrolytes and Biomacromolecules EPFL-Ecublens CH-1015 Lausanne, Switzerland E-mail: [email protected]

Prof. Ann-Christine Albertsson Department of Polymer Technology The Royal Institute of Technology S-10044 Stockholm, Sweden E-mail: [email protected]

Prof. Hans-Joachim Cantow Freiburger Materialforschungszentrum Stefan Meier-Str. 21 79104 Freiburg i. Br., Germany E-mail: [email protected]

Prof. Karel Dusek Institute of Macromolecular Chemistry, Czech Academy of Sciences of the Czech Republic Heyrovsky´ Sq. 2 16206 Prague 6, Czech Republic E-mail: [email protected]

Prof. Sam Edwards Department of Physics Cavendish Laboratory University of Cambridge Madingley Road Cambridge CB3 OHE, UK E-mail: [email protected]

Prof. Hartwig Hcker Lehrstuhl fr Textilchemie und Makromolekulare Chemie RWTH Aachen Veltmanplatz 8 52062 Aachen, Germany E-mail: [email protected]

Prof. Jean-Franois Joanny Institute Charles Sadron 6, rue Boussingault F-67083 Strasbourg Cedex, France E-mail: [email protected]

Prof. S. Kobayashi Department of Materials Chemistry Graduate School of Engineering Kyoto University Kyoto 606-8501, Japan E-mail: [email protected]

Prof. Prof. Kwang-Sup Lee Department of Polymer Science & Engineering Hannam University 133 Ojung-Dong Teajon 300-791, Korea E-mail: [email protected]

Prof. Ian Manners Department of Chemistry University of Toronto 80 St. George St. M5S 3H6 Ontario, Canada E-mail: [email protected]

Prof. Oskar Nuyken Lehrstuhl fr Makromolekulare Stoffe TU Mnchen Lichtenbergstr. 4 85747 Garching E-mail: [email protected]

Prof. Samuel I. Stupp Department of Measurement Materials Science and Engineering Northwestern University 2225 North Campus Drive Evanston, IL 60208-3113, USA E-mail: [email protected]

VI

Editorial Board

Prof. Ulrich W. Suter

Prof. Gerhard Wegner

Vice President for Research ETH Zentrum, HG F 57 CH-8092 Zrich, Switzerland E-mail: [email protected]

Max-Planck-Institut fr Polymerforschung Ackermannweg 10 Postfach 3148 55128 Mainz, Germany E-mail: [email protected]

Advances in Polymer Science Available Electronically

For all customers with a standing order for Advances in Polymer Science we offer the electronic form via SpringerLink free of charge. Please contact your librarian who can receive a password for free access to the full articles. By registration at: http://www.SpringerLink.com If you do not have a standing order you can nevertheless browse through the table of contents of the volumes and the abstracts of each article by choosing Advances in Polymer Science within the Chemistry Online Library. You will find information about the – Editorial Board – Aims and Scope – Instructions for Authors – Sample Contribution at www.springeronline.com using the search function.

Contents

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales M. Klppel . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

1

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM) and their Application to Polymers and Polymer Composites M. Munz, B. Cappella, H. Sturm, M. Geuss, E. Schulz . . . . . . . . . . . . . . . .

87

Author Index Volumes 101–164 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 211 Subject Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 225

Adv Polym Sci (2003) 164:1–86 DOI 10.1007/b11054

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales Manfred Klppel Deutsches Institut fr Kautschuktechnologie e. V., Eupener Strasse 33, 30519 Hannover, Germany E-mail: [email protected] Abstract The chapter considers the disordered nature of filler networks on different length scales and relates it to the specific reinforcing properties of active fillers in elastomer composites. On nanoscopic length scales, the surface structure and primary aggregate morphology of carbon blacks, the most widely used filler in technical rubber goods, are analyzed by static gas adsorption and transmission electron microscopy (TEM) techniques, respectively. They are found to be closely related to two distinct disordered growth mechanisms during carbon black processing, surface growth and aggregate growth. The role of disorder becomes also apparent on mesoscopic length scales of elastomer composites, where a filler network in formed due to attractive filler-filler interactions. An analysis of the d.c.-conductivity and dielectric properties of conductive carbon black-rubber composites indicates that no universal percolation structure is realized, but a superimposed kinetic aggregation mechanism of the particles takes place. The assumed kinetic cluster-cluster aggregation (CCA) of filler particles in elastomers is confirmed by the predicted scaling behavior of the small strain elastic modulus. Based on the analysis of in-rubber morphology of filler particles and clusters on nanoscopic and mesoscopic length scales, a constitutive micro-mechanical model of stress softening and hysteresis of filler reinforced rubbers up to large strain is developed. It refers to a non-affine tube model of rubber elasticity, including hydrodynamic amplification of the rubber matrix by a fraction of rigid filler clusters with filler-filler bonds in the unbroken, virgin state. The filler-induced hysteresis is described by an anisotropic free energy density, considering the cyclic breakdown and re-aggregation of the residual fraction of more fragile filler clusters with already broken filler-filler bonds. Experimental investigations of the quasi-static stress-strain behavior of silica and carbon black filled rubbers up to large strain agree well with adaptations found by the developed model. Keywords Elastomer composites · Disordered structures · Filler networking · Reinforcement · Micro-mechanics · Constitutive material laws

1

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

2

2

Experimental Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . .

8

2.1 2.2 2.3 2.4 2.5

Materials and Sample Preparation Gas Adsorption Measurements . . Microscopic Techniques. . . . . . . Mechanical Analysis . . . . . . . . . Dielectric Measurements . . . . . .

. . . . .

8 9 10 11 11

3

The Disordered Structure of Carbon Black . . . . . . . . . . . . . . .

12

3.1

Surface Roughness and Activity on Atomic Length Scales . . . . . .

12

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

Springer-Verlag Berlin Heidelberg 2003

2

Manfred Klppel

3.1.1 3.1.2 3.2 3.2.1 3.2.2

Universality of Carbon Black Surface Roughness. . . . . . . . . . . . Energy Distribution of Carbon Black Surfaces . . . . . . . . . . . . . Morphology of Carbon Black Aggregates on Nanoscales . . . . . . . Fractal Analysis of Primary Carbon Black Aggregates . . . . . . . . Effect of Mixing on In-Rubber Morphology of Primary Aggregates

12 19 24 25 29

4

Carbon Black Networking on Mesoscopic Length Scales . . . . . .

33

4.1 4.2 4.2.1 4.2.2 4.3

Microscopic and Scattering Analysis . . . . . . . . . . . . . . . . Investigations of Electrical Properties . . . . . . . . . . . . . . . . Percolation Behavior of the d.c.-Conductivity. . . . . . . . . . . Dielectric Analysis of Carbon Black Networks . . . . . . . . . . Flocculation Dynamics and the Nature of Filler-Filler Bonds .

. . . . .

33 35 35 38 45

5

Rubber Reinforcement by Fractal Filler Networks . . . . . . . . . .

51

5.1 5.1.1 5.1.2 5.1.3 5.2 5.2.1 5.2.2 5.2.3

Structure and Elasticity of Filler Networks at Small Strain. . . . Cluster-Cluster Aggregation (CCA) in Elastomers . . . . . . . . . Elasticity of Flexible Chains of Filler Particles. . . . . . . . . . . . Scaling Behavior of the Small Strain Modulus. . . . . . . . . . . . Stress Softening and Filler-Induced Hysteresis at Large Strain . Strength and Fracture of Filler Clusters in Elastomers . . . . . . Free Energy Density of Reinforced Rubbers . . . . . . . . . . . . . Stress-Strain Cycles of Filled Rubbers in the Quasi-Static Limit

. . . . . . . .

52 52 53 56 59 59 62 69

6

Summary and Conclusions . . . . . . . . . . . . . . . . . . . . . . . . .

79

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

82

. . . . .

. . . . . . . . . . . . .

1 Introduction Since the development of fractal geometry by Mandelbrot [1, 2] it has been learned that the apparently random structure of many colloidal aggregates formed in disorderly growth processes is subject to strong statistical constraints [3–8]. It is now well known that the fractal structure of colloidal aggregates results from the random movement, e.g., diffusion, of the aggregating particles that may be represented in computer simulations of cluster growth processes via random walks of single particles [3, 9] or whole clusters [10, 11]. Thereby, different universality classes of fractal aggregates can be distinguished by characteristic fractal exponents, dependent on the conditions of cluster growth [12]. In these studies we are primary interested in two classes of disorderly grown colloidal aggregates:

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

3

1. Clusters that are build in a diffusion limited cluster-cluster aggregation (CCA) process, where particles and clusters diffuse across each other and stick upon contact, irreversibly. 2. Clusters resulting from a ballistic cluster-cluster aggregation process, where particles and clusters move on linear trajectories.

A physical realization of the CCA-process is found during fast gelation of colloids in solution, where physical (and not chemical) bonds between particles and clusters are formed. From light scattering data of corresponding gold-, silica-, and polystyrene clusters as well as from computer simulations of CCA-clusters the fractal dimension takes the universal values df1.8 in all these cases [3–8, 12, 13]. The size distribution of the clusters is typically found to be broadly peaked around a maximum cluster size. This is in contrast to percolation clusters, where the size distribution shows a characteristic scaling behavior implying that the number of clusters increases successively with decreasing cluster size [6, 7]. A physical realization of ballistic cluster-cluster aggregation is found during carbon black processing, where surface growth due to random deposition of carbon nuclei also takes place [14–18]. Corresponding computer simulations of primary aggregate formation under ballistic conditions yields for the mass fractal dimension df1.95 [11, 12]. The surface growth of carbon black appears to be governed by a random deposition mechanism that falls into a universality class with a surface fractal dimension ds2.6 [3, 6, 7, 19]. We will consider the simultaneous cluster and surface growth of carbon black more closely in Sect. 3, where the energetic surface structure is also analyzed [20]. Recently it has been argued that CCA-clusters are also built in elastomer composites. Accordingly, their particular structure can be used for the modeling of rubber reinforcement by active fillers like carbon blacks or silica [21–23]. This approach is not evident, because long range diffusion of filler particles or clusters, as assumed in the CCA-process, is strongly suppressed in high viscosity media. Instead, the polymeric structure of highly entangled rubbers give rise to fluctuations of colloidal particles around their mean position with a fluctuation length of the order of the entanglement length of the rubber [22–24]. For that reason the assumption of CCA-clusters in filler reinforced rubbers appears reasonable for sufficient large filler concentrations, only, where the mean trajectory length of aggregating particles or clusters becomes smaller than the fluctuation length. This condition is fulfilled for filler concentrations F above the gel point F* of the filler network if the gelation concept of Ball and Brown is applied [25]. Then, the mean trajectory length in gelling systems becomes small and the cluster size is governed by the available empty space only. However, due to the restricted mobility of filler particles in rubber the gel point is shifted to filler concentrations that are orders of magnitude larger than the critical concentration F* in solution [22, 23]. This is the main difference between the two systems that appears to be important for rubber reinforcement.

4

Manfred Klppel

Fig. 1 Schematic view of filler morphology in three concentration regimes. For F

Different concentration limits of the filler arise from the CCA concept [22]. With increasing filler concentration first an aggregation limit F+ is reached. For F>F+, the distance of neighboring filler particles becomes sufficiently small for the onset of flocculation and clusters with solid fraction FA are formed. Dependent on the concentration of filler particles, this flocculation process leads to spatially separated clusters or, for F>F*, a through going filler network that can be considered as a space-filling configuration of fractal CCA-clusters. The different cases for spherical filler particles are shown schematically in Fig. 1. So far, the formation and structure of filler networks in elastomers and the mechanical response, e.g., the pronounced dynamic amplitude dependence or stress softening, of reinforced rubbers, is not fully understood, though this question is of high technical interest. A deeper understanding of filler networking and reinforcement could provide a useful tool for the design, preparation, and testing of high performance elastomers, as applied in tires, seals, bearings, and other dynamically loaded elastomer components. Different attempts have been considered in the past that were primary focusing on the reinforcing mechanism of carbon black, the most widely used filler in rubber industry [26, 27]. The strongly non-linear dynamic-mechanical response of carbon black filled rubbers, reflected primarily by the amplitude dependence of the viscoelastic complex modulus, was brought into clear focus by the extensive work of Payne [28–35]. Therefore, this effect is often referred to as the Payne effect. As shown in Fig. 2a, for a specific frequency and temperature, the storage modulus G0 decreases from a small strain plateau value G0 o to an apparently high amplitude plateau value G0 1 with increasing strain amplitude. The loss modulus G00 shows a more or less pronounced peak. It can be evaluated from the tangent of the measured loss angle, tan d=G00 /G00 , as depicted in Fig. 2b. Obviously, the loss tangent shows a low plateau value at small strain amplitude, almost independent of filler concentration, and passes through a broad maximum with increasing strain.

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

5

Fig. 2 a Amplitude dependence of the storage modulus of Butyl/N330-samples. b Amplitude dependence of the loss tangent of the same Butyl/N330-samples at various carbon black concentrations [28]

The Payne effect of carbon black reinforced rubbers has also been investigated intensively by a number of different researchers [36–39]. In most cases, standard diene rubbers widely used in the tire industry, like SBR, NR, and BR, have been applied, but also carbon black filled bromobutyl rubbers [40–42] or functional rubbers containing tin end-modified polymers [43] were used. The Payne effect was described in the framework of various experimental procedures, including pre-conditioning-, recovery- and dynamic stress-softening studies [44]. The typically almost reversible, non-linear response found for carbon black composites has also been observed for silica filled rubbers [44–46]. The temperature dependence of the Payne effect has been studied by Payne and other authors [28, 32, 47]. With increasing temperature an Arrhenius-like drop of the moduli is found if the deformation amplitude is kept constant. Beside this effect, the impact of filler surface characteristics in the non-linear dynamic properties of filler reinforced rubbers has been discussed in a review of Wang [47], where basic theoretical interpretations and modeling is presented. The Payne effect has also been investigated in composites containing polymeric model fillers, like microgels of different particle size and surface chemistry, which could provide some more insight into the fundamental mechanisms of rubber reinforcement by colloidal fillers [48, 49]. The pronounced amplitude dependence of the complex modulus, referred to as the Payne effect, has also been observed in low viscosity media, e.g., composites of carbon black with decane and liquid paraffin [50], carbon black suspensions in ethylene vinylacetate copolymers [51], and clay/water suspensions [52, 53]. It was found that the storage modulus decreases with

6

Manfred Klppel

dynamic strain amplitude in a qualitative manner similar to that of carbon black filled rubbers. This emphasizes the role of a physically bonded filler network structure in the Payne effect, which governs the small strain dynamic properties even in absence of rubber. Further, these results indicate that the Payne effect is primarily determined by structure effects of the filler. The elastomer seems to act merely as a dispersing medium that influences the kinetics of filler aggregation, but does not have a pronounced influence on the overall mechanical behavior of three-dimensional filler networks. However, the critical strain amplitude where the Payne effect appears is found to be shifted to significantly smaller values, if the low viscosity composites are compared to corresponding rubber composites. This indicates a strong impact of the polymer-matrix on the stability and strength of filler networks. The strong non-linearity of the viscoelastic modulus with increasing dynamic strain amplitude has been related to a cyclic breakdown and re-aggregation of filler-filler bonds [21–23, 48, 54–57]. Thereby, different geometrical arrangements of particles in a particular filler network structure, resulting, e.g., from percolation as in the L-N-B-model of Lin and Lee [56] or kinetic cluster-cluster aggregation [21–23, 48], have been considered. Nevertheless, a full micro-mechanical description of energy storage and -dissipation in dynamically excited reinforced rubbers is still outstanding. A review of the different attempts is given by Heinrich and Klppel [57]. Beside the Payne effect, relevant for dynamical loading of filler reinforced rubbers, the pronounced stress softening, characteristic for quasi-static deformations up to large strain, is of major interest for technical applications. It is often referred to as the Mullins effect due to the extensive studies of Mullins and coworkers [58–60] on the stress softening phenomena. Dependent on the history of straining, e.g., the extent of previous stretching, the rubber material undergoes an almost permanent change that alters the elastic properties and increases hysteresis, drastically. Most of the softening occurs in the first deformation and after a few deformation cycles the rubber approaches a steady state with a constant stress-strain behavior. The softening is usually only present at deformations smaller than the previous maximum. An example of (discontinuous) stress softening is shown in Fig. 3, where the maximum strain is increased, successively, from one uniaxial stretching cycle to the next. So far the micro-mechanical origin of the Mullins effect is not totally understood [26, 36, 61]. Beside the action of the entropy elastic polymer network that is quite well understood on a molecular-statistical basis [24, 62], the impact of filler particles on stress-strain properties is of high importance. On the one hand the addition of hard filler particles leads to a stiffening of the rubber matrix that can be described by a hydrodynamic strain amplification factor [22, 63–65]. On the other, the constraints introduced into the system by filler-polymer bonds result in a decreased network entropy. Accordingly, the free energy that equals the negative entropy times the temperature increases linear with the effective number of network junctions [64–67]. A further effect is obtained from the formation of filler clusters or a

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

7

Fig. 3 Example of stress softening with successively increasing maximum strain for an E-SBR-sample filled with 80 phr N 339

filler network due to strong attractive filler-filler bonds [21, 22, 26, 36, 61, 64–67]. Stress softening is supposed to be affected by different influences and mechanisms that have been discussed by a variety of authors. In particular, it has been attributed to a breakdown or slippage [68–71] and disentanglements [72] of bonds between filler and rubber, a strain-induced crystallization-decrystallization [73, 74], or a rearrangement of network chain junctions in filled systems [60]. A model of stress-induced rupture or separation of network chains from the filler surface has been derived by Govindjee and Simo [69], who developed a complete macroscopic constitutive theory on the basis of statistical mechanics. A remarkable approach has been proposed by Witten et al. [21], who found a scaling law for the stress-strain behavior in the first stretching cycle by modeling the breakdown of a CCA-network of filler particles. They used purely geometrical arguments by referring to the available space for the filler clusters in strained samples, leading to universal scaling exponents that involve the characteristic fractal exponents of CCAclusters. However, they did not consider effects coming in from the rubber matrix or the polymer-filler interaction strength, though these are evident from experimental data, e.g., the impact of matrix cross-linking or filler surface treatment (graphitization) on stress-strain curves. It indicates that stress-induced breakdown of filler clusters takes place, where the stress on the filler clusters is transmitted by the rubber matrix. The above interpretations of the Mullins effect of stress softening ignore the important results of Haarwood et al. [73, 74], who showed that a plot of stress in second extension vs ratio between strain and pre-strain of natural rubber filled with a variety of carbon blacks yields a single master curve [60, 73]. This demonstrates that stress softening is related to hydrodynamic strain amplification due to the presence of the filler. Based on this observation a micro-mechanical model of stress softening has been developed by referring to hydrodynamic reinforcement of the rubber matrix by rigid filler

8

Manfred Klppel

clusters that are irreversibly broken during the first deformation cycle [75, 76]. Thereby, a non-Gaussian tube model of rubber elasticity has been applied [24, 62, 77, 78]. In the present chapter we will first focus on the specific morphology and energetic surface properties of carbon black (Sect. 3). In particular, we will consider the surface roughness and activity on atomic length scales as obtained by recent gas adsorption investigations [20, 79–82]. Then, we will concentrate on the primary aggregate structure that can be well characterized by TEM-measurements [83–85]. Both morphological characteristics of carbon black are compared to results of computer simulations and analytical models of disorderly growth processes under ballistic conditions [18, 84]. In Sect. 4, we will consider the structures involved in secondary aggregation and networking of carbon black in elastomers [22, 23] that has also been extended to elastomer blends [86, 87]. We will discuss the developed model in the framework of experimental results concerning filler flocculation and dielectric properties of carbon black reinforced rubbers. Based on the investigations of carbon black morphology and energetic surface structure we will then develop a model of rubber reinforcement by kinetically aggregated filler networks in Sect. 5. We will first consider the linear viscoelastic behavior by referring to the elasticity of the fractal CCA-unit cells of the filler network [22, 23, 48, 57, 85, 88]. Then, we will focus on a micro-mechanical concept of stress-induced filler cluster breakdown that combines the hyperelastic response of the hydrodynamically reinforced rubber matrix with the non-linear viscoelastic response of reversibly broken filler clusters [75, 76, 89]. It allows for an explanation of both, the Payne effect and the Mullins effect, by referring to a single micro-mechanical mechanism.

2 Experimental Methods 2.1 Materials and Sample Preparation

For the preparation of filler reinforced elastomer composites, most frequently commercial rubber grades with variable microstructure and broad molar mass distribution are applied. The typical rubber grades, considered in the present review, are as follows: 1. Natural rubber NR (SMR 5L; 99.9 vol.% cis) 2. Solution-styrene-butadiene rubber S-SBR (Buna VSL-2525–0; 25 vol.% vinyl, 25 vol.% styrene, Mw=206,600 g/mol, Mw/Mn=2.75) 3. Emulsion-styrene-butadiene rubber E-SBR (Intol 1524; 15 vol.% vinyl, 23.5 vol.% styrene, Mw=205,300 g/mol, Mw/Mn=2.12) 4. Ethylene-propylene-diene rubber EPDM (Keltan 512; 55 vol.% ethylene) 5. Nitrile-butadiene rubber NBR (Perbunan 3307; 33 vol.% acryl-nitrile)

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

9

In addition to the commercial rubber grades, model polymers with variable molar mass and narrow molecular weight distribution are often used for studying reinforcement mechanisms. (In Sect. 4.3 we consider a special S-SBR type with 29 vol.% vinyl and 25 vol.% styrene units; Mw/Mn=1.1). In general, furnace carbon blacks with different structure and specific surface area are employed as reinforcing fillers. Furthermore, commercial silica grades are applied, especially in the tire industry. In Sect. 5 we refer to a highly dispersive silica grade (Ultrasil 7000 GR) together with a bi-functional silane as coupling agent (Si 69).) The filler loading can range from very small amounts up to 100 phr. The notation “per hundred rubber” (phr), representing the mass (in grams) of an ingredient with respect to 100 g of rubber, is widely used in the rubber industry. The conversion to volume fraction F is obtained by the elementary formula F=phr/rCB (100 g/ rPol+phr/rCB)1, where phr is the mass of carbon black (in grams) per 100 g polymer, while rPol0.9 g/cm3 and rCB1.8 g/cm3 is the mass density of the pure polymer and carbon black, respectively. As polymeric model fillers with specific surface groups and narrow size distribution, different microgel types, e.g., poly(styrene)-microgel, PS(m), and poly(methoxy-styrene)-microgel, PMS(m), are applied. They can be prepared by emulsion polymerization techniques as described, e.g., in [48]. The rubber composites are in general processed in an interlocking mixer, as widely used in rubber industry, e.g., Werner & Pfleiderer GK 1.5 E with a mixing chamber of 1500 cm3. For obtaining a sufficient dispersion of the filler, at least 4 min mixing time are necessary. For the silica/silane systems, most frequently a two step mixing procedure is applied, for obtaining a reasonable coating reaction of the silane on the silica surface. Furthermore, a small amount of ZnO and stearinic acid is added to all compounds for supporting a fast filler dispersion and vulcanization. In general, the mixer is filled up to 75% of its capacity for the specimens with less than 40 phr filler, 70% for loading between 40 and 70 phr, and 60% for more than 70 phr filler. The cross-linking system is added on a roller mill in a separate mixing step (Here, 1.7 phr sulfur and 2.5 phr N-cyclohexylbenzothiazol-2-sulfenamide (CBS) is used). The composites with graphitized blacks are mixed on a roller mill for 20 min to ensure a sufficient dispersion. The composites are cured in a steam press, most frequently up to 90% of the rheometer optimum (T90 time) at 160 C. 2.2 Gas Adsorption Measurements

The morphological and energetic surface characterization of carbon black on atomic length scales can be performed by volumetric gas adsorption techniques. A schematic view of three different application regimes of this technique is shown in Fig. 4. According to this scheme, the surface roughness of particular fillers is estimated in the mono- and multi-layer regime. Furthermore, a characterization of the energy distribution of adsorption sites of carbon black and other colloids is obtained in the sub-layer regime.

10

Manfred Klppel

Fig. 4 Schematic representation of gas adsorption techniques in different layer regimes (decreasing pressure from top to bottom)

A classical volumetric adsorption apparatus equipped with absolute capacitance pressures transducers can be used for the estimation of adsorption isotherms in the pressure range 103 mbar

[nm] : mean perimeter

The macro-dispersion of the fillers can be determined by light-microscopic techniques with computer-assisted image processing on glazed cuttings of the vulcanized samples. At least five picture details have to be evaluated for each specimen. The dispersion coefficient D is calculated from the ratio of non-dispersed filler agglomerates and the volume fracture F of the filler in the composites in accordance with ASTM:D2663. For the characterization of micro-dispersion of fillers, i.e., in rubber primary aggregate morphology of carbon black, the uncured composites are immersed for a week in a good solvent, with the solvent being changed a number of times in order to remove the unbounded polymer. Afterwards the specimens are dispersed in a vibrator. The highly diluted suspensions are then dipped on a grid and carefully condensed. Micrographs are taken using the Electron-Spectroscopy-Imaging-Transmission-Electron-Microscopy (ESI-TEM) technique, e.g., on an EM 902 (Zeiß) equipment. For the evaluation of aggregate morphology (analogous to ASTM: 3849) roughly 500 particles of each carbon black type are measured with respect to cross-sec-

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

11

tional area A, perimeter P and diameter d. This preparation procedure is indicated by the terminology “in rubber state”. In a second preparation procedure, referred to as “dry state”, the carbon black is resolved in a solvent and dispersed by ultrasonic treatment. Afterwards, the highly diluted suspension is dipped on a grid and treated as above. Further morphological investigations by TEM are performed on ultra-thin cuts (~80 nm). By making use of energy filters (ESI), the inelastically scattered electrons can be removed. The micrographs provided by the elastically scattered electrons only show a good contrast based on the differences in carbon densities in the phases under consideration. 2.4 Mechanical Analysis

Dynamic-mechanical testing of cross-linked samples are often carried out with high precision on specimen strips in torsion mode, e.g., with a Rheometrics Dynamic Analyzer II (RDA) with a sample size of 28102 mm. Here, temperature-and strain sweeps are performed in a displacement range from 0.01% to about 5% strain and a frequency range between 0.1 and 100 Hz. Dynamic mechanical testing of uncross-linked samples can be made, e.g., with a Rubber Process Analyzer RPA 2000 (Alpha Technologies) from 0.28% to 350% strain at various frequencies and elevated temperatures. The quasistatic mechanical testing of the vulcanized samples is performed with a tensile tester. Uniaxial stress-strain measurements are carried out on (S2) strip-samples with cyclically increasing load (discontinuous damage mode) and up to rupture stress. Equi-biaxial stress-strain measurements are performed on a special frame with quadratic sample sheets of size 100100 mm and thickness 2 mm up to 110% strain maximum. During the tests, the stretching velocity is chosen to be small in order to avoid dynamic contributions to the moduli. In general, 10 mm/min is used, corresponding to a strain rate of @e/@t4103 s1. 2.5 Dielectric Measurements

For dielectrical investigations, samples are prepared as cross-linked sheets of a thickness between 1 and 2 mm. The dielectric measurements in a frequency range from 101 to 107 Hz are performed using a frequency response analysis system, e.g., the computer controlled Solartron SI 1260 Impedance/ Gain-Phase Analyzer and a Novocontrol broadband dielectric converter. The high frequency measurements in the range from 106 to 109 Hz can be performed in the wave reflection mode, e.g., with an Agilent 4291B RF Impedance Analyzer.

12

Manfred Klppel

3 The Disordered Structure of Carbon Black Reinforcement of elastomers by colloidal fillers, like carbon black or silica, plays an important role in the improvement of mechanical properties of high performance rubber materials. The reinforcing potential is mainly attributed to two effects: 1. The formation of a physically bonded flexible filler network 2. Strong polymer filler couplings

Both of these effects refer to a high surface activity and specific surface of the filler particles [26, 27, 47]. In view of a deeper understanding of such structure-property relationships of filled rubbers it is useful to consider the morphological and energetic surface structure of carbon black particles as well as the primary and secondary aggregate structure in rubber more closely. 3.1 Surface Roughness and Activity on Atomic Length Scales 3.1.1 Universality of Carbon Black Surface Roughness

For the characterization of surface roughness of carbon blacks, different experimental techniques have been applied in the past. Beside microscopic investigations, e.g., AFM that give an impressive but more qualitative picture [90–92], scattering techniques such as SANS [93] and SAXS [94–96] as well as gas adsorption techniques [79–84, 97–99] have been used for a fractal analysis of surface roughness. The results discussed in the literature appear somewhat controversy, since almost flat surfaces with ds2 [98, 99] and also rough surfaces with 2.2

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

13

Fig. 5a,b Schematic presentation of a mono-layer coverage of a fractal surface with: a small; b large gas molecules

Waals- and surface tension interaction, respectively. Dependent on the dominance of one of the two potentials, remarkably different estimates of surface roughness are obtained. For that reason a proper analysis of these factors is necessary for getting reliable results. In the present chapter we will summarize results of two different evaluation procedures for the surface roughness of carbon blacks. In the monolayer regime we refer to the scaling behavior of the estimated BET-surface area with the size of adsorbed probe molecules (yardstick method). On smooth flat surfaces the BET-area is independent of the adsorbed probe or applied yardstick, while on rough surfaces it decreases with increasing probe (yardstick) size due to the inability of the large molecules to explore smaller cavities. This is shown schematically in Fig. 5. In the case of carbon black a power law behavior of the BET-surface area with varying yardstick size is observed, indicating a self-similar structure of the carbon black surface. Double logarithmic “yardstick-plots” of the BETmono-layer amount Nm vs cross-section s of the probe molecules are shown in Fig. 6 for an original furnace black N220 and a graphitized (T=2500 C) sample N220g. It demonstrates that the roughness exponent or surface frac-

14

Manfred Klppel

Fig. 6 Yardstick-plot (Eq. 1) of N220 (triangle) and a graphitized N220g (filled circles) with adsorption cross section s determined from the bulk liquid density r (Eq. 2); 1 argon, 2 methane, 3 ethane, 4 propane, 5 iso-butane, 6 n-butane; The slopes yield for N220: ds=2.56€0.04, for N220g: ds=2.32€0.03. Adsorption temperatures and densities r are chosen according to the evaporation points of the gases at 1000 mbar

tal dimension ds differs for the two carbon black samples. By using the relation introduced by Mandelbrot [1, 2]: ds

Nm s 2

ð1Þ

one obtains from the slopes of the two regression lines of Fig. 6a surface fractal dimension ds2.56 for the N220-sample and ds2.32 for the graphitized N220g sample. An extrapolation of both regression lines yields an intersection at an ultimate cross-section that corresponds to a yardstick length of about 1 nm, indicating that graphitization reduces the roughness of carbon black on small length scales below 1 nm, only. Figure 6 clearly demonstrates that the reduction of BET-surface area during graphitization is length scale (yardstick) dependent, proving that it is related to a change of surface morphology and not, e.g., a result of reduced energetic surface activity (see below). An important point in the above evaluation of carbon black surface morphology is the correct estimation of the cross-section s of the applied probe molecules. This is done by referring to the mass density r of the probe molecules in the bulk liquid state that are considered as spheres in a hexagonal close packing: M 2=3 s ¼ 1:091 ð2Þ Na r

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

15

Fig. 7 Yardstick-plots (Eq. 1) of the graphitized black N220g obtained with a series of alkenes (ethylene, propylene, iso-butylene) (filled symbols) and alkanes (ethane, propane, iso-butane) (open symbols). Adsorption temperatures are chosen as evaporation points at vapor pressures p0103 mbar (lower curves) and p0104 mbar (upper curves) of the condensed gases, respectively

Here, M is the molar mass of the probe molecules and Na is the Avogadro number. The crucial point now is the temperature dependence of r that differs for the different probe molecules, mainly due to variations in the characteristic temperatures, e.g., the evaporation points. We found that Eq. (2) can be applied without further corrections and high correlation coefficients of the “yardstick-plots” in Fig. 6 and Fig. 7 are obtained only if the temperature during the adsorption experiments of a chemically similar, homological series of gases is chosen according to the same reference state, as defined in the framework of the theory of corresponding states. This is demonstrated in the “yardstick-plots” of Fig. 7, showing that for the same carbon black (N220g) a different scaling factor is obtained within one series of gases, if the adsorption temperatures are chosen with respect to different reference pressures, i.e., the evaporation temperatures at po=103 mbar and po=104 mbar, respectively. As shown in Fig. 7, a different scaling factor is also observed for the two different homological series of gases, i.e., the alkanes and alkenes, respectively. However, the scaling exponent and hence the surface fractal dimension ds2.3 is unaffected by the choice of the reference pressure or applied series of adsorption gases. An alternative approach to the characterization of surface morphology of carbon blacks is the consideration of film formation of adsorbed molecules in the multi-layer regime. In this case, the surface roughness is evaluated with respect to a fractal extension of the classical Frenkel-Halsey-Hill (FHH)-theory, where, beside the van der Waals surface potential, the vaporliquid surface tension has to be taken into account [100, 101]. Then the

16

Manfred Klppel

Helmholtz free energy of the adsorbed film is given as the sum of the van der Waals attraction potential of all molecules in the film with all atoms in the adsorbent, the vapor-liquid surface free energy and the free energy of all molecules in the bulk liquid. This leads to the following relation between the adsorbed amount N and the relative pressure p/p0 [100, 101]: po J N ln ð3Þ p with J¼

3 ds 3

J ¼ 3 ds

FHH regime

ð3aÞ

CC regime

ð3bÞ

The different exponents for the FHH- and capillary condensation (CC)-regime consider the two cases where adsorption is dominated by the van der Waals potential and the vapor-liquid surface tension, respectively. The two cases are shown schematically in Fig. 8b,c, respectively. Note that in the CCregime a flat vapor-liquid surface is obtained due to a minimization of curvature by the surface tension. In contrast, in the FHH-regime the vapor-liquid surface is curved, since it is located on equi-potential lines of the van der Waals potential with constant distance to the adsorbent surface. At low relative pressures p/p0 or thin adsorbate films, adsorption is expected to be dominated by the van der Waals attraction of the adsorbed molecules by the solid that falls off with the third power of the distance to the surface (FHH-regime, Eq. 3a). At higher relative pressures p/p0 or thick adsorbate films, the adsorbed amount N is expected to be determined by the surface tension g of the adsorbate vapor interface (CC-regime, Eq. 3b), because the corresponding surface potential falls off less rapidly with the first power of the distance to the surface, only. The cross-over length zcrit. between both regimes depends on the number density np of probe molecules in the liquid, the surface tension g, the van der Waals interaction parameter a as well as on the surface fractal dimension ds [100, 101]: rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a np ð4Þ zcrit ¼ ð ds 2 Þ g Note that the cross-over length zcrit. decreases with increasing surface fractal dimension ds, implying that the FHH-regime may not be observed on very rough surfaces, i.e., the film formation may be governed by the surface tension g on all length scales z>a (compare Fig. 10). The film thickness z is related to the surface relative coverage N/Nm and the mean thickness a0.35 nm of one layer of nitrogen molecules [102] according to the scaling law [1, 2]:

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

17

Fig. 8a–c Schematic view of the coverage of: a a smooth; b,c a fractal surface according to the fractal FHH-theory: (open circles) monolayer-regime, (gray circles) FHH-regime, (filled circles) CC-regime; z: average film thickness, a: monolayer thickness

z 3 d s N ¼ Nm a

ð5Þ

The monolayer amount Nm can be estimated from a classical BET-plot and hence the film thickness z can be obtained directly from the adsorbed amount N if the surface fractal dimension ds is known. So-called FHH-plots of the nitrogen adsorption isotherms at 77 K of various graphitized furnace blacks are shown in Fig. 9. The graphitized furnace blacks have two linear ranges. Starting from low pressures (right side), the first linear range is fitted by Eq. (3a), because the film is not very thick and the van der Waals attraction of the molecules by the solid governs the adsorption process (FHH-regime). With rising pressure, at a critical film thickness of about zcrit0.5 nm (Eq. 5), the vapor-liquid surface tension g becomes dominant and a step-like increase of the adsorbed amount is observed. The fractal FHH-theory claims fractal dimensions of ds2.3 up to a

18

Manfred Klppel

Fig. 9 FHH-plot of nitrogen adsorption isotherms at 77 K on various graphitized furnace blacks, as indicated. The dashed line characterizes the transition between the FHH- and the CC-regime. The ds-values, listed in the insert, refer to the FHH-regime at low pressures

length scale of z1 nm, independent of grade number. At this length scale a geometrical cut-off appears and the surface becomes rougher. In the final linear regime, corresponding to z>1 nm, the surface fractal dimension takes the value ds2.6 (CC-regime). This linear range has an upper cut off length of z6 nm. Figure 10 shows that contrary to the graphitized blacks the untreated furnace blacks have only one linear range with a fractal dimension of ds2.6 (CC-regime, Eq. 3b). Obviously the van der Waals attraction can be neglected and the surface tension g controls the adsorption process on all length scales. This is due to the larger surface fractal dimension ds as compared to the graphitized furnace blacks that shifts the cross-over length zcrit. to smaller values (Eq. 4). Assuming that the number density np, the surface tension g of the adsorbate and the van der Waals interaction parameter a are approximately the same for liquid nitrogen adsorbed on graphitized and untreated furnace blacks, a cross-over length of zcrit0.35 nm can be estimated from Eq. (4) with the experimental values of the fractal dimensions and the crossover length zcrit.0.5 nm on a graphitized carbon black. The value zcrit.0.35 nm is already in the range of the detection limit given by the layer thickness a0.35 nm. Hence, the nitrogen adsorption on furnace carbon blacks is dominated by the vapor-liquid surface tension on all length scales and a cross-over between the FHH- and the CC-regime does not appear. The results for the surface fractal dimension of a series of furnace blacks and graphitized blacks, obtained by nitrogen adsorption in the multilayer regime, are summarized in Fig. 11. The cut off lengths are quite similar

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

19

Fig. 10 FHH-plots of nitrogen adsorption isotherms at 77 K of various furnace blacks, as indicated. The surface fractal dimension appears to be universal, i.e., it varies between ds=2.55 and ds=2.59 for the depicted furnace blacks

within both series of blacks and agree with those found in Fig. 9 and Fig. 10. In Fig. 11 a weak trend of increasing surface fractal dimension with increasing specific surface (decreasing primary particle size) is observed. This results from increasing curvature of the particle surface with decreasing size, since crystallite structures with edges are present on the surface that lead to a more pronounced roughness, if arranged on a strongly curved surface. We will see in the next section that the amount of crystallite edges and slit shaped cavities increases slightly with increasing specific surface, leading to a more pronounced energetic surface activity for the fine carbon blacks. This relatively small effect correlates well with the weak trend of the surface fractal dimension observed in Fig. 11. The observed almost universal value of the surface fractal dimension ds2.6 of furnace blacks can be traced back to the conditions of disordered surface growth during carbon black processing. It compares very well to the results evaluated within the an-isotropic KPZ-model as well as numerical simulations of surface growth found for random deposition with surface relaxation. This is demonstrated in some detail in [18]. 3.1.2 Energy Distribution of Carbon Black Surfaces

The energy distribution f(Q) of carbon black surfaces is calculated by assuming that the measured overall isotherm consists of a sum of generalized Langmuir isotherms of various interaction energies Q, implying that the energy distribution can be identified with the numerically obtained weighting

20

Manfred Klppel

Fig. 11 Surface fractal dimensions ds on atomic length scales of furnace blacks and graphitized blacks in dependence of specific surface. The data are obtained from nitrogen adsorption isotherms in the multilayer regime

function [103, 104]. For a continuous distribution function f(Q) the overall isotherm Q(p,T) is given by Qðp; TÞ ¼

Z1

qðp; T; QÞ f ðQÞ dQ

ð6Þ

0

The integral in Eq. (6) is normalized to unity. This has to be taken into consideration if solid samples with different specific surface areas are compared. For an evaluation of the local model isotherm q(p,T,Q) with constant interaction energy Q, the effects of multi-layer adsorption and lateral interactions between neighboring adsorbed molecules are considered by applying two modifications to the Langmuir isotherm: (i) a multi-layer correction according to the well known BET-concept and (ii) a correction due to lateral interactions with neighboring gas molecules introduced by Fowler and Guggenheim (FG) [105]: qðp; T; QÞ ¼

b2BET bFG bL p 1 þ bBET bFG bL p

ð7Þ

with bBET ¼

1 1

p p0

zn c q

bFG ¼ e RT

Q Na s t 0 bL ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ eRT 2p MRT

ð8Þ

ð9Þ ð10Þ

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

21

Fig. 12 Adsorption isotherms (Q=N/Nm) and corresponding energy distribution functions of ethylene on N220 at various temperatures; ((1) T=177 K; (2),(3) T=223 K; (4) T=233 K)

Here, zn is the number of neighboring adsorption sites, c is the contribution of the lateral interaction to Q, and q is the probability that the neighboring sites are occupied by a gas molecule. R is the gas constant, T is temperature, t0 is Frenkels characteristic adsorption time, s is the adsorption crosssection of the gas molecules, Na is Avogadros constant, and M is molar mass. Note that the probability that the neighbor sites are occupied with other gas molecules is taken to be the local surface coverage q and not the overall surface coverage Q. This means that sites with the same interaction energies Q are assumed to be arranged in patches, which is in accordance with the picture of graphite like micro crystallites on the surface of the carbon black particles [26]. A probability Q stands for a random distribution of sites with Q. By referring to adsorption isotherms of ethylene down to very low surface coverings (103 to 1 mono-layers), the energy distribution function of adsorption sites on different furnace blacks was estimated with Eqs. (6) to (10) by applying a numerical iteration procedure. This is described in some detail in [20, 79]. For a test of the evaluation procedure, the resulting energy distribution functions obtained from four different isotherms (three different temperatures) of ethylene on N220 are compared in Fig. 12. It becomes obvious that the isotherms measured at different temperatures lead to the same result for the energy distribution function, approximately, confirming the applied procedure. An analysis of the energy distribution function of ethylene on N220 is shown in Fig. 13, where the distribution function is fitted to four different Gauss-functions. Obviously, the good fit indicates that four different types of adsorption sites can be distinguished on the N220 surface. We relate the low energetic peak (I) to the basaltic layers and peak (III) to the edges of carbon crystallites. Peak (II) is referred to amorphous carbon and peak (IV) results from a few highly energetic slit like cavities between carbon crystallites. This is shown schematically in Fig. 14.

22

Manfred Klppel

Fig. 13 Fitting of the energy distribution function of ethylene on N220, already shown in Fig. 12 (T=223 K), to four Gaussian-peaks (I–IV)

The attachment of peak (II) to the amorphous carbon is concluded from the observation that this peak does not appear in the case of the graphitized black N220g and graphitic powder. The corresponding isotherms and energy distribution functions are depicted in Fig. 15. A comparison to the above analyzed N220 and a strongly reinforcing channel gas black demonstrates the relatively large amount of highly energetic sites of these blacks (Fig. 15). A comparison of the adsorption isotherms and the resulting energy distribution functions of three different furnace blacks is shown in Fig. 16. Corresponding to the difference in level and shape of the isotherms the amount of highly energetic sites varies significantly. The black N115 has a large fraction of highly energetic sites, while the N550 shows a small fraction of highly en-

Fig. 14 Schematic view of the association between morphological arrangements of carbon crystallites and energetic characteristics of carbon black surfaces. Four different types of adsorption sites are distinguished that refer to the de-convolution shown in Fig. 13

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

23

Fig. 15 Adsorption isotherms and evaluated energy distribution functions of ethylene on four different colloidal fillers at T=223 K; (1) channel gas black; (2) graphitic powder; (3) N220; (4) graphitized N220g

ergetic sites. The results of the peak analysis for the examined blacks and the graphitic powder are quantified in Table 1. A more detailed representation of the energetic surface heterogeneity of carbon blacks is found in [20, 79]. Summarizing we can conclude from the analysis of the surface energy distribution of carbon blacks that four different energetic sites can be distinguished. The fraction of highly energetic sites decreases significantly with grade number and disappear almost completely during graphitization. It indicates that the reinforcing potential of carbon black is closely related to the amount of highly energetic sites that can be well quantified by the applied gas adsorption technique. Theoretical investigations on the effect of morphological as well as energetic surface roughness on the polymer-filler inter-

Fig. 16 Adsorption isotherms and evaluated energy distribution functions of ethylene on three different furnace blacks at T=223 K; (1) N115; (2) N220; (3) N550

24

Manfred Klppel

Table 1 Estimated fraction [%] of the four different types of energetic sites (I–IV) for adsorption of ethylene on various colloids

Channel-gas-black N115 N220 N550 Graphitic powder Graphitized N220g

I

II

III

IV

61 69 84 93 94 99

2 13 7 6 0 0

31 15 7 1 4 <1

6 3 2 <1 2 <1

action strength confirm this finding [64, 65, 106, 107]. The combination of two types of disorder, given by the pronounced morphological roughness (ds=2.6) and the inhomogeneous energetic surface structure of carbon blacks, enhances the polymer filler coupling, significantly. It represents an important reinforcing mechanism on atomic length scales associated with the required strong phase binding in high performance elastomer composites. 3.2 Morphology of Carbon Black Aggregates on Nanoscales

Carbon blacks for the rubber industry are produced in a variety of classes and types, depending on the required performance of the final product. In general they consist of a randomly ramified composition of primary particles that are bonded together by strong sinter bridges. Significant effects of the different grades of carbon blacks in elastomer composites result from variations in the specific surface and/or “structure” of the primary aggregates [26, 27]. The specific surface depends strongly on the size of the primary particles and differs from about 10 m2/g for the very coarse blacks up to almost 200 m2/g for the fine blacks. The “structure” of the primary aggregates describes the amount of void volume and is measured, e.g., by oil (DBP) absorption. It typically varies between 0.3 cm3/g and 1.7 cm3/g for furnace blacks. The characteristic shape of carbon black aggregates is illustrated in Fig. 17, where transmission electron micrographs (TEM) of three different grades of furnace blacks (N220, N330, N550) are shown. The variation in size of the primary particles, increasing from left to right, becomes apparent. It implies a decline of the specific surface from 116 m2/g for N220, 81 m2/g for N330, up to 41 m2/g for N550. The “structure” or amount of specific voids of the three grades is almost the same and differs between 1 cm3/g and 1.2 cm3/g, only. Since the specific weight of carbon black is almost twice that for DBP, this corresponds to a factor of 2 for the void volume as compared to the solid volume of the aggregates. It means that about 2/3 of the aggregate volume is empty space, i.e., the solid fraction Fp of the primary aggregates is relatively small (Fp0.33).

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

25

Fig. 17 Transmission electron micrographs (TEM) of three different grades of furnace blacks N220, N330, and N550 (dry state). (Bar length: 100 nm)

It is shown below that Fp fulfills a scaling relation which involves the size and mass fractal dimension of the primary aggregates. Due to significant deviations of the solid fraction Fp from 1, the filler volume fraction F of carbon black in rubber composites has to be treated as an effective one in most applications, i.e., Feff=F/Fp (compare [22]). 3.2.1 Fractal Analysis of Primary Carbon Black Aggregates

For a quantitative analysis of the structure of carbon blacks as shown in Fig. 17 it is useful to consider the solid volume Vp or the number of primary particles Np per aggregate in dependence of aggregate size d. In the case of fractal objects one expects the scaling behavior [1, 2] Vp N p d d f

ð11Þ

The exponent df is denoted mass fractal dimension or simply fractal dimension. It characterizes the mass distribution in three dimensional space and can vary between 1

8 A2 3P

ð12Þ

However, it is not quite clear whether this relation can be applied for non-Euclidean, ramified structures. Simulation results of carbon black formation under ballistic conditions by Meakin et al. [14] indicate that a scaling equation is fulfilled, approximately, between the number of particles Np in a primary aggregate and the relative cross section area A/Ap: Np ¼ 1:51 ð A = Ap Þ 1:08

ð13Þ

Here, Ap is the cross section area of a single primary particle. Dependent on the application of Eqs. (12) or (13), respectively, significantly different values for the mass fractal dimension are obtained.

26

Manfred Klppel

Fig. 18 TEM-micrograph of carbon black aggregates (N339) prepared from ready mixed S-SBR-composites with 60 phr filler (in-rubber state)

This discrepancy is demonstrated in Fig. 18 and Fig. 19 by considering an example of a fractal analysis of primary carbon black aggregates. Figure 18 shows a TEM-micrograph of the furnace black N339 prepared from a ready mixed composite of S-SBR after removing of the unbounded polymer as explained in Sect. 2.3 (in-rubber state). A double logarithmic plot of the solid volume Vp and the particle number Np, estimated from Eqs. (12) and (13), vs aggregate diameter d is shown in Fig. 19a,b, respectively. The aggregate average diameter d is estimated as the mean value from 16 measurements on a single aggregate with a 15% variation in the angle of rotation. The obtained fractal dimensions differ significantly for the two evaluation procedures.

Fig. 19 a Fractal analysis according to Eq. (11) of primary carbon black aggregates (N339) prepared from S-SBR-composites with 60 phr filler (in-rubber state). Vp is evaluated from Eq. (12). b Fractal analysis according to Eq. (11) of the same set of primary carbon black aggregates (N339) as shown in Fig. 19a. Np is evaluated by using Eq. (13)

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

27

From the slope of the two regression lines one finds df=2.45 and df=1.94, respectively. In view of a discussion of this discrepancy, we consider the conditions of primary aggregate growth during carbon black processing in some detail. Figure 20 shows a schematic representation of carbon black formation in a furnace reactor, where a jet of gas and oil is combusted and quenched, afterwards. Beside the aggregate growth, resulting from the collision of neighboring aggregates, surface growth due to the deposition of carbon nuclei on the aggregates takes place during the formation of primary carbon black aggregates. The surface growth leads to the universal surface roughness, analyzed by gas adsorption technique in Sect. 3.1.1 and investigated from a theoretical point of view in [18]. Obviously, the surface growth is also responsible for the strength of the primary aggregates, since it proceeds in the contact range of the collided aggregates implying a strong bonding by sinter bridges (Fig. 20). Due to the high temperature in the reactor, aggregate as well as surface growth take place under ballistic conditions, i.e., the mean free path length of both growth mechanisms is large compared to the characteristic size of the resulting structures [14–16]. Then the trajectories of colliding aggregates (or nuclei) can considered to be linear. Numerical simulations of ballistic cluster-cluster aggregation yield a mass fractal dimension df1.9–1.95 [11, 12, 17]. This compares to the above TEM-result df1.94 evaluated with Eq. (13). It means that the assumption of ballistic cluster-cluster aggregation during carbon black processing, used already in the derivation of Eq. (13), is confirmed by the TEM-data of the relatively fine black N339. For the more coarse blacks, with a typically small primary particle number, finite size effects can lead to a more compact morphology that differs from the scaling prediction of ballistic cluster aggregation. A further deviation can result from electrostatic repulsion effects due to the application of processing agents (alkali metal ions) for designing the coarse blacks (compare [22]). Note that a similar relation as Eq. (13) was derived in the 1960s by Medalia and Heckman [111, 112]. The value df=1.94 also agrees fairly well with other estimates obtained, e.g., by electric force microscopy [113], TEM [114], or SAXS [95, 96]. Therefore, it appears likely that the approach considering the solid volume of primary aggregates, as evaluated from the two-dimensional crosssection area by Eq. (12), leads to an overestimation of the mass fractal dimension. A more realistic estimate is obtained with Eq. (13). By referring to Eq. (12), the data obtained by Herd et al. [108] show a successively increasing value of the mass fractal dimension from df2.3 to df2.8 with increasing grade number (or particle size) of the furnace blacks. As expected, they fit quite well to the above estimate df2.45 for the black N339. A summary of these data and a discussion including other fractal parameters is found in [22].

Fig. 20 Schematic view of carbon black processing in a furnace reactor. Primary aggregates are built by two simultaneous growth processes: (i) surface growth (SG) and (ii) aggregate growth (AG)

28 Manfred Klppel

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

29

Fig. 21 Aggregate size distribution obtained from TEM-analysis (in-rubber state) of ESBR-samples filled with 50 phr N330 at various mixing times, as indicated [115]

3.2.2 Effect of Mixing on In-Rubber Morphology of Primary Aggregates

It is well established that the specific properties of carbon black filled elastomers, e.g., viscoelasticity or electrical conductivity, are strongly affected by the disordered, ramified structure of the primary aggregates [26, 27]. On the one hand, this structure is characterized by the mass fractal dimension considered above. On the other hand, it is determined by a lower and upper cut-off length, i.e., primary particle size and aggregate size, respectively. In the following we will focus on the upper cut-off length or, more precisely, on the size distribution of primary aggregates in ready mixed composites. We will see that this quantity depends on the conditions of sample preparation, since aggregate rupture can take place if high shear stresses are applied during the mixing procedure. In the literature it has been found that during mixing aggregate breakdown occurs for a number of carbon blacks in highly viscous rubbers [115– 118]. Recently, the aggregate breakdown was also attributed to classes of specific shapes of individual carbon blacks [108]. The opinion about the mechanical consequences of this process is quite different. On the one side, no obvious relationship to reinforcement is conjectured [116]. On the other side, improvements of the mechanical performance, due to the creation of new, active carbon surface, is assumed, which participates in formation of a strong filler-rubber coupling [118]. Figure 21 shows results obtained from TEM-analysis of primary aggregate size distribution of E-SBR/N330-samples at various mixing levels. With increasing mixing time, a shift in aggregate size distribution to smaller values is observed. The maximum of the distribution of aggregate cross section area shifts from about 0.03 m2 to about 0.02 m2. The shift of the maximum can be related to a breakdown of aggregates into smaller pieces as mixing time increases. It can also be referred to an improved micro-dispersion

30

Manfred Klppel

Fig. 22 Aggregate size distribution obtained from TEM-analysis (in-rubber state) of ESBR-samples filled with 40 and 80 phr N339, respectively, at fixed mixing time of 4 min

with specific influences on the mechanical property spectrum [85]. A characteristic effect of increasing mixing time on aggregate size is the reduction in the shoulder, occurring in the case of aggregate cross section areas greater than 0.05 m2, in favor of smaller aggregates. This is indicative for the rupture of single aggregates into two pieces. The observed aggregate breakdown during mixing can be understood on a more fundamental level, if the above discussed two simultaneous growth mechanisms, surface- and aggregate growth, during carbon black processing are considered again (Fig. 20). Obviously, the surface growth implies a strong bonding between adjacent primary particles by rigid sinter bridges that keep the primary aggregates together. However, this process goes on during the aggregate growth leading to a hierarchy of bonding strengths. The bonds formed in the beginning of aggregate growth become stronger than the final ones, because the time for stabilization by sinter bridges decreases with increasing time in the reaction zone. The bonds formed between collided aggregates just at the end of the reaction zone, before the quenching process takes place, remain relatively weak. This also becomes apparent in the upper scheme of Fig. 20. For that reason we expect that increasing mixing severity during compounding with highly viscous polymer melts leads to aggregate breakdown and changes in aggregate size distributions. According to Fig. 22, this is also observed for an increased filler loading. As shown in Fig. 22, the maximum of the size distribution is shifted to smaller values with rising filler concentration from 40 phr N339 to 80 phr N339 in E-SBR-composites. This results from the increased viscosity, since shear forces during mixing are enhanced with rising viscosity of the composite. A comparison of the morphology of N339 in E-SBR- and S-SBR-composites with increasing carbon black concentration is summarized in Table 2. It emphasizes the successive decrease of the mean primary aggregate size with increasing filler loading for both systems. The composites with E-SBR have a slightly larger aggregate size in the range of higher filler concentrations compared to those with S-SBR. On the one hand this can be assumed to result from a lower viscosity, especially under elongation deformations, which is of high relevance for filler dispersion during mixing. On the other,

31

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

Table 2 Characteristic parameters from TEM-analysis for primary aggregates of N339 in ESBR- and S-SBR-composites, respectively, at various filler concentrations and fixed mixing time (4 min) N339 [phr] E-SBR 20 40 60 80 S-SBR 20 40 60 80

[nm2]

21,600 14,570 12,090 12,170

777 600 534 516

1,750,230 1,009,400 838,779 780,592

22,900 15,820 12,580 8,060

857 639 539 399

1,711,680 1,113,475 839,255 482,050

it may also be related to a weaker polymer-filler coupling between the carbon black surface and the E-SBR-chains [119]. The observed effect of mixing on aggregate size distribution has a pronounced influence on the mechanical properties of the composites. This can be quantified by considering the solid fraction Fp of primary aggregates that represents a measure for the “structure” of carbon blacks. It is given by the ratio between the solid volume and the overall aggregate volume. Then, with Eq. (11) one finds the following scaling relation with respect to the average diameter d of the aggregates: Vp Fp ¼ p 3 d df 3 6d

ð14Þ

A fractal analysis according to Eq. (14) of carbon black aggregates (N339) in ready mixed E-SBR-composites is depicted in Fig. 23. The predicted scaling behavior of the aggregate solid fraction with diameter can be observed, though there is a larger scattering of the data as compared to those in Fig. 19. The slope of the solid regression line yields df2.33. Note that this differs significantly from the above estimate (Fig. 19a), which is mainly due to the different averaging procedures. An analysis of the solid fraction FP, calculated according to Eq. (14), indicates that for a constant aggregate diameter d there is a distribution of FP, as well as for a constant FP there is a scatter of the average diameter. The limiting value of the solid fraction Fp=1, corresponding to spherical particles, fits very well to the size of the primary particles of the carbon black N339 given by about 30 nm (dashed lines). As argued above, aggregates are efficiently diminished in size and partly broken due to the higher shear forces with increasing carbon black loading. This is emphasized in Fig. 24 by the increasing value of the mean solid frac-

32

Manfred Klppel

Fig. 23 Fractal analysis according to Eq. (14) of primary carbon black aggregates (N339) prepared from E-SBR-composites with 60 phr filler (in-rubber state). Vp is evaluated from Eq. (12)

tion

Fig. 24 Mean aggregate solid fraction vs filler volume fraction of N339 in E-SBR- and SSBR-composites, respectively, as obtained from TEM-analysis (in-rubber state)

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

33

packing before mixing, e.g., in the pelletized state. With increasing “structure” (decreasing solid fraction), the number of attractive contacts per unit volume decreases and the force, necessary to separate the aggregates in a pellet, is reduced. In comparison, for the coarse blacks the number density of contacts between neighboring aggregates in a pellet is relatively small and therefore also “low structure” grades are quite easily dispersed. Summarizing we conclude that the primary aggregate “structure” can be well analyzed by TEM-techniques. It is readily described by a fractal approach that refers to a cluster-cluster aggregation mechanism of primary particles during carbon black processing. During compounding of carbon blacks with highly viscous rubbers, rupture of primary aggregates takes place depending on the mixing severity. This leads to a reduced aggregate size and an increased solid fraction with increasing mixing time or filler loading, which has a significant influence on the mechanical properties of the composites. This will be considered in a micro-mechanical model of rubber reinforcement in Sect. 5.

4 Carbon Black Networking on Mesoscopic Length Scales 4.1 Microscopic and Scattering Analysis

A key factor for a deeper understanding of structure-property relationships of high performance elastomers is the morphological arrangement of filler particles on mesoscopic length scales due to secondary aggregation, also referred to as filler flocculation, cluster formation or networking. Even though the presence of such secondary network structures is often used in discussing filler specific mechanisms as the Payne effect, its morphology, as depicted in Fig. 25, is rarely studied on a quantitative level in comparison to that of the primary aggregates. In particular, the morphology of secondary filler networks is of high relevance for micro-mechanical models of rubber reinforcement, involving the original relaxed network structure as well as its stress-induced breakdown during deformations. Such models have been developed by assuming, e.g., a percolation structure for the filler network [56] with a characteristic mass fractal dimension df=2.5 [6, 7]. Investigations of carbon black network structure in polyethylene (HDPE) by electric force microscopy confirm this value, approximately, delivering df=2.6 on length scales between 0.8 and 2 mm [113]. However, recent studies of carbon black (N330) network structure in rubber (EPDM) by scanning electron microscopy found significantly smaller values for the mass fractal dimension in the intermediate length scale range between about 200 nm and 2 mm, increasing from df=1.9 to df=2.4 with increasing filler concentration [120]. The variation of the fractal dimension was referred to a spatial inter-penetration of spanning cluster arms in three-dimensional space that does not allow for a proper estimation

34

Manfred Klppel

Fig. 25 TEM-micrograph of a carbon black network obtained from an ultra-thin cut of a filled rubber sample

of df. The value df=1.9 for low filler concentrations was conjectured to lie close to the characteristic value df=1.8 expected for cluster-cluster aggregation (CCA) [6, 7]. The CCA-morphology has been considered by Witten et al. in modeling the quasi-static stress-strain behavior of filler reinforced rubbers [21]. Furthermore, based on the assumption of a CCA-filler network, the scaling behavior of the small strain elastic modulus with filler concentration could be well described [22, 23, 48, 85], though there is no unique experimental evidence for this particulate morphology (see below). So far, scattering techniques fail to provide reliable information on the connectivity of the filler network on larger length scales. This is again due to the spatial inter-penetration of the filler network in three-dimensional space, since labeling techniques, as considered, e.g., for polymer networks, cannot be applied. SAXS-studies on carbon black (N330) filled polyethylene have demonstrated that inter-penetration of primary aggregates in dense pellets causes the fractal domain to vanish due to a loss of correlation between primary particles [95]. A well defined scaling behavior of the scattering curves could only be obtained if a vanishing inter-penetration of neighboring aggregates was insured, i.e., spatially well separated aggregates, obtained from de-pelletized or fluffy black at sufficiently low filler concentrations, were realized. The same effect of inter-cluster correlation causes difficulties in obtaining information on the structure and connectivity of filler networks in elastomers, since inter-penetration cannot be avoided. This is also obvious in the TEM-micrograph shown in Fig. 25, where the three-dimensional, inter-penetrating connectivity of the carbon black network structure becomes apparent.

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

35

Fig. 26 D.c.-conductivity vs carbon black volume fraction of E-SBR samples filled with various furnace blacks. The solid lines are least square fits according to Eq. (15). Experimental data are taken from [124]

4.2 Investigations of Electrical Properties 4.2.1 Percolation Behavior of the d.c.-Conductivity

An important tool for analyzing the structure of carbon black networks in elastomers is provided by investigations of the electrical percolation behavior and the dielectric properties in a broad frequency range [22, 23, 121– 139]. This is evident from the fact that, in an isolating polymer matrix, the charge carriers follow the conducting paths given by the connectivity of the filler network. In particular, the electrical percolation threshold decreases with increasing specific surface and/or “structure” of carbon black primary aggregates and decreasing compatibility between polymer and filler [121– 125]. This emphasizes the role of mean aggregate distance or gap size between primary aggregates or clusters. It refers to a thermally activated hopping or tunneling of charge carriers across the gaps that governs the conductivity of carbon black filled polymers above the percolation threshold. The non-universal value of the percolation exponent of the d.c.-conductivity gives a further hint on the role of charge carrier tunneling in the conduction mechanism of filled polymer composites [126, 127]. The electrical percolation behavior for a series of carbon black filled rubbers is depicted in Fig. 26 and Fig. 27. The inserted solid lines are least square fits to the predicted critical behavior of percolation theory, where only the filled symbols are considered that are assumed to lie above the percolation threshold. According to percolation theory, the d.c.-conductivity sdc increases with the net concentration FFc of carbon black according to a power law [6,128]:

36

Manfred Klppel

Fig. 27 D.c.-conductivity vs carbon black volume fraction of various rubber samples filled with the furnace black N660. The solid lines are least square fits according to Eq. (15). Experimental data are taken from [124]

sdc ¼ so

F Fc m for F > Fc 1 Fc

ð15Þ

The critical concentration Fc denotes the percolation threshold, so is the limiting d.c.-conductivity for F=1 and the exponent m is called percolation exponent. As outlined in [23], percolation theory predicts a universal value m2 for all types of 3-D-lattices. However, the fitted lines in Fig. 26 and Fig. 27 yield a non-universal behavior of m, i.e., significantly larger values that depend on the carbon black grade and on the type of rubber. This is apparent from the data shown in Table 3, where the fitting parameters Fc, m, and s0 are listed together with the correlation coefficients r2 for all sample series. Obviously, there is a clear trend that the critical concentration Fc as well as the percolation exponent m increase with increasing grade number of carbon black and, apart from the very coarse blacks, the limiting conductivity so decreases. Furthermore, these parameters are found to be highly affected by the microstructure of the rubber matrix. This behavior can be understood if a superimposed kinetic aggregation process of primary carbon black aggregates in the rubber matrix is considered that alters the local structure of the percolation network. A corresponding model for the percolation behavior of carbon black filled rubbers that includes kinetic aggregation effects is developed in [22], where the filler concentrations F and Fc are replaced by effective concentrations. In a simplified approach, not considering dispersion effects, the effective filler concentration is given by: ( B ) F F Fþ Feff ¼ 1þb ð16Þ Fp Fp

37

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

Table 3 Fitting parameters of Eq. (15) for the data shown in Figs. 26 and 27 Sample series

N2SA [m2/g]

FP(CDBP)

Fc

m

so [S/cm]

r2

E-SBR/N110 E-SBR/N220 E-SBR/N299 E-SBR/N339 E-SBR/N358 E-SBR/N550 E-SBR/N650 E-SBR/N774 EPDM/N660 NR/N660 L-SBR(18)/N660 L-SBR(23)/N660 L-SBR(35)/N660 E-SBR/N660

138 116 106 95 85 41 38 29 36 36 36 36 36 36

0.36 0.36 0.35 0.35 0.34 0.41 0.40 0.45 0.43 0.43 0.43 0.43 0.43 0.43

0.091 0.090 0.105 0.110 0.109 0.162 0.162 0.185 0.129 0.143 0.159 0.178 0.191 0.193

3.7 3.4 3.2 2.7 3.4 4.0 7.1 10.6 6.3 7.8 6.2 4.6 5.2 5.5

3.9103 1.3102 4.2103 2.0104 4.8104 8.0104 0.36 17.2 122 1078 0.43 0.026 0.093 1.02

0.966 0.920 0.938 0.989 0.985 0.998 0.994 0.960 0.994 0.998 0.992 0.986 0.997 0.999

N2SA: Nitrogen surface area FP(CDBP): Primary aggregate solid fraction from CDBP-absorption with data from [26]

In Eq. (16), FP is the solid fraction of the primary aggregates, which takes into account that carbon blacks are “structured” (compare Sect. 3.2.). F+ is a critical concentration (aggregation limit), where secondary aggregation starts and b and B are characteristic growth exponents of secondary aggregation. These three parameters are governed by the mean primary aggregate distance and their mobility in the rubber matrix, i.e., they depend on the specific surface and “structure” of carbon black grade and on the type of rubber. In particular, it is shown in [22] that the cluster growth function Eq. (16) allows for a quantitative description of the dependence of the Young modulus on filler concentration in the case of spherical, mono-disperse model fillers (micro-gels). In [48] it is demonstrated that the ability of secondary aggregation of filler particles in highly viscous polymers is reduced with increasing polymer-filler interaction. The same effect is described in the literature for the case of surface modified as well as graphitized carbon blacks [61, 129, 130]. The consideration of kinetic aggregation of “structured” filler particles by an effective filler concentration Feff, as given by Eq. (16), instead of F and Fc in the percolation model Eq. (15), allows for a consistent interpretation of the observed variation of fitting parameters listed in Table 3. A first effect on Fc results from the “structure”, as described by FP, that generally tends to larger values for the coarse blacks with large grade number. Since TEMdata for FP, shown, e.g., in Fig. 23 and Fig. 24, are not available for all sample series, the values FP(CDBP)=(1+rCB CDBP/100)1 are inserted in Table 3. They are given by the amount of di-butylphthalate absorption per 100 g of carbon black after mechanical treatment (compressed DBP number (CDBP) according to ASTM D3493-90) and the mass density rCB=1.8 g/cm3 of car-

38

Manfred Klppel

bon black. Obviously, a single factor, e.g., the numerically estimated value of the percolation threshold in a simple cubic lattice, Fc,eff0.31 [6], gives no correlation between FP(CDBP) and the experimental values of Fc, indicating that the external bracket term of Eq. (16) differs from one. It means that the power law term, considering kinetic aggregation, must be significant. Accordingly, the percolation threshold Fc increases with increasing grade number mainly due to the restriction of mobility with decreasing specific surface of the primary aggregates. The impact of rubber type on Fc (Fig. 27) can also be related to the variation of particle mobility, since a strong polymer-filler coupling in a more compatible polymer matrix reduces the particle mobility. Accordingly, beside the effect of “structure” considered by FP(CDBP), the enhanced polymer-filler interaction in the series from EPDM via NR to the SBRs [124] as well as the decreasing specific surface area (N2SA) with rising carbon black grade number lead to an increase of the percolation threshold Fc, since both effects hinder the kinetic aggregation process. A reduced aggregation corresponds to higher values of the growth exponent B in Eq. (16), which can be related to the increase of the percolation exponent m with increasing grade number, observed in Table 3. This is realized on a qualitative level, when the percolation Eq. (15) is rewritten with effective volume fractions as given by Eq. (16). Then, if for sufficient large filler concentrations the one in the first bracket term of Eq. (16) is neglected and if furthermore F+ is approximated by Fc, one obtains an approximative scaling equation for the conductivity with respect to the net concentration FFc with an effective exponent m(B+1) that can be significantly larger than m. This explains the non-universal value of the conductivity exponent that increases with the cluster growth exponent B. Consequently, the consideration of a superimposed kinetic aggregation in the framework of percolation theory allows for a qualitative understanding of the variation of Fc and m for the different sample series. We finally note that for a proper quantitative description of the percolation behavior of carbon black composites it is also necessary to consider the effect of primary aggregate breakdown more closely, i.e., the dependence of FP on filler concentration and mixing conditions entering Eq. (16) (compare Sect. 3.2.2). This is beyond the scope of the present chapter. A quantitative description of percolation including a full characterization of in-rubber morphology of primary carbon black aggregates will be a task of future work. 4.2.2 Dielectric Analysis of Carbon Black Networks

The dielectric properties of carbon black filled rubbers are closely related to the morphological structure of filler networks, providing an important analysis tool on mesoscopic length scales. On the one hand, the tunneling or hopping of charge carriers over conductive gaps provide information on the specific morphology of filler-filler bonds on nanoscopic length scales [121, 122, 131–134]. On the other hand, the scaling behavior of the conductivity

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

39

Fig. 28 A.c.-conductivity s0 vs frequency and temperature of a NR-sample filled with 80 phr carbon black (N339)

in the high frequency regime is indicative for anomalous diffusion of charge carriers on fractal carbon black clusters on mesoscopic length scales [23, 134–139]. In the following, both of these effects will be analyzed by referring to exemplary results. Fig. 28 shows the real part of the a.c.-conductivity s0 of a highly filled NR/N339 sample in the frequency- and temperature range 101 to 107 Hz and 100 to 150 C, respectively. At low frequencies, below around 105 Hz, the conductivity is almost independent of frequency but shows a pronounced temperature dependence. At high frequencies, a relaxation transition is observed leading to a step-like increase of the conductivity. In the low frequency regime, the conductivity first decreases slightly with increasing temperature, when the glass transition temperature, Tg-60 C, is exceeded. This can be related to an enhanced thermal expansion of the rubber above Tg. It increases the size of conducting gaps between adjacent, highly conducting carbon black aggregates somewhat, implying that the gap size is the dominating factor for the conductivity. Since no thermal activation of the conductivity is observed at low temperatures, the conduction mechanism can be concluded to be due to tunneling across gaps. Consequently, the gap size is of the order of 1 nm, i.e., the typical tunnel distance of quantum particles [121, 122]. It can be related to the presence of a thin polymer film in the contact area between flocculated primary carbon black aggregates.

40

Manfred Klppel

Fig. 29 A.c.-conductivity s0 vs frequency at 20 C of NBR-samples filled with various amounts of N220, as indicated. The solid lines correspond to the scaling behavior Eq. (17), obtained in the high frequency range up to 1 GHz

With rising temperature, above around 0 C, the conductivity shown in Fig. 28 increases significantly. A closer analysis indicates a characteristic Arrhenius behavior in the temperature regime between 20 and 60 C. Recently, such behavior has also been observed for other carbon black filled elastomers [133]. Obviously, the conduction mechanism in this temperature regime changes, implying a thermally activated hopping of charge carriers across the gaps between adjacent carbon black aggregates [121, 122]. For temperatures larger than about 60 C the conductivity levels out. This can be related to the impact of an increasing gap size on the conductivity, i.e., the strong exponential decrease of the conductivity with increasing gap size due to a more pronounced thermal expansion. Investigations of highly filled composites with various rubbers show that a qualitative similar behavior of the temperature dependence of the conductivity as in Fig. 28 is realized, but the temperature where the conductivity levels out seems to be roughly correlated with the glass transition temperature of the polymer. In particular, for BR-composites with a relatively low glass transition temperature, the conductivity levels out around room temperature and shows a pronounced drop by orders of magnitude at higher temperatures. For these systems a conductor-isolator transition is observed at about 130 C, which must be related to a strong increase of the gaps beyond a distance where hopping or tunneling of charge carriers can take place. For a deeper understanding of structure-property relationships it is useful to consider the effect of carbon black grade and concentration as well as polymer type on the dielectric properties more closely. In Fig. 29 the real part of the a.c.-conductivity s0 at 20 C of a series of rubber composites, consisting of the more polar statistical co-polymer NBR and the fine black N220, is depicted for various filler concentrations in the high frequency regime up to 1 GHz. For the lower carbon black concentrations, a power law behavior with exponent around 0.6 is observed, while the highly filled com-

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

41

Fig. 30 a Conductivity s0 vs frequency at 20 C of S-SBR-samples filled with various amounts of N550, as indicated. b Permittivity e0 vs frequency at 20 C of the same SSBR-samples

posite exhibits a cross-over from a plateau value to a power law behavior. Obviously, the characteristic cross-over frequency increases with rising filler concentration. This behavior becomes more transparent in Fig. 30a,b, where the a.c.-conductivity s0 and relative dielectric constant (permittivity e0 ), respectively, for a series of less polar S-SBR-samples filled with various amounts of the coarse black N550 are show at 20 C in a broader frequency range up to 107 Hz. For filler concentrations below the percolation threshold (F0.15), the conductivity behaves essentially as that of an isolator and increases almost linearly with frequency. Above the percolation threshold (F0.2), it shows a characteristic conductivity plateau in the small frequency regime. Since at low frequencies the value of the conductivity s0 agrees fairly well with the d.c.-conductivity, the plateau value exhibits the characteristic percolation behavior considered above. In the high frequency regime the conductivity depicted in

42

Manfred Klppel

Fig. 30a behaves similarly to that of the NBR/N220-samples shown in Fig. 29, i.e., above a critical frequency wx it increases according to a power law with an exponent n significantly smaller than one. In particular, just below the percolation threshold for F=0.15 the slope of the regression line in Fig. 30a equals 0.98, while above the percolation threshold for F=0.2 it yields n=0.65. This transition of the scaling behavior of the a.c.-conductivity at the percolation threshold results from the formation of a conducting carbon black network with a self-similar structure on mesoscopic length scales. The reduced value of the scaling exponent, observed in Fig. 29 and Fig. 30a for filler concentrations above the percolation threshold, can be related to anomalous diffusion of charge carriers on fractal carbon black clusters. It appears above a characteristic frequency wx, when the charge carriers move on parts of the fractal clusters during one period of time. Accordingly, the characteristic frequency wx for the cross-over of the conductivity from the plateau to the power law regime scales with the correlation length x of the filler network. For a quantitative analysis of the scaling and cross-over behavior of the a.c.-conductivity above the percolation threshold we refer to the predictions of percolation theory [128, 136, 137]: s0 ðwÞ w n

for

w>wx

ð17Þ

and

dw x F Fc m wx ðFÞ ﬃ wx;o ﬃ wx;o do 1 Fc

ð18Þ

For the evaluation of the front factor the Einstein equation for the conductivity so can be used. It yields wx;o ¼ t1 x;o ¼

6 so kB T e2 no do2

ð19Þ

Here, e is the electron electric charge, no is the charge carrier density, and do is the size of the lattice units, i.e., the primary aggregates. The two critical exponents n=(dw-df+1)/dw0.6 and m=ndw3.3 are given by the characteristic structure parameters of percolation in three dimensions, i.e., the fractal dimension df2.5, the anomalous diffusion exponent dw3.8, and the correlation length exponent n0.87 [128, 137]. The experimental value n=0.65 found in Fig. 30a is in fair agreement with this prediction, indicating that for sufficient high carbon black concentrations a percolation structure of the filler network is realized in the systems. However, the experimental value n=0.65 lies also not far away from the predicted value n0.74 for a kinetically aggregated CCA-network structure, obtained with a fractal dimension df1.8 and an anomalous diffusion exponent dw3.1. A more detailed discussion of the scaling behavior of the conductivity in the framework of the two models, percolation and kinetic aggregation, is presented in [23]. The permittivity shown in Fig. 30b characterizes the polarization of the samples in an alternating field. At low carbon black concentrations, the per-

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

43

mittivity is relatively small (e0 ﬃ10) and almost independent of frequency. At higher carbon black concentrations, above the percolation threshold (F0.2), relatively high values of the permittivity (e0 ﬃ103) are found in the low frequency regime, but with increasing frequency a relaxation transition takes place and the permittivity e0 falls off drastically. The location of the relaxation transition on the frequency scale, wR, is shifted to higher frequencies with rising carbon black concentration. Note that the corresponding relaxation current leads to the step-like increase of the conductivity in the high frequency regime, observed for the system NR/N339 in Fig. 28. For the present sample series S-SBR/N550, shown in Fig. 30a,b, this relaxation current is not significant on the chosen logarithmic scale. Obviously, it is hidden by the relatively high conduction plateau. In this sense, conductivity and permittivity are decoupled, allowing for a proper analysis of the anomalous diffusion- and polarization transitions, separately. An explanation of the observed relaxation transition of the permittivity in carbon black filled composites above the percolation threshold is again provided by percolation theory. Two different polarization mechanisms can be considered: (i) polarization of the filler clusters that are assumed to be located in a non polar medium, and (ii) polarization of the polymer matrix between conducting filler clusters. Both concepts predict a critical behavior of the characteristic frequency wR similar to Eq. (18). In case (i) it holds that wRﬃwx, since both transitions are related to the diffusion behavior of the charge carriers on fractal clusters and are controlled by the correlation length x of the clusters. Hence, wR corresponds to the anomalous diffusion transition, i.e., the cross-over frequency of the conductivity as observed in Fig. 30a. In case (ii), also referred to as random resistor-capacitor model, the polarization transition is affected by the polarization behavior of the polymer matrix and it holds that [128, 136, 137] 1 F Fc q wR ðFÞ ﬃ ð20Þ Ro Co 1 Fc Here, Ro is the resistance of the occupied lattice units and Co is the capacitance of the non-occupied lattice units. In a first attempt, not considering anomalous diffusion effects, the exponent has been evaluated as q=m+s2.7, where s0.7 and m2.0 are the conductivity exponents (in three dimensions) below and above the percolation threshold, respectively. However, by including anomalous diffusion effects one obtains q=m=ndw3.3 [136, 137]. For a quantitative analysis of the percolation behavior of wR, considered in Eq. (20), the permittivity data shown in Fig. 30b have been fitted to an empirical Cole-Cole function [131, 132]. The fits are quite good, yielding relatively small broadness parameters between 0.36 and 0.5. The obtained relaxation times tR=wR1 are depicted in Fig. 31 in dependence of filler concentration F. Furthermore, the cross-over times tx=wx1 and the limiting low frequency plateau values of the conductivity s0 (w!0), obtained from the data in Fig. 30a, are represented in Fig. 31. They have been evaluated by a simple shifting procedure for constructing a conductivity master curve, as

44

Manfred Klppel

Fig. 31 Characteristic parameters of the S-SBR/N550 composites, s0 (w!0), tx, and tR, for various carbon black concentrations F obtained from Fig. 30a, b. The solid lines are adapted to Eqs. (15), (18), and (20), respectively

applied, e.g., in [135]. The solid lines depicted in Fig. 31 are fitted curves for the characteristic composite parameters s0 (w!0)=sdc, tx, and tR according to Eqs. (15), (18) and (20), respectively. Thereby, a common exponent q=m=10.1 and a single value of the percolation threshold Fc=0.165 have been assumed, providing best fits to the experimental data with correlation coefficients r2 between 0.978 and 0.996. The conductivity exponent corresponding to Eq. (15) is found as m=7.4 and the limiting conductivity for F=1 yields so=12.4 S/cm. For the two front factors of Eqs. (18) and (20) one obtains tx,o=1.41014 s and tR,o=6.31013 s. If the estimated fitting parameters are compared to the predicted values of percolation theory, one finds that all three exponents are much larger than expected. The value of the conductivity exponent m=7.4 is in line with the data obtained in Sect. 3.3.2, confirming the non-universal percolation behavior of the conductivity of carbon black filled rubber composites. However, the values of the critical exponents q=m=10.1 also seem to be influenced by the same mechanism, i.e., the superimposed kinetic aggregation process considered above (Eq. 16). This is not surprising, since both characteristic time scales of the system depend on the diffusion of the charge carriers characterized by the conductivity. The front factors obtained from the fittings in Fig. 31 can be used for a dielectric characterization of the network units, e.g., for an evaluation of the charge carrier density no of the primary carbon black aggregates as given by Eq. (19). Therefore, the electric charge e2=2.31028 Jm and the conductivity so=1.11013 s1 have to be inserted with respect to Gaussian units. The mean diameter of primary aggregates in S-SBR composites (50 phr N550) has been obtained from TEM analysis as do=157 nm. With T=293 K and kB=1.381023 J/K this yields for the reduced charge carrier density no

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

45

do3=2.6, i.e., the number of charge carriers per primary aggregate is of order one. This relative small number of charge carriers can be related to the tunneling or hopping conductivity mechanism between conducting nanoscopic islands (primary aggregates) with a high Coulomb exclusion energy. The exclusion energy for a single electron can be roughly estimated from the limiting relaxation time tR,o=RoCo, if the resistance Ro of the lattice units is expressed by the conductivity so via Roﬃ(sodo)1=5.1103 W. This yields for the capacitance of the lattice units Co=1.21016 F, or in Gaussian units Co=1.1106 m. Hence, the exclusion energy of a single electron results as EC=e2/2Co=1022 J. This value is more than one order of magnitude smaller than the thermal energy kBT=41021 J, which has to be exceeded for insuring the dominance of the Coulomb exclusion energy. Accordingly, from this estimates it appears that the charge carrier density is not limited by the exclusion energy but governed by thermal fluctuations. However, note that this calculation is not very precise, since the local geometrical structure of the lattice units is not considered properly. A more fundamental study of charge transport mechanisms in carbon black filled rubbers should take into account that the lattice units are fractal objects (primary carbon black aggregates), which are separated by small gaps not larger than a few nanometers. 4.3 Flocculation Dynamics and the Nature of Filler-Filler Bonds

For a deeper understanding of filler networking in elastomers it is useful to monitor structural relaxation phenomena during heat treatment (annealing) of the uncross-linked composites. This can be achieved by investigations of the time development of the small strain storage modulus G0 0 that provides information about the flocculation dynamics [140–143]. Figure 32a shows the time development of G0 0 of S-SBR melts of variable molar mass filled with 50 phr carbon black (N234), when a step-like increase of the temperature from room temperature to 160 C is applied. Figure 32b shows a strain sweep of the same systems after 60 min annealing time. Dependent on the molar mass Mw, as indicated, a pronounced increase of G0 0 is observed in the first minutes that levels out more or less to a plateau value at larger annealing times. In agreement with recent studies of Wang et al. [143], the largest plateau value is observed for the lowest molar mass, indicating that the increase of the modulus results from flocculation of primary aggregates to form secondary aggregates (clusters) and finally a filler network. It appears that a weakly bonded superstructure develops in the systems during heat treatment that stiffens the polymer matrix. With increasing dynamic strain amplitude, as depicted in Fig. 32b, a stress-induced breakdown of the filler clusters takes place and the storage modulus decreases by about one order of magnitude (Payne effect). With respect to the variable molar mass of the systems, Fig. 32b shows a cross-over of the moduli with increasing strain, indicating that a larger molar mass stabilizes the filler-filler bonds more effectively. This can be related to the overlapping action of tightly bound polymer chains in the contact area between adjacent filler particles.

46

Manfred Klppel

Fig. 32 a Time development of the small strain storage modulus of uncross-linked SSBR composites with 50 phr N234 during heat treatment at 160 C for various molar masses, as indicated (0.28% strain, 1 Hz). b Strain dependency of the storage modulus of the samples depicted in a after heat treatment for 60 min at 160 C

Inspired by the above flocculation analysis and the dielectric investigations described before, a model concerning the structure-property relationships of filler-filler bonds in a bulk rubber matrix can be developed as illustrated in Fig. 33. According to this model, the stiffness of filler-filler bonds is governed by the remaining gap size between contacting particles. This, in turn, depends on the ability to squeeze out the bound polymer chains from the contact area under the attractive action of the van der Waals force between the filler particles. This process leads to a stiffening of filler-filler bonds. It is favored by several factors, e.g., a high ambient temperature, low molar mass, small particle size, weak polymer-filler- and strong filler-filler interaction. The mechanical connectivity between the filler particles is provided by a flexible, nanoscopic bridge of glassy-like polymer, resulting from the immobilization of the rubber chains in the confining geometry close to the gap.

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

47

Fig. 33 Schematic view considering the structure of filler-filler bonds in a bulk rubber matrix. The impact of gap size on the stiffness of filler-filler bonds becomes apparent

Since the stiffness of the bonds transfers to the stiffness of the whole filler network, the small strain elastic modulus of highly filled composites is expected to reflect the specific properties of the filler-filler bonds. In particular, the small strain modulus increases with decreasing gap size during heat treatment as observed in Fig. 32a. Furthermore, it exhibits the same temperature dependence as that of the bonds, i.e., the characteristic Arrhenius behavior typical for glassy polymers. Note however that the stiffness of the filler network is also strongly affected by its global structure on mesoscopic length scales. This will be considered in more detail in the next section. In the case of carbon black filled diene-rubber composites the polymerfiller interaction is generally quite strong due to the high affinity between the p-electrons at the carbon surface and those in the double bonds of the chains. According to the site energy distribution function estimated in Sect. 3.1.2, the typical interaction energy between carbon black and ethylene, representing a single double bond, lies between 10 and 35 kJ/mol and depends on the grade number. A more practical procedure for characterizing the polymer-filler interaction in elastomer composites is the estimation of bound rubber, i.e., the amount of polymer tightly bound to the filler surface after mixing [144]. It is well known that this amount increases with the molar mass of the polymer and the specific surface area of the filler particles, but is also affected significantly by the surface activity, given, e.g., by the site energy distribution function of the filler obtained with polymer analogous gases [144–147]. A further effect comes in from the preparation conditions of the composites, e.g., mixing time [148], since the formation of bound rubber is a slow dynamical process that requires time. Figure 34 shows the result of bound rubber estimates at room temperature for variously mixed S-SBR composites filled with 50 phr of four different carbon blacks. The furnace blacks were mixed for 3 and 6 min in an in-

48

Manfred Klppel

Fig. 34 Results of bound rubber estimates at room temperature for various carbon black filled S-SBR composites, as indicated

ternal mixer, respectively, while the graphitized black N220g was mixed for 20 min on a roller mill. The dispersion rating was found to be larger than 90% for all systems. It becomes obvious that the amount of bound rubber increases with increasing mixing time from 3 to 6 min. This results from an exchange of shorter chains, already bound to the filler surface, by longer chains during the ongoing mixing process. The longer chains are bound more tightly to the surface due to a higher number of adhesive contact spots per chain [144–146]. Beside the effect of mixing time the estimated bound rubber reflects the difference in specific surface of the furnace blacks that increases from N550 (41 m2/g) via N220 (116 m2/g) to N115 (143 m2/g). A deviation from this correlation is observed for the graphitized black N220g that shows a significantly smaller amount of bound rubber as compared to its relatively large specific surface (88 m2/g). This effect can be attributed to the lower surface activity of the graphitized black that results from the marked reduction of highly energetic sites during graphitization (compare Fig. 15 and Table 1). From this observation it appears that the highly energetic sites are the dominating factor for strong polymer-filler couplings. The different interaction strength between polymer and filler leads to characteristic implications for the structural relaxation behavior (flocculation) of filler particles in highly entangled polymer melts. Figure 35 shows the strain dependency of the storage modulus G0 for the two composites SSBR/N220g and S-SBR/N220 (mixing time 6 min) before and after heat treatment (annealing) of the samples for 20 min at 160 C. Obviously, a significant increase of the small strain modulus of both systems results during heat treatment, referring to the flocculation of filler particles. With increasing strain the moduli decrease significantly due to a stress-induced successive breakdown of filler clusters. A comparison of the two systems filled with the furnace black N220 and the graphitized black N220g shows a stronger increase of the moduli for the system with the graphitized black, indicating a

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

49

Fig. 35 Strain dependency of the storage modulus (G0 at 60 C) of uncross-linked S-SBR composites filled with 50 phr N220 and N220g, respectively, before and after heat treatment for 20 min at 160 C

more pronounced flocculation during heat treatment. According to the model of filler-filler bonds considered in Fig. 33, the lower amount of tightly bound polymer around the graphitized black N220g supports the flocculation. It implies smaller contact gaps, because the polymer between the contacting particles can be squeezed out more readily by the attractive van der Waals forces. This leads to stiffer filler-filler bonds and hence to a higher modulus of the filler network. From principal reasons it is also possible that the global structure of the filler network of the two systems prepared with the furnace and graphitized black after heat treatment is generally different, e.g., the arrangement of the graphitized carbon particles is more compact. However, we will argue below that the formation of the filler network is governed by a diffusion controlled cluster-cluster aggregation (CCA)-process that leads to a universal CCA-network structure. Under this condition the difference in stiffness of the two systems has to be related to a change of the local stiffness of the filler-filler bonds. The impact of bound rubber on the spacing of filler-filler contact gaps during annealing of carbon black composites at elevated temperature is affected by the amount of bound rubber estimated at this particular temperature. However, the values listed in Fig. 34, obtained at room temperature, may not be representative, because the amount of bound rubber depends on the extraction temperature. In general, the amount of bound rubber is also affected by the solvent used for extraction and decreases with increasing extraction temperature [150–153]. In earlier studies a linear decrease in bound rubber with temperature was observed, extrapolating to zero at 375 C [150]. Other authors found a much more dramatic decrease with minimum bound rubber at about 100 C [151]. Subsequent studies of Chapman et al. [152], comparing extraction in vacuum, nitrogen, and air, respectively, found a moderate decrease of bound rubber of about 30% at 100 C in vacu-

50

Manfred Klppel

um as compared to room temperature and a much more pronounced decrease in air and also in nitrogen atmosphere. They concluded that oxidative chain scission reduces the bound rubber content at elevated temperature if determined in air and also in nitrogen. Similar results were obtained by Kida et al. [153]. They concluded from NMR-relaxation measurements that only the content of the outer, most mobile rubber phase is reduced while the highly immobilized phase close to the carbon black surface remains almost constant up to 113 C. From these results we can expect that for an annealing temperature of about 160 C, which is also applied during vulcanization, bound rubber is still present at the carbon black surface and hinders the aggregation of neighboring particles. Note that this is also expected from simple energetic arguments, since the above estimated adsorption energy of ethylene on N220, Q10–35 kJ/mol, is almost one order of magnitude larger that the thermal energy RT=3.6 kJ/mol at 160 C. The effect of bound rubber on the stiffness of filler-filler bonds is essential for the small strain modulus G0 0. It allows for a qualitative explanation of various well known phenomena described, e.g., in the pioneering papers of Payne [28–35]. In particular, the observed decrease of G0 0 with increasing mixing time [33, 148] can be related to a softening of the bonds due to a successive increase of bound rubber. Furthermore, the variation of G0 0 with polymer type [30, 154] can be related to the impact of bound rubber on the spacing of filler-filler bonds, implying that a strong polymer-filler coupling or high molar mass lowers the value of G0 0. Note that this interpretation can also explain the more or less significant correlation between the small strain modulus and the electrical conductivity level obtained, e.g., in [154]. This kind of correlation is also found, if composites with graphitized and nongraphitized carbon blacks of the same grade number are compared. The higher stiffness of composites with graphitized blacks is typically accompanied by a higher conductivity level [121]. Both effects refer to a smaller gap size between contacting primary aggregates in the case of graphitized blacks. Beside the stiffness of filler-filler bonds, the amount of bound rubber impacts also the strength of the bonds between interacting filler particles. Due to the overlapping action of the tightly bound polymer chains close to the contact area of neighboring filler particles, the mechanical stability of fillerfiller bonds increases with increasing amount of bound rubber. This explains the cross-over behavior of the moduli (after heat treatment) as observed in Fig. 32b and Fig. 35: The systems with the lower amount of bound rubber, i.e., the composites with graphitized blacks and the low molar mass of the polymer, respectively, show the largest values of the small strain modulus G0 0, but the drop of the moduli with increasing strain appears at significantly smaller strain amplitudes. The stabilizing bound rubber layer can be considered to act like a spanning net around the filler clusters, implying a high flexibility of the filler network. We will see that this kind of reinforcing action is responsible for the pronounced hysteresis and high strength of reinforced rubbers in the dynamic strain regime up to around 100%. Further

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

51

significant effects of the bound rubber layer result in the quasi-static high strain regime. This will be considered in the next section. In conclusion, the investigations of electrical properties of carbon black filled rubbers, presented in Sect. 4.2, indicate that a percolation structure for the filler network is realized on mesoscopic length scales, if a critical filler concentration is exceeded. This structure seems to be modified by a superimposed kinetic aggregation process that refers to the non-universal value of the percolation exponent and the impact of specific surface on the percolation threshold. Further experimental evidence for a kinetic aggregation mechanism of colloidal particles dispersed in a rubber matrix is given by the mechanical response of the uncross-linked composites during heat treatment (annealing), demonstrating that a relative movement (flocculation) of the particles takes place that depends on particle size, molar mass of the polymer as well as polymer-filler and filler-filler interaction. It has been argued that the mechanical stiffness of filler-filler bonds is governed by the remaining gap size between adjacent filler particles that develops during annealing (and cross-linking) of filled rubbers. Based on the model of filler-filler bonds depicted in Fig. 33, a qualitative explanation of the observed flocculation effects is possible by referring to the amount of bound rubber and its impact on the stiffness and strength of filler-filler bonds.

5 Rubber Reinforcement by Fractal Filler Networks In the last decades, remarkable progress has been obtained in understanding filler networking and its implications on the mechanical response of dynamically excited and highly strained rubber composites. This is summarized in a recent review of Heinrich and Klppel [57]. According to this paper, two fundamental micro-mechanical concepts of non-linear viscoelasticity, which are based on fractal approaches of filler networking, have been developed: the (L-N-B)-model [56] and the cluster-cluster-aggregation (CCA)-model [21–23, 85]. They consider the arrangement of filler particles in clusters with well defined fractal structure and the elasticity or fracture of such clusters under external strain. The two models refer to different geometrical arrangements of filler particles in particulate fractal network structures, described by percolation theory or kinetic cluster-cluster aggregation, respectively. We will focus here on the CCA-model of filler networking, since the investigations of flocculation and electrical properties considered in the last section provide strong evidence for a kinetic aggregation mechanism of filler particles in elastomers. A further strong indication for the CCA-mechanism is given by the predicted scaling behavior of the small strain modulus considered below. We will see that this scaling behavior is well fulfilled for different elastomer systems with various fillers. On the contrary, the corresponding scaling prediction of percolation theory clearly fails if applied for filler reinforced rubbers, since experimental data result in much smaller exponents than the predicted one [57].

52

Manfred Klppel

Fig. 36 Schematic view of kinetically aggregated filler clusters in rubber below and above the gel point F*: the left side characterizes the local structure of carbon black clusters, build by primary particles and primary aggregates; accordingly, every black disc on the right side represents a primary aggregate

5.1 Structure and Elasticity of Filler Networks at Small Strain 5.1.1 Cluster-Cluster Aggregation (CCA) in Elastomers

The kinetic cluster-cluster-aggregation (CCA)-model is based upon the assumption that nanoscopic filler particles, like carbon blacks, are not fixed in space but can perform random movements, i.e., the particles are allowed to fluctuate around their mean position in a polymer matrix. Upon contact of neighboring particles or clusters they stick together, irreversibly. This refers to the fact that the thermal energy of colloidal particles is in general much smaller than their interaction energy. Due to the high viscosity of the polymer, the mobility of the particles is restricted, but it increases significantly with decreasing particle size and increasing temperature because the viscosity decreases. For sufficient high temperature, small filler particles and high filler concentrations, above the gel point (F>F*), the mean distance of the particles becomes smaller than the fluctuation length, implying that the aggregation mechanism is no longer influenced by the restricted mobility of the particles. Under this condition, diffusion limited cluster by cluster aggregation leads to a space-filling configuration of CCA-clusters, similar to colloid aggregation in low viscosity media [21–23, 25, 85]. A schematic view of this situation above the gel point F>F* is shown in Fig. 36. For filler concentrations just below the gel point, an irregular configuration of partly separated clusters results as shown in the center of Fig. 36. Note that the global connectivity of such systems, as experienced, e.g., by the electrical conductivity measurements in Sect. 4.2, is similar to a percolation structure, since the clusters are “randomly connected” by small conducting gaps. This reflects the fact that the mechanical gel point is generally larger than the electrical percolation threshold (F*>Fc). A discussion of this point is found in [22].

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

53

Due to the characteristic self-similar structure of the CCA-clusters with fractal dimension df1.8 [3–8, 12], the cluster growth in a space-filling configuration above the gel point F* is limited by the solid fraction FA of the clusters. The cluster size is determined by a space-filling condition, stating that, up to a geometrical factor, the local solid fraction FA equals the overall solid concentration F: FA ðFÞ ¼NF1 F for F>F

ð21Þ

The proportionality constant NF in Eq. (21) is a generalized Flory-Number of order one (NFﬃ1) that considers a possible interpenetrating of neighboring clusters [22]. For an estimation of cluster size in dependence of filler concentration we take into account that the solid fraction of fractal CCAclusters fulfils a scaling law similar to Eq. (14). It follow directly from the definition of the mass fractal dimension df given by NAﬃ(x/d)df, which implies 3df NA ðxÞ d3 Fp VA d FA ðxÞ ¼ ﬃ Fp ð22Þ 3 3 x ðp=6Þ x x Here, VA is the solid volume and NA is the number of particles or primary aggregates of size d in the clusters of size x. Fp is the solid fraction of primary aggregates considered in Sect. 3.2.2. For spherical filler particles it equals Fp=1. From a combination of Eqs. (21) and (22) one finds that the cluster size x decreases with increasing filler concentration F according to a power law. This reflects the fact that smaller clusters occupy less empty space than larger clusters (space-filling condition). It means that the correlation length of the CCA filler network, i.e., the size of the fractal heterogeneity, decreases with increasing filler concentration. This is similar as in percolation theory, though the scaling behavior is generally different. 5.1.2 Elasticity of Flexible Chains of Filler Particles

In view of a micro-mechanical characterization of the elasticity of fractal CCA-filler networks it is sufficient to consider the elastic properties of a single unit cell, because the system is homogeneous on length scales larger than the correlation length x. This implies that the elastic modulus GA of a single CCA-cluster is representative for the whole network. It can be evaluated by referring to Kantor and Webmans model of flexible chains of filler particles that is based on a vectorial Born-lattice model with a tension- and bending energy term between contacting particles [155]. Thereby, we use an approximation of the CCA-cluster backbone as a single spanning arm, i.e., we describe it as a tender, curved rod [21–23]. This is possible, because the CCAcluster backbone has almost no branches [3, 12], implying that the energy of a strained cluster is primary stored in filler-filler bonds along the connecting

54

Manfred Klppel

Fig. 37 Schematic view of the decomposition of a CCA-cluster in elastically active backbone particles and inelastic dead ends. Energy is stored along the connecting path of the backbone particles, indicated as the curved line

path between the backbone particles. A schematic representation of this approach is depicted in Fig. 37. According to this model, the clusters act as molecular springs with end to end distance x, consisting of NB backbone units of length d. The connectivity of the backbone units is characterized by the backbone fractal dimension df,B. Due to the fractal nature of CCA-clusters it holds that df ;B x NB ﬃ ð23Þ d In the present approximation, df,B is identified with the minimum fractal dimension, i.e., df,B=dmin1.3 for CCA-clusters [3, 12]. Following the line of Kantor and Webmans two-dimensional model, the strain energy H of a chain composed of a set of NB singly connected units {bi} of length d under an applied force F at the two ends of the chain is given by [155] H ¼

where S2? ¼

F 2 N B S2? F 2 Lll d þ 2Q 2G NB 1 X ½ ðF z Þ ðR i 1 R N B Þ 2 F 2 NB i ¼ 1

ð24Þ

ð25Þ

is the squared radius of gyration of the projection of the chain on a two dimensional plane and Lll ¼

NB 1 X ðF bi Þ2 F2 d i ¼ 1

ð26Þ

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

55

Fig. 38 Illustration of Kantor and Webmans model of flexible chains with tension-, bending-, and twisting energy terms [155]

Here, G and Q are local elastic constants corresponding to the changes of angles between singly connected bonds and longitudinal deformation of single bonds, respectively. The vector z is a unit vector perpendicular to the plane. For long chains the second term in Eq. (24) can be neglected and the major part of the strain energy H results from the first term, i.e., the bending term of the chain. Then, the force constant k of the chain, relating the elastic energy to the displacement squared of the end of the chain, is well approximated by the bending force constant kS [155]: k kS ¼G=ðNB S2? Þ

ð27Þ

The mathematical treatment of a three-dimensional generalization of this linear elastic model is more complex. In this case the angular deformation is not limited to the on-plane bending, but also off-plane twisting takes place. This model is depicted schematically in Fig. 38. In a simplified approach introduced by Lin and Lee [56], the contributions from the two different kinds of angular deformation, bending and twisting, have been taken into account by an averaged bending-twisting deformation. This is obtained by replacing the elastic constant G, in the first term of Eq. (24), through an averaged elastic constant G of different kinds of angular deformations. Then, by using the relation S?ﬃx and Eq. (23), one obtains for the force constant kkS of the cluster backbone: k G d 2 þ df ;B kS ¼ 2 ð28Þ d x where k is a geometrical factor of order one. The elastic modulus of the cluster backbone is then found as

56

Manfred Klppel

GA x1 kS ¼

kG d3

3þdf ;B d x

ð29Þ

Equation (29) describes the modulus GA of the clusters as a local elastic bending-twisting energy term G times a scaling function that involves the size and geometrical structure of the clusters. Note that in the case of a linear cluster backbone with df,B=1, Eqs. (28) and (29) correspond to the well know elastic behavior of linear, flexible rods, where the bending modulus falls off with the fourth power of the length x. The above approach represents a generalization of this behavior to the case of curved, flexible rods. Experimental evidence for the elastic response of filler clusters of nano-particle chain aggregates is given by Friedlander et al. [156, 157], who showed by TEM analysis that aggregates of inorganic metal oxides stretch under tension and contract when the tension is relaxed. 5.1.3 Scaling Behavior of the Small Strain Modulus

The small strain viscoelastic behavior of filler reinforced rubbers is well known to be strongly affected by the properties of the filler network. This refers to the fact that the elastic modulus GA of the filler network units, i.e., the CCA clusters, is generally much larger than the elastic modulus GR of the rubber and a rigidity condition GA>>GR is fulfilled. However, from Eq. (29) it is clear that the rigidity condition cannot be fulfilled in all cases, because the modulus GA of the clusters decreases rapidly with increasing size of the clusters. It means that only relatively small filler clusters can reinforce a rubber matrix with GRﬃ0.1 MPa, since large clusters are too soft. In the present linear viscoelastic model of the small strain behavior of elastomer composites, only this case is considered, i.e., the rigidity condition GA>>GR is assumed to be fulfilled. For filler concentrations above the gel point F*, where a through-going filler network is formed, stress between the (closely packed) CCA-clusters is transmitted directly between the spanning arms of the clusters that bend substantially. In this case, the strain of the rubber is almost equal to the strain of the spanning arms of the clusters (eReA). It means that, due to the rigidity condition, GA>>GR, the overwhelming part of the elastic energy is stored in the bending arms of the clusters and the contribution of the rubber to the small strain modulus G0 0 of the sample can be neglected, i.e., G0 0GA. Accordingly, the stored energy density (per unit strain) of highly filled elastomers can be approximated by that of the filler network. This in turn equals the stored energy density of a single CCA-cluster, due to the homogeneity of the filler network on length scales above the cluster size x. In the framework of the approximation given by the rigidity condition, a simple power law relation can be derived for the dependency of the small strain modulus G0 0 of the composite on filler concentration F. It is obtained,

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

57

Fig. 39 Double logarithmic plot of the small strain storage modulus vs filler volume fraction for a variety of carbon black filled composites, as indicated. The solid lines with slope 3.5 correspond to the prediction of Eq. (30). Data of butyl/N330 composites are taken from [28] (compare Fig. 2a)

if GA in Eq. (29) is expressed by the solid fraction Eq. (22) and the space-filling condition Eq. (21) is used: G FA ð3þdf ;B Þ=ð3df Þ G F ð3þdf ;B Þ=ð3df Þ G0o ﬃ 3 ﬃ 3 ð30Þ d d Fp Fp Accordingly, we expect a power law behavior G0 0~(F/Fp)3.5 of the small strain elastic modulus for F>F*. Thereby, the exponent (3+df,B)/(3df )3.5 reflects the characteristic structure of the fractal heterogeneity of the filler network, i.e., the CCA-clusters. The strong dependency of G0 0 on the solid fraction Fp of primary aggregates reflects the effect of “structure” on the storage modulus. The predicted power law behavior G0 0~F3.5 for filler concentrations above the gel point is confirmed by the experimental results depicted in Fig. 39 and Fig. 40, where the small strain storage modulus of a variety of filled rubbers is plotted against filler loading in a double logarithmic manner. Figure 39 shows the scaling properties for carbon black composites, i.e., for the low structure black N326 in NR and S-SBR, respectively, and the classical butyl/N330-data of Payne [28], already depicted in Fig. 2a. Within the framework of experimental errors, Eq. (30) is found to be fairly well fulfilled for all systems. Note however that the 3.5-power law is in general not fulfilled for high structure blacks, since for such systems Fp cannot be considered to be independent of filler concentration, but increases due to an enhanced aggregate fracture with increasing filler loading (compare Sect. 3.2.2). Figure 40 demonstrates that the 3.5-power law also holds for NR composites with inorganic- and polymeric fillers, respectively. Beside a technical sil-

58

Manfred Klppel

Fig. 40 Double logarithmic plot of the small strain storage modulus vs filler volume fraction for a variety of NR composites, as indicated. The solid lines with slope 3.5 correspond to the prediction of Eq. (30) [158, 159]

ica filler, polystyrene (PS)- and poly-methoxy-styrene (PMS) microgels are applied as model fillers of definite size (d=100 nm) with a very narrow distribution width. Since these model fillers consist of spherical particles with Fp=1, no disturbing influence of mixing severity on Fp, as found, e.g., for the SBR/N339 composites in Sect. 3.2.2, can appear. The scaling factors of the solid lines allow for an approximate estimation of the front factors of ¯ /d 3 of filler-filler bonds Eq. (30). It yields a typical apparent energy density G of the order of 1 GPa, corresponding to an energy G ﬃ 1012 J. The predicted scaling behavior Eq. (30) is also found to be well fulfilled for carbon black suspensions in ethylene-vinyl-acetate copolymers [51]. Furthermore, it is confirmed by viscoelastic data obtained for S-SBR composites with highly cross-linked BR-microgels of various size [57]. Equation (39) describes the small strain modulus G0 0 as product of a local 3 of filler-filler bonds and a geometrical factor, considerelastic constantG/d ing the structure of the filler network. Accordingly, the temperature- or fre quency dependency of G0 0 is determined by the bending-twisting energy G of the filler-filler bonds, which is controlled by the bound rubber phase around the filler clusters. Coming back to the model of filler-filler bonds developed in Sect. 4.3 and depicted in Fig. 33, the energy in a strained bond is primary stored in a nanoscopic bridge of immobilized, glassy polymer between the filler particles, implying that the temperature- or frequency dependence of G0 0 is given by that of the glassy polymer. Consequently, for highly filled rubbers above the glass transition temperature, we expect an Arrhenius temperature behavior typical for polymers in the glassy state. This is in agreement with experimental findings [26–28]. We finally note that the decomposition of G0 0 into a local elastic constant and a geometrical factor implies that the same form as Eq. (30) must also hold for the loss modulus G00 0. This follows from the fact that in the linear

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

59

viscoelastic regime any geometrical factor must act on the real and imaginary part of the complex modulus in the same way. Otherwise, the KramersKronig relations, indicative for linear systems, cannot be fulfilled [160]. From experimental data this is not always obvious, since the relatively small phase angle at small strain amplitudes can not be estimated as accurate as the norm of the modulus. In particular, the viscoelastic data of Payne [28] on butyl/N330-composites, depicted in Fig. 2b, show that the tan d at small strain is almost independent of filler loading, implying that in the linear regime storage and loss modulus transform with the same geometrical factor. 5.2 Stress Softening and Filler-Induced Hysteresis at Large Strain 5.2.1 Strength and Fracture of Filler Clusters in Elastomers

So far, we have considered the elasticity of filler networks in elastomers and its reinforcing action at small strain amplitudes, where no fracture of fillerfiller bonds appears. With increasing strain, a successive breakdown of the filler network takes place and the elastic modulus decreases rapidly if a critical strain amplitude is exceeded (Fig. 42). For a theoretical description of this behavior, the ultimate properties and fracture mechanics of CCA-filler clusters in elastomers have to be evaluated. This will be a basic tool for a quantitative understanding of stress softening phenomena and the role of fillers in internal friction of reinforced rubbers. The failure- or yield strain eF of filler clusters in elastomers can be estimated by referring to the elasticity model of flexible chains with tensionand bending-twisting energy terms, introduced above. According to this model, a single cluster corresponds to a series of two molecular springs: a soft one, representing the bending-twisting mode, and a stiff one, representing the tension mode. This mechanical equivalence is illustrated in Fig. 41. governs the elasOn the one hand, the soft spring with force constant kS~G ticity of the whole system, provided that the deformation of the stiff spring can be neglected. On the other hand, the stiff spring impacts the fracture behavior of the system, since it considers the longitudinal deformation and, hence, separation of filler-filler bonds. The cluster breaks down when a critical separation of bonded filler particles is exceeded, i.e., if the failure strain eb of filler-filler bonds is reached. The failure strain eF of the filler cluster is then determined by the stress equilibrium between the two springs, which reads in the case of large clusters with kb>>kS: kb Q eb x 2þdf ;B eF ¼ 1 þ ð31Þ eb ks kG d Here, kb=Q/d 2 is the force constant of longitudinal deformations of fillerfiller bonds and kS is the bending-twisting force constant of the cluster, which is given by Eq. (28). From Eq. (31) one finds that the yield strain of a

60

Manfred Klppel

Fig. 41 Schematic view demonstrating the mechanical equivalence between a filler cluster and a series of soft and stiff molecular springs, representing bending-twisting- and tension deformation of filler-filler bonds, respectively

and infiller cluster depends on the ratio between the elastic constants Q/G creases with the cluster size x according to a power law. Consequently, larger clusters show a higher extensibility than smaller ones, due to the ability to bend and twist around the bonds. This kind of elastic behavior of filler clusters and the dependence of strength on cluster size implies a high flexibility of filler clusters in strained rubbers. It plays a crucial role in rubber reinforcement even up to large strains. In particular, the Payne effect, shown, e.g., in Fig. 2 and Fig. 42, can be modeled by referring to a specific size distribution of clusters in the filler network and assuming a successive breakdown of filler clusters with increasing strain [56]. Then, the broadness of the transition regime of the storage modulus (about three decades of strain) reflects the width of the size distribution of clusters in the filler network. Equations (29)–(31) allow for a qualitative analysis of the transition of the elastic modulus from the small strain plateau value to the high strain non-linear behavior. This transition becomes apparent in Fig. 42, showing the strain dependent storage modulus of EPDM- and S-SBR composites filled with the same amount of graphitized and non-graphitized N220, respectively. Since in first approximation the morphology of primary carbon black aggregates can be considered to be not much different, i.e., d=constant and Fp=constant, Eqs. (29) and (30) imply with GA G0 0 that the cluster size x is roughly the same for all four systems. Hence, the differences observed in the critical strain amplitude eapp, where non-linearity appears, and those in the small strain modulus G0 0 have to be related to differences in the elastic Due to Eq. (29), the higher values of G0 0 for the EPDMconstants Q and G. composites and the systems with the graphitized black, respectively, indicate stiffer filler-filler bonds with larger values of the bending-twisting constant Equation (31) implies that the lower values of eapp for the systems with G. the graphitized black can partly be related to the same effect, i.e., larger val provided eapp~eF is assumed. However, a closer analysis shows that ues of G, the shift factor describing the variation of eapp is significantly larger than that of G0 0. This emphasizes that the systems with the graphitized black ex-

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

61

Fig. 42 Strain dependency of the storage modulus at 20 C of cross-linked S-SBR- and EPDM composites filled with 50 phr N220 and graphitized N220g, respectively

hibit smaller values of the tension energy Q of filler-filler bonds, reflecting a lower interaction strength between the particles. These results can be well understood, if the model of filler-filler bonds developed in Sect. 4.3 is considered, again. It implies that the local elastic con¯ are controlled by the rubber phase around fillers, i.e., they stants Q and G are attributed to the amount of bound rubber and its influence on the spacing of contact gaps. The elastic constant Q is also affected by the van der Waals force between contacting filler particles, representing the driving force of filler aggregation. A comparison of the S-SBR-systems shown in Fig. 42 and the annealed systems in Fig. 35 makes clear that cross-linking has no pronounced effect on the viscoelastic data, though the difference between both filler types decreases during cross-linking and the cross-over point is shifted to somewhat smaller strain amplitudes. Note that, apart from cross-linking, the systems have been prepared with respect to the same procedure, but the measurement temperature is different. For analyzing the fracture behavior of filler clusters in strained rubbers, it is necessary to estimate the strain of the clusters in dependence of the external strain of the samples. In the case of small strains, considered above, both strain amplitudes in spatial direction m are equal (eA,m=em), because the stress is transmitted directly between neighboring clusters of the filler network. For strain amplitudes larger than about 1%, this is no longer the case, since a gel-sol transition of the filler network takes place with increasing strain [57, 154] and the stress of the filler clusters is transmitted by the rubber matrix. At larger strains, the local strain eA,m of a filler cluster in a strained rubber matrix can be determined with respect to the external strain em, if a stress equilibrium between the strained cluster and the rubber matrix is assR;m ðem Þ . With Eq. (29) this implies sumed eA;m GA ðxm Þ ¼^

62

Manfred Klppel

eA;m ðem Þ ¼

3þdf ;B d 3 xm ^ R;m em s kG d

ð32Þ

Here, xm denotes the cluster size in spatial direction m of the main axis ^ R;m ðem Þ is the norm of the relative stress of the rubber with resystem and s spect to the initial stress at the beginning of each strain cycle, where @em/ @t=0: ^ R;m ðem Þ sR;m ðem Þ sR;m ð@em =@t ¼ 0Þ ð33Þ s The application of this normalized, relative stress in Eq. (32) is essential for a constitutive formulation of cyclic cluster breakdown and re-aggregation during stress-strain cycles. It implies that the clusters are stretched in spatial directions with @em/@t>0, only, since eA,m0 holds due to the norm in Eq. (33). In the compression directions with @em/@t<0 re-aggregation of the filler particles takes place and the clusters are not deformed. An analytical model for the large strain non-linear behavior of the nominal stress sR,m(em) of the rubber matrix will be considered in the next section. A comparison of Eqs. (31) and (32) makes clear that for large deformations, when the stress of the clusters is transmitted by the rubber matrix, the strain eA,m of the clusters increases faster with their size xm than the failure strain eF,m. Accordingly, with increasing strain the large clusters in the system break first followed by the smaller ones. The maximum size xm of clusters surviving at exposed external strain em is estimated by the stress equilibrium between the rubber matrix and the failure stress sF,m=eF,mGA(xm) of the clusters: xm ðem Þ ¼

Q eb 2 ^ R; m ðem Þ d s

ð34Þ

This allows for an evaluation of the stress contribution of the stretched filler clusters if the size distribution of the clusters in the system is known. Note that for small deformations, where eA,m=em holds, the situation is different, since eA,m is independent of cluster size. Then, the small clusters break first followed by the larger ones. 5.2.2 Free Energy Density of Reinforced Rubbers

Starting from a particular size distribution of kinetically aggregated filler clusters in a rubber matrix, we can now formulate the free energy density of a highly strained sample by assuming the following microscopic scenario. With increasing strain of a virgin sample, a successive breakdown of filler clusters takes place under the exposed stress of the bulk rubber. This process begins with the largest clusters and continues up to a minimum cluster size xm,min in spatial direction m, which is given by Eq. (34) evaluated for the ^ R;m ðem;max Þ reached at maximum exmaximum stress of the rubber matrix s

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

63

Fig. 43 Schematic view of the decomposition of filler clusters in rigid and fragile units for pre-conditioned samples. The right side shows the cluster size distribution with the pre-strain dependent boundary size xmin

ternal strain e,max. During the back-cycle, complete re-aggregation takes place, but the filler-filler bonds that are formed after once being broken are significantly weaker and softer than the original annealed ones. For subsequent stress-strain cycles of a pre-conditioned sample, two micro-mechanical mechanisms of rubber reinforcement are distinguished: 1. Hydrodynamic reinforcement of the rubber matrix by the fraction of hard, rigid filler clusters with strong filler-filler bonds that have not been broken during previous deformations. 2. Cyclic breakdown and re-aggregation of the residual fraction of fragile, soft filler clusters with weaker filler-filler bonds.

The fraction of rigid filler clusters decreases with increasing pre-strain, while the fraction of fragile filler clusters increases. The decomposition into rigid and fragile filler cluster units is illustrated in Fig. 43. The fragile filler clusters with soft bonds bend substantially in the stress field of the rubber, implying that their contribution to hydrodynamic reinforcement is relatively small. The mechanical action of the fragile filler clusters refers primary to a viscoelastic effect, since any type of cluster that is stretched in the stress field of the rubber stores energy that is dissipated when the cluster breaks. This mechanism leads to a filler-induced viscoelastic contribution to the total stress that impacts the internal friction of filled rubber samples, significantly. Note that this kind of viscoelastic response is present also in the limit of quasi-static deformations, where no explicit time dependency of the stress-strain cycles is taken into account. According to these considerations, we assume that for quasi-static, cyclic deformations of filler reinforced rubbers up to large strain the total free energy density consists of two contributions: Wðem Þ ¼ WR ðem Þ þ WA ðem Þ

ð35Þ

The first addend is the equilibrium energy density stored in the extensively strained rubber matrix, which includes hydrodynamic reinforcement by a

64

Manfred Klppel

fraction of rigid filler clusters (see below). The second addend considers the energy stored in the substantially strained fragile filler clusters: WA ðem Þ ¼

_ m >0 eX m

xm ðem Þ

1 2d

Z

GA x0m e2A;m x0m ; em f x0m dx0m

ð36Þ

xm;min

where the dot denotes time derivative. Here, f(x) is the normalized size distribution of the CCA-clusters in spatial direction of the main axis system. It can be evaluated by referring to Smoluchowskis equation for the kinetics of irreversible cluster-cluster aggregation of colloids [8, 161, 162]. In the case of large clusters (and large times), one can obtain a reduced form of the size distribution function [8]: !2 W ! xm ð1 2 WÞ xm 4d for m ¼ 1; 2; 3 f ðxm Þ ¼ exp < xm > < xm > < xm > ð37Þ For W<0, this distribution function is peaked around a maximum cluster size (2W/(2W1))<xm>, where <xm> is the mean cluster size. 2W=a+df1 is a parameter describing details of the aggregation mechanism, where a0 is an exponent considering the dependency of 0 the diffusion constant D of the clusters on its particle number, i.e., D~NAa . This exponent is in general not very well known. In a simple approach, the particles in the cluster can assumed to diffusion independent from each other, as, e.g., in the Rouse model of linear polymer chains. Then, the diffusion constant varies inversely with the number of particles in the cluster (D~NA1), implying 2W=0.44 for CCA-clusters with characteristic fractal dimension df=1.8. The sum in Eq. (36) is taken over the stretching directions with @em/@t>0, only, implying that the free energy density is anisotropic. This corresponds to the assumption that clusters are strained and successively broken in stretching directions, while healing of the clusters takes place in the compression directions. It insures that a cyclic breakdown and re-aggregation of clusters can be described. The integration in Eq. (36) is performed over the fraction of fragile filler clusters that are not broken at exposed strain e of the actual cycle (Eq. 34). The clusters smaller than x,min, representing the fraction that survived the first deformation cycle, are not considered in Eq. (36). Due to the stiff nature of their filler-filler bonds, referring to the bonds in the virgin state of the sample, these clusters behave rigid and give no contribution to the stored energy. Instead, they dominate the hydrodynamic reinforcement of the rubber matrix. This is specified by the strain amplification factor X, which relates the external strain em of the sample to the internal strain ratio lm of the rubber matrix: lm ¼ 1 þ Xem

ð38Þ

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

65

In the case of a pre-conditioned sample and for strains smaller than the previous straining (em<em,max), the strain amplification factor is constant and determined by em,max (X=X(em,max)). For the first deformation of virgin samples it depends on the external strain (X=X(em)). By applying a relation derived by Huber and Vilgis [64, 65] for the strain amplification factor of overlapping fractal clusters, X(em,max) or X(em) can be evaluated by averaging over the size distribution of rigid clusters in all space directions. In the case of pre-conditioned samples this yields

F X ðem;max Þ ¼ 1 þ c Fp

xm;min 3d2 X Z 3 f 1 m¼1

d

x0m d

!dw df

f x0m dx0m

ð39Þ

0

where c is a constant of order one and dw3.1 [23] is the anomalous diffusion exponent on fractal CCA-clusters. For the deformation of a virgin sample, X(em) is obtained in a similar way by performing the integration from zero up to the strain dependent cluster size xm(em) determined by Eq. (34). An important role in the present model is played by the strongly non-linear elastic response of the rubber matrix that transmits the stress between the filler clusters. We refer here to an extended tube model of rubber elasticity, which is based on the following fundamental assumptions. The network chains in a highly entangled polymer network are heavily restricted in their fluctuations due to packing effects. This restriction is described by virtual tubes around the network chains that hinder the fluctuation. When the network elongates, these tubes deform non-affinely with a deformation exponent n=1/2. The tube radius r in spatial direction of the main axis system depends on the deformation ratio l as follows: rm ¼ro lnm

ð40Þ

where ro is the tube radius in the non-deformed state. The assumption of the non-affine tube deformation (n=1/2) is essential. It was initially derived based upon fundamental molecular statistical calculations [24, 163, 164] and later on confirmed by applying scaling arguments [77, 78, 165]. Experimental evidence of non-affine tube deformations according to Eq. (40) is provided by neutron scattering of strained rubbers [166] as well as stress-strain measurements on swollen polymer networks [167]. An extension of the non-affine tube model for applications up to large strains is obtained by considering that the network chains have a finite length and the stress in the network becomes infinitely large, when the chain sections between two subsequent trapped entanglements are stretched fully. The trapping of chain entanglements by two cross-link points prevents the sliding of the chains across each other under extension, implying that the entanglement becomes an elastically effective network junction. The free energy density of the extended, non-Gaussian tube model with non-affine tube deformation is then as follows [75–78, 168]:

66

Manfred Klppel

! 8 3 P > Te > 2 > " l 3 1 > m n e Gc < m¼1 T ! þ ln 1 e WR ðem Þ ¼ 2 > 3 ne P 2 > T > > lm 3 : 1 nee

3 X

!#) l2m

3

m¼1

m¼1

þ 2 Ge

3 X

! l1 m

3

ð41Þ

m¼1

Here, ne is the number of statistical chain segments between two successive entanglements and Te is the trapping factor (0

ð42Þ

r Na l2s kB T pﬃﬃﬃ 4 6 Ms ro2

ð43Þ

Ge ¼

Here, nmech is the mechanically effective chain density specified, e.g., in [168], Ac0.67 [170] is a microstructure factor which describes the fluctuations of network junctions, Na the Avogadro number, r mass density, Ms and ls molar mass and length of a statistic segment, respectively, kB the Boltzmann constant, and T absolute temperature. From Eq. (41) the nominal stress sR, that relates the force F in spatial direction to the initial cross section Ao, is found by differentiation, sR,m=@WR/@lm. For uniaxial extensions of unfilled rubbers (X=1) with l1=l, l2=l3=l1/2 the following relation can be derived:

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

8 > < 2 sR;1 ¼ Gc l l > :

1 Te =ne 1 Tnee ðl2 þ 2=l 3Þ

67

2

Te =ne g þ 2Ge ðl1=2 l2 Þ 1 Tnee ðl2 þ 2=l 3Þ

ð44Þ

For equi-biaxial extensions with l1=l2=l, l3=l2 one finds for the nominal stress: 8 > < 1 Te =ne 5 sR;1 ¼ Gc l l 2 > : 1 Tnee ð2l2 þ l4 3Þ Te =ne 1 Tnee ð2l2 þ l4 3Þ

) þ 2Ge ðl l2 Þ

ð45Þ

In the case of a pure-shear deformation with l1=l, l2=1, and l3=l1 one obtains 8 > < 1 Te =ne 3 sR;1 ¼ Gc l l 2 > : 1 Tnee ðl2 þ l2 2Þ Te =ne 1 Tnee ðl2 þ l2 2Þ

) þ 2Ge ð1 l2 Þ

ð46Þ

By fitting experimental data for different deformation modes to these functions, the three network parameters of unfilled polymer networks Gc, Ge, and ne/Te can be determined. The validity of the concept can be tested if the estimated fitting parameters for the different deformation modes are compared. A “plausibility criterion” for the proposed model is formulated by demanding that all deformation modes can be described by a single set of network parameters. The result of this plausibility test is depicted in Fig. 44, where stress-strain data of an unfilled NR-vulcanizate are shown for the three different deformation modes considered above. Obviously, the material parameters found from the fit to the uniaxial data provide a rather good prediction for the two other modes. The observed deviations are within the range of experimental errors. It should be pointed out that the material parameter Ge can be determined in principle more precisely by means of equi-biaxial measurements than by uniaxial measurements. This is due to the fact that the first addend of the Ge-term in Eq. (45) increases linearly with l. This behavior results from the high lateral contraction on the equi-biaxial extension (l3=l2). It postulates a close dependency of the equi-biaxial stress on the tube constraint modu-

68

Manfred Klppel

Fig. 44 Stress-strain data (symbols) and simulation curves (Eqs. 44–46) of an unfilled NR for three deformation modes. The model parameters are found from a fit to the uniaxial data (Gc=0.43 MPa, Ge=0.2 MPa, ne/Te=68)

lus, since Gc and Ge contribute nearly equally to stress, also at larger extensions. For the uniaxial extensions described in Eq. (44) this is not the case. Here, the tube constraints lead to significant effects only in the region of lower extensions, since the Ge-term in Eq. (44) approaches zero as the l values increase. Nevertheless, the experiments can be carried out more easily in the uniaxial case, and as a result, more reliable experimental data can be obtained. For practical applications, the parameter Ge can also be determined from the value of the plateau modulus GNo, since the relationship Ge1/2GNo applies in accordance with the tube model. This implies that the parameter Ge is not necessary a fit parameter but rather it is specified by the microstructure of the rubber used. Note that the fit value Ge=0.2 MPa obtained in Fig. 44 is in fair agreement with the above relation, since GNo0.58 MPa is found for uncross-linked NR-melts [171]. A comparison of the predictions of the extended tube model to stressstrain data of unfilled rubbers offered good agreement for various polymers and cross-linking systems [75–78, 167, 170, 172, 173]. Further confirmation of the non-affine tube approach was obtained in recent investigations considering mechanical stress-strain data and a transversal NMR-relaxation analysis of differently prepared NR-networks [168]. A representation of the molecular statistical foundations of tube-like topological constraints in strained polymer networks is found in [76], where the path integral formulation of rubber elasticity is briefly reviewed. In the second part of [76], a first attempt for considering stress softening phenomena of filled rubbers on the basis of the extended tube model is formulated. Subsequent investigations have shown that a constitutive formulation of stress softening fulfilling the “plausibility criterion” cannot be achieved in this simplified approach [89]. In the following section we will see that the extended model, as developed above, passes the “plausibility test” fairly well also for filled rubbers.

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

69

The important point lies in the determination of the topological tube constraint modulus Ge according to its physical value Ge1/2GNo, which was not realized in the first considerations. 5.2.3 Stress-Strain Cycles of Filled Rubbers in the Quasi-Static Limit

For filler reinforced rubbers, both contributions of the free energy density Eq. (35) have to be considered and the strain amplification factor X, given by Eq. (39) differs from one. The nominal stress contributions of the cluster deformation are determined by sA,m=@WA/@eA,, where the sum over all stretching directions, that differ for the up- and down cycle, have to be considered. For uniaxial deformations e1=e, e2=e3=(1+e)1/21 one obtains a positive contribution to the total nominal stress in stretching direction for the up-cycle if Eqs. (29)–(36) are used: Q eb ^ R;1 ðeÞ d3 s

up s0;1 ðeÞ

Z

^ R;1 ðeÞ ¼ sR;1 ðeÞ þ s

fðx1 Þ dx1

ð47Þ

Q eb

^ R;1 ðemax Þ d3 s

with the abbreviations ^ R;1 ðeÞ ¼ sR;1 ðeÞ sR;1 ðemin Þ s

ð48Þ

and x1=x1/d. For the down-cycle in the same direction one finds a negative contribution to the total stress: Q eb ð1þeÞ3=2 ~ R;1 ðeÞ 2d3 s

sdown sR;1 ðeÞ 0;1 ðeÞ ¼ sR;1 ðeÞ 2~

Z

fðx1 Þ dx1

ð49Þ

3=2 Q eb ð1þemin Þ ~ R;1 ðemin Þ 2d3 s

with the abbreviation 1 þ emax 3=2 ~ R;1 ðeÞ ¼ sR;1 ðeÞ sR;1 ðemax Þ s 1þe

ð50Þ

The negative sign in Eq. (49) results from the norm, implying, e.g., for the relative nominal stresses in direction 1 and 2: ^ R;2 ðeÞ ¼ 2 ð1 þ eÞ3=2 s ~ R;1 ðeÞ s

ð51Þ

This is in contrast to the transformation behavior of the nominal stresses of the rubber matrix with a negative sign: sR;2 ðeÞ ¼ 2 ð1 þ eÞ3=2 sR;1 ðeÞ

ð52Þ

70

Manfred Klppel

Note that the different choice of the extrema with @em /@t=0 in Eqs. (48) and (50) are due to the fact that an up-cycle begins at e=emin, but a downcycle begins at e=emax. As a rule, the relative stresses in the lower boundaries of the integrals in Eqs. (47) and (49) have to be chosen in such a way that they reach their maximum values, implying that all fragile clusters are broken and xm=xm,min. In deriving Eq. (49) we assumed an isotropic cluster size distribution, i.e., f(x1)=f(x2)=f(x3). This appears reasonable since f(xm) refers to the size distribution of clusters in the virgin, unstrained state. However, from the basic concept of cluster breakdown in the stretching direction and re-aggregation in the compression direction, respectively, it is clear that the size distribution of the filler clusters during the deformation cycles is strongly anisotropic. It leads to the characteristic hysteresis of a pre-strained sample, as given by Eqs. (47)–(50), even in the case of a quasi-static deformation at infinite slow strain rates. Figure 45a–c shows an adaptation of the developed model to uniaxial stress-strain data of a pre-conditioned S-SBR-sample filled with 40 phr N220. The fits are obtained for the third stretching cycles at various prestrains by referring to Eqs. (38), (44), and (47) with different but constant strain amplification factors X=Xmax for every pre-strain. For illustrating the fitting procedure, the adaptation is performed in three steps. Since the evaluation of the nominal stress contribution of the strained filler clusters by the integral in Eq. (47) requires the nominal stress sR,1 of the rubber matrix, this quantity is developed in the first step shown in Fig. 45a. It is obtained by demanding an intersection of the simulated curves according to Eqs. (38) and (44) with the measured ones at maximum strain of each strain cycle, where all fragile filler clusters are broken and hence the stress contribution of the strained filler clusters vanishes. The adapted polymer parameters are Gc=0.176 MPa and ne/Te=100, independent of pre-strain. According to the considerations at the end of Sect. 5.2.2, the tube constraint modulus is kept fixed at the value Ge=0.2 MPa, which is determined by the plateau modulus GNo0.4 MPa [174, 175] of the uncross-linked S-SBR-melt (Ge=1/2GNo). The adapted amplification factors Xmax for the different pre-strains (emax=1, 1.5, 2, 2.5, 3) are listed in the insert of Fig. 45a. Figure 45b (upper part) shows the residual stress contribution of the strained filler clusters for the different pre-strains, obtained by subtracting the polymer contributions (solid lines) from the experimental stress-strain data (symbols) of Fig. 45a. The resulting data (symbols) are fitted to the second addend of Eq. (47) (solid lines), whereby the size distribution of filler clusters Eq. (37), shown in the lower part of Fig. 45b, has been used. The size distribution f(x1) is determined by the adapted mean cluster size <x1><x1/d>=26 and the pre-chosen distribution width W=0.5, which allows for an analytical solution of the integral in Eq. (47). The tensile strength of filler-filler bonds is found as Qeb/d3=24 MPa. The different fit lines result from the different stress-strain curves sR,1(e) that enter the upper boundary of the integral in Eq. (47). Note that this integral, representing the contribution of the strained filler clusters to the total stress, becomes zero at e=emax for every pre-strain.

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

71

Figure 45c shows the complete adaptation with Eq. (47) of the uniaxial stress-strain data, i.e., the sum of the two contributions shown in Fig. 45a,b. The fits for all pre-strained samples are very good in the large as well as the small strain regime, which is separately shown up to 150% strain in the insert of Fig. 45c. Furthermore, beside the third stretching cycles at various pre-strains, the first stretching of the virgin sample is shown. It is compared to a simulation curve given by Eq. (47) with the above specified material parameters and a strain dependent amplification factors X=X(e). Unfortunately, Eq. (39) cannot simply be applied for an estimation of X(e), since the upper boundary of the integral xm(e) depends on X(e) itself (Eq. 34) and a general analytic solution of the integral is not known. For that reason an empirical power law dependency of the amplification factor X on a scalar strain variable E, involving the first deformation invariant I1(em), has been applied [76, 89]: X ðEÞ ¼ X1 þ ðXo X1 Þ ð1 þ EÞy

with E ðem Þ

3 X

ð53Þ

!1=2 2

ð1 þ em Þ 3

ð54Þ

m¼1

Here, X1 and Xo are the strain amplification factors at infinite and zero strain, respectively, and y is an empirical exponent. An adaptation of this empirical function, Eq. (53), to the Xmax-values obtained for the pre-strained samples shown in Fig. 45a delivers the parameters Xo=11.5, X1=1.21, and y=0.8, which are used for the simulation of the first stretching cycle shown in Fig. 45c. A comparison of the experimental data for the first stretching cycle of the samples to the simulation curve in Fig. 45c shows no good agreement. Significant deviations are observed especially in the low strain regime, shown in the insert, where an extrapolation of the function X(E) is used. The reason for the deviations may partly lie in the application of the power law approximation Eq. (53) for X(E), instead of the micro-mechanically motivated Eq. (39). This may also lead to the unphysical negative value of X at extrapolated infinite strain (X1=1.21). A better fit between simulation and experimental data of the first extension of the virgin sample is obtained if the same model as above is used, but an empirical cluster size distribution is chosen instead of the physically motivated distribution function Eq. (37). This is demonstrated in Fig. 46a,b, where the adaptation of the same experimental data as above is made with a logarithmic normal form of the cluster size distribution function f(x1) with x1=x1/d: 2 1 >Þ exp lnðx1 =<x 2 b2 pﬃﬃﬃﬃﬃﬃﬃﬃ f ðx1 Þ ¼ ð55Þ p=2 b x1

72

Manfred Klppel

Fig. 45 a Uniaxial stress-strain data (symbols) of S-SBR samples filled with 40 phr N220 at various pre-strains emax and simulation curves (lines) of the polymer contribution according to Eqs. (38) and (44). The set of polymer parameters is found as Gc=0.176 MPa, Ge=0.2 MPa, and ne/Te=100. b Stress contributions of the strained filler clusters for the different pre-strains (upper part), obtained by subtracting the polymer contributions from the experimental stress-strain data of a. The solid lines are adaptations with the integral term of Eq. (47) and the cluster size distribution Eq. (37), shown

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

73

Figure 46a shows that a reasonable adaptation of the stress contribution of the clusters can be obtained, if the distribution function Eq. (55) with mean cluster size <x1>=25 and distribution width b=0.8 is used. Obviously, the form of the distribution function is roughly the same as the one in Fig. 45b. The simulation curve of the first uniaxial stretching cycle now fits much better to the experimental data than in Fig. 45c. Furthermore, a fair simulation is also obtained for the equi-biaxial measurement data, implying that the “plausibility criterion”, discussed at the end of Sect. 5.2.2, is also fulfilled for the present model of filler reinforced rubbers. Note that for the simulation of the equi-biaxial stress-strain curve, Eq. (47) is used together with Eqs. (45) and (38). The strain amplification factor X(E) is evaluated by referring to Eqs. (53) and (54) with e1=e2=e and e3=(1+e)21. Similar well fitting simulation curves for the experimental stress-strain data as those shown in Fig. 46b can also be obtained for higher filler concentrations and silica instead of carbon black. In most cases, the log-normal distribution Eq. (55) gives a better prediction for the first stretching cycle of the virgin samples than the distribution function Eq. (37). Nevertheless, adaptations of stress-strain curves of the pre-strained samples are excellent for both types of cluster size distributions, similar to Fig. 45c and Fig. 46b. The obtained material parameters of four variously filled S-SBR composites used for testing the model are summarized in Table 4, whereby both cluster

in the lower part. The obtained parameters of the filler clusters are Qeb/d 3=24 MPa, <x1>=26, and W=0.5. c Uniaxial stress-strain data (symbols) of the S-SBR samples with 40 phr N220 at various pre-strains emax and for the first stretching, as indicated. The insert shows a magnification for the smaller strains. The lines are simulation curves with parameters specified in a,b

74

Manfred Klppel

75

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

Table 4 Material parameters obtained from adaptations of the model to uniaxial stressstrain data of four S-SBR samples filled with 40 and 60 phr N220 (C40, C60) and silica (S40, S60), respectively. Further polymer parameters are given as Ge=0.2 MPa and ne/Te=100, independent of sample type Cluster distribution Eq. (55) Sample type C40 C60 S40 S60

Gc [MPa] 0.176 0.190 0.120 0.130

<x>

b

25 18 19 22

0.8 0.8 0.8 0.8

Qeb/d3 [MPa] 26 26 24 24

Cluster distribution Eq. (37) <x>

W

26 20 27 31

0,5 0,5 0,5 0,5

Qeb/d3 [MPa] 24 24 28 28

X(E) Eq. (53) X1

Xo

y

1.209 0.329 0.165 0.148

11.52 17.40 14.12 15.24

0.803 1.180 1.094 1.130

size distributions, Eq. (37) and Eq. (55), have been considered. The obtained fit parameters for the polymer network, filler cluster morphology, and bond fracture mechanics appear physically suitable. In particular, the value of the cross-link modulus Gc increases with filler concentration due to the attachment of polymer chains at the filler surface, implying an increased effective cross-link density with rising filler loading. The Gc-values of the silica filled systems are found to be somewhat smaller than the carbon black filled systems, indicating that a higher fraction of curatives is deactivated by adsorption at the silica surface as compared to the carbon black surface. The estimated mean cluster size between <x>20 to 30 times the particle diameter d appears reasonable. With d100 nm one finds <x> on the length scale of a few micrometers. Note that, due to Eq. (34), the quantity Qeb/d 3 represents the failure stress of filler-filler bonds, i.e., the limiting stress where all clusters are broken and the cluster size equals the particle size (x=d). The obtained fair agreement of the fitted values Qeb/d 324 to 28 MPa with the tensile strength of the samples, which typically lies around 20 MPa, indicates that the failure stress of filler reinforced rubber samples is closely related to the failure stress of the filler-filler bonds. It demonstrates that the proposed mechanism of rubber reinforcement by stress-induced filler cluster breakdown can be considered to be responsible for the strongly enhanced tensile

t Fig. 46 a Stress contributions of the strained filler clusters for the different pre-strains (upper part), obtained as in Fig. 45b. The solid lines are adapted with the integral term of Eq. (47) and the log-normal cluster size distribution Eq. (55), shown in the lower part. The obtained parameters of the filler clusters are Qeb/d 3=26 MPa, <x1>=25, and b=0.8. b Uniaxial stress-strain data (symbols) as in Fig. 45c. The insert shows a magnification for the smaller strains, which also includes equi-biaxial data for the first stretching cycle. The lines are simulation curves with the log-normal cluster size distribution Eq. (55) and material parameters as specified in the insert of Fig. 45a and Table 4, sample type C40

76

Manfred Klppel

strength of filled rubbers. Obviously, rupture of the whole sample appears somewhat before the last filler-filler bonds break down. The success of the developed model in predicting uniaxial and equi-biaxial stress strain curves correctly emphasizes the role of filler networking in deriving a constitutive material law of reinforced rubbers that covers the deformation behavior up to large strains. Since different deformation modes can be described with a single set of material parameters, the model appears well suited for being implemented into a finite element (FE) code for simulations of three-dimensional, complex deformations of elastomer materials in the quasi-static limit. Beside the consideration of the up-cycles in the stretching direction, the model can also describe the down-cycles in the backwards direction. This is depicted in Fig. 47a,b for the case of the S-SBR sample filled with 60 phr N 220. Figure 47a shows an adaptation of the stress-strain curves in the stretching direction with the log-normal cluster size distribution Eq. (55). The depicted down-cycles are simulations obtained by Eq. (49) with the fit parameters from the up-cycles. The difference between up- and down-cycles quantifies the dissipated energy per cycle due to the cyclic breakdown and re-aggregation of filler clusters. The obtained microscopic material parameters for the viscoelastic response of the samples in the quasi-static limit are summarized in Table 4. A comparison of the simulation curves in Fig. 47a with experimental stress-strain cycles, depicted, e.g., in Fig. 3, shows a significantly different behavior of the down-cycles. Obviously, the evaluated stress contribution of the strained filler clusters during the down cycle, i.e., the integral term of Eq. (49), is too small to explain the difference between the experimentally observed up- and down-cycles in the high strain regime, where the upturn of the stress appears. The reason for this deviation can partly be found in the pronounced set behavior of reinforced rubbers that shifts the remaining strain at zero stress to increasing positive values with increasing pre-strain (compare Fig. 3). So far, this set behavior is not considered in the developed model. Concerning the measurement results, it has been compensated by shifting the experimental stress-strain curves of the pre-strained samples into the origin. This procedure is described more closely in [76]. In view of an illustration of the viscoelastic characteristics of the developed model, simulations of uniaxial stress-strain cycles in the small strain regime have been performed for various pre-strains, as depicted in Fig. 47b. Thereby, the material parameters obtained from the adaptation in Fig. 47a (Table 4, sample type C60) have been used. The dashed lines represent the polymer contributions, which include the pre-strain dependent hydrodynamic amplification of the polymer matrix. It becomes clear that in the small and medium strain regime a pronounced filler-induced hysteresis is predicted, due to the cyclic breakdown and re-aggregation of filler clusters. It can considered to be the main mechanism of energy dissipation of filler reinforced rubbers that appears even in the quasi-static limit. In addition, stress softening is present, also at small strains. It leads to the characteristic decline of the polymer contributions with rising pre-strain (dashed lines in

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

77

Fig. 47 a Uniaxial stress-strain data in stretching direction (symbols) of S-SBR samples filled with 60 phr N 220 at various pre-strains emax and simulations (solid lines) of the third up- and down-cycles with the cluster size distribution Eq. (55). Fit parameters are listed in the insert and Table 4, sample type C60. b Simulation of uniaxial stress-strain cycles for various pre-strains between 10 and 50% (solid lines) with material parameters from the adaptation in a. The dashed lines represent the polymer contributions according to Eqs. (38) and (44) with different strain amplification factors

Fig. 47b), which impacts the slope of the stress-strain cycles. This softening effect results from the drop of the strain amplification factor Xmax with increasing pre-strain, which has been determined by an extrapolation of the adapted values, shown in the insert of Fig. 47a, with the power law approximation Eq. (53). It is important to note that stress softening is also present during dynamic stress-strain cycles of filled rubbers at small and medium strain. In particular, this can be concluded from the dynamic mechanical data of the S-SBR samples filled with 60 phr N 220 as shown in Fig. 48. In the framework of the above model, the observed shift of the center point of the cycles to smaller stress values with increasing strain amplitude or maximum strain and the accompanied drop of the slope of the hysteresis cycles can be related to a de-

78

Manfred Klppel

Fig. 48 Dynamic stress-strain cycles obtained from uniaxial harmonic excitations at 1 Hz of the S-SBR samples filled with 60 phr N 220 at fixed pre-strain and various strain amplitudes, as indicated

creasing strain amplification factor Xmax. It implies that a pronounced Payne effect appears also for pre-strained samples that compares to the one observed for dynamic excitations around the stress-strain origin. This has led to some conceptual problems in relating the Payne effect to filler network breakdown [176, 177], which is briefly reviewed in the introduction section of [57]. The problems arise primary from the fact that the shifting of the center points of the hysteresis cycles due to stress softening is ignored if the concept of linear viscoelasticity is applied and only the dynamic storage and loss moduli are considered. The experimental stress-strain cycles shown in Fig. 48 are quite similar to the simulation curves in Fig. 47b, though the stress level of the experimental curves is somewhat larger. This can partly be related to the fact that the true stress is shown, which is by a factor of about 1.25 larger than the apparent stress. Nevertheless, it appears that the extrapolated strain amplification factors Xmax, used for the simulation, are too small and a separate adaptation for the small strain regime is needed. However, at present an adaptation of the developed model to the dynamic data is not possible, mainly for two reasons. On the one hand, an explicit time dependency of the stress-strain cycles is not considered so far. On the other, only full cycles from maximum to minimum strain can be described, where all fragile clusters break down and re-combine. A more general model must also consider the re-aggregation mechanism in dependence of strain, in order to describe all kind of stressstrain cycles. This will be a task of future work. Despite these limitations there is strong evidence that the Payne effect can be described on the basis of the derived model of stress softening and filler-induced hysteresis, which allows for a proper simulation of quasi-static stress-strain curves, referred to

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

79

as Mullins effect. This demonstrates that both effects can be traced back to the same micro-mechanical mechanism.

6 Summary and Conclusions In the first part of the chapter (Sect. 3), the morphology and surface activity of carbon black, the most important filler in the rubber industry, are analyzed. It is shown that, due to the disordered nature of carbon black formation during processing in a furnace reactor, the morphology of furnace blacks is well described by referring to a fractal analysis. Investigations of the surface roughness of carbon blacks by static gas adsorption point out that all furnace blacks exhibit a pronounced surface roughness with an almost unique value of the surface fractal dimension ds2.5–2.6 on atomic length scales below 6 nm. This universality is related to a particular random deposition mechanism of carbon nuclei on condensed carbon particles that governs the surface growth of carbon blacks during processing. Graphitization of carbon blacks diminishes the roughness of the surface on length scales below z<1 nm, while on larger length scales the surface fractal dimension remains unchanged. The surface fractal dimension of all examined graphitized blacks is found as ds2.3 below 1 nm, independent of the applied evaluation procedure. An analysis of the surface energy distribution of furnace blacks demonstrates that four different energetic sites can be distinguished. They are shown to be related to the characteristic surface morphology of carbon blacks. The fraction of highly energetic sites decreases significantly with grade number and disappears almost completely during graphitization. It indicates that the reinforcing potential of carbon black is closely related to the amount of highly energetic sites that can be well quantified by the applied gas adsorption technique at low pressure. According to the universal surface roughness of furnace blacks independent of grade number, one expects that the reinforcing potential owing to the surface roughness of carbon blacks is not much different. Nevertheless, the detected high energetic and morphological disorder of the carbon black surface can considered to be responsible for a strong polymer-filler coupling and phase bonding. Beside the specific surface, this is an important factor for obtaining adequate ultimate properties of carbon black reinforced rubbers. The morphology of the more or less ramified primary carbon black aggregates, as analyzed by TEM techniques, is readily described by a fractal approach. This refers to the specific cluster-cluster aggregation mechanism of primary particles under ballistic conditions, which is realized during carbon black processing. It implies a mass fractal dimension df1.9–1.95, which is indeed found for the fine blacks. For the more coarse furnace blacks larger values of df are obtained that increase with the grade number. This results from electrostatic repulsive interactions between the aggregates due to the application of processing agents. During compounding of carbon blacks with highly viscous rubbers, rupture of primary aggregates takes place de-

80

Manfred Klppel

pending on the mixing severity and grade number. It implies that the aggregate size decreases with increasing mixing time or filler loading, preferably for the high structured coarse blacks. The resulting influence on the mechanical properties of the composites can be described on a quantitative level by considering the rising solid fraction of primary aggregates with increasing mixing severity, which impacts the mechanically effective filler concentration. In the second part of the chapter (Sect. 4), carbon black networking in elastomer composites is analyzed by applying TEM-, electrical percolation-, dielectric- as well as flocculation investigations. This provides information on the fractal nature of filler networks as well as the morphology of fillerfiller bonds. It becomes obvious that TEM analysis gives a limited microscopic picture of the filler network morphology, only, due to spatial interpenetration of flocculated neighboring filler clusters. Investigations of the d.c.-conductivity demonstrate that no universal percolation structure for the filler network is realized on mesoscopic length scales if a critical filler concentration is exceeded. Instead, the structure appears to be modified by a superimposed kinetic aggregation process, which explains the detected nonuniversal value of the percolation exponent and the impact of filler specific surface and polymer micro-structure on the percolation threshold. Flocculation studies, considering the small strain mechanical response of the uncross-linked composites during heat treatment (annealing), demonstrate that a relative movement of the particles takes place that depends on particle size, molar mass of the polymer, as well as polymer-filler and filler-filler interaction. This provides strong experimental evidence for a kinetic clustercluster aggregation mechanism of filler particles in the rubber matrix to form a filler network. The a.c.-conductivity exponent in the high frequency regime is shown to be related to an anomalous diffusion mechanism of charge carriers on fractal carbon black clusters. This confirms the fractal nature of filler networks in elastomers below a certain length scale, though it gives no definite information on the particular network structure. From the dielectric investigations it becomes obvious that charge transport above the percolation threshold is limited by a hopping or tunneling mechanism of charge carriers over small gaps of order 1 nm between adjacent carbon black particles. From this finding and the observed dependency of the flocculation dynamics on the amount of bound rubber, a model of filler-filler bonds is developed. It relates the mechanical stiffness of filler-filler bonds to the remaining gap size between the filler particles that develops during annealing (and cross-linking) of filled rubbers. In this model, stress between adjacent filler particles in a filler cluster is assumed to be transmitted by nanoscopic, flexible bridges of glassy-like polymer, implying that a high flexibility and strength of filler clusters in elastomers is reached. This picture of filler-filler bonds allows for a qualitative explanation of the observed flocculation effects by referring to the amount of bound rubber and it is impact on the stiffness and strength of filler-filler bonds. In the last part of the chapter (Sect. 5), a micro-mechanical model of rubber reinforcement by flexible filler clusters is developed that allows for a

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

81

quantitative analysis of stress softening and hysteresis of filler reinforced rubbers up to large quasi-static deformations. It is shown that the kinetic cluster-cluster aggregation (CCA) model of filler networking in elastomers represents a reasonable theoretical basis for understanding the small strain viscoelastic properties of reinforced rubbers. According to this model, filler networks consist of a space-filling configuration of CCA-clusters with characteristic mass fractal dimension df1.8. The consideration of flexible chains of filler particles, approximating the elastically effective backbone of the filler clusters, allows for a micro-mechanical description of the elastic properties of tender CCA-clusters in elastomers. The main contribution of the elastically stored energy in the strained filler clusters results from the bending-twisting deformation of filler-filler bonds. The predicted power-law behavior of the small strain modulus of filler reinforced rubbers is confirmed by a variety of experimental data, including carbon black and silica filled rubbers as well as composites with model fillers (microgels). Beside the elastic behavior, the failure properties of filler-filler bonds and filler clusters are considered in dependence of cluster size. This completes the micro-mechanical description of tender but fragile filler clusters in the stress field of a strained rubber matrix. By assuming a specific cluster size distribution in reinforced rubbers, which is motivated by an asymptotic solution of Smoluchowskis equation for the kinetics of irreversible clustercluster aggregation, a constitutive material model of filler reinforced rubbers is derived. It is based on a non-affine tube model of rubber elasticity, including hydrodynamic amplification of the rubber matrix by a fraction of rigid filler clusters with filler-filler bonds in the unbroken, virgin state. The fillerinduced hysteresis is described by an anisotropic free energy density, considering the cyclic breakdown and re-aggregation of the residual fraction of more fragile filler clusters with already broken filler-filler bonds. The model assumes that the breakdown of filler clusters during the first deformation of the virgin samples is totally reversible, though the initial virgin state of filler-filler bonds is not recovered. This implies that, on the one hand, the fraction of rigid filler clusters decreases with increasing pre-strain, leading to the pronounced stress softening after the first deformation cycle. On the other hand, the fraction of fragile filler clusters increases with increasing pre-strain, which impacts the filler-induced hysteresis. It is demonstrated that the quasi-static stress-strain cycles of carbon black as well as silica filled rubbers can be well described in the scope of the theoretic model of stress softening and filler-induced hysteresis up to large strain. The obtained microscopic material parameter appear reasonable, providing information on the mean size and distribution width of filler clusters, the tensile strength of filler-filler bonds, and the polymer network chain density. In particular it is shown that the model fulfils a “plausibility criterion” important for FE applications. Accordingly, any deformation mode can be predicted based solely on uniaxial stress-strain measurements, which can be carried out relatively easily. From the simulations of stress-strain cycles at small and medium strain it can be concluded that the model of anisotropic cluster breakdown and re-

82

Manfred Klppel

aggregation for pre-strained samples represents a fundamental micro-mechanical basis for the description of non-linear viscoelasticity of filler reinforced rubbers. Thereby, the mechanisms of energy storage and dissipation are traced back to the elastic response of the polymer network as well as the elasticity and fracture properties of flexible filler clusters. For a time dependent, complete characterization of non-linear viscoelastic stress-strain cycles of filler reinforced rubbers, the dynamic-mechanical response of the polymer matrix has to be considered as well. Furthermore, the re-aggregation rate must be specified in dependence of strain, in order to describe any kind of stress-strain cycles. This will be a task of future work. Acknowledgements It is a great pleasure to thank Dr. G. Heinrich (Continental AG) and Prof. R. H. Schuster (DIK) for continuous support and many inspiring discussions. Im also grateful to Dr. M. Gerspacher (Sid Richardson Carbon Co.) for the very fruitful cooperation and for providing electrical data. Helpful discussions with Prof. Th. Vilgis (MPI Mainz), Prof. E. Straube (University Halle-Wittenberg), and Prof. W. Gronski (University Freiburg) are appreciated. Special thanks are extended to Dr. A. Schrder (Freudenberg AG) and Dr. J. Schramm (Continental AG) for the fruitful cooperation during their employment at the DIK. The cooperation and friendly help of Dr. J. Meier, Dr. Th. Alshuth, Dr. H. Geisler, and Dipl. Phys. A. Mller (all DIK) is highly appreciated. Support by the Deutsche Kautschukgesellschaft e. V., the Luise Arntz Stiftung, Continental AG, Bayer AG, Columbian Chemicals Co., Sid Richardsen Carbon Co., and Degussa AG is gratefully acknowledged.

References 1. Mandelbrot BB (1977) Fractals: form, chance and dimension. WH Freeman, San Francisco 2. Mandelbrot BB (1982) The fractal geometry of nature. WH Freeman, New York 3. Meakin P (1990) Prog Solid State Chem 20:135 4. Lin MY, Lindsay HN, Weitz DA, Ball RC, Klein R (1989) Nature 339:360 5. Witten TA, Cates ME (1986) Science 232:1607 6. Bunde A, Havlin S (eds) (1991) Fractals and disordered systems. Springer, Berlin Heidelberg New York 7. Bunde A, Havlin S (eds) (1994) Fractals in science. Springer, Berlin Heidelberg New York 8. Jullien B (1990) New J Chem 14:239 9. Witten TA, Sander LM (1981) Phys Rev Lett 47:1400; Phys Rev B Condens Matter B27:5686 10. Meakin P (1984) Phys Rev A 29:997 11. Ball RC, Jullien R (1984) J Phys (Paris) Lett 45:L103 12. Meakin P (1988) Adv Colloid Interface Sci 28:249 13. Weitz DA, Oliveria M (1983) Phys Rev Lett 52:1433 14. Meakin P, Donn B, Mulholland GW (1989) Langmuir 5:510 15. Megaridis CM, Dobbins RA (1990) Combust Sci Technol 71:95 16. Samson RJ, Mulholland GW, Gentry JW (1987) Langmuir 3:272 17. Sutherland DN (1970) Nature 226:1241 18. Heinrich G, Klppel M (2001) Kautschuk Gummi Kunstst 54:159 19. Barabasi AL, Stanley HE (1996) Fractal concepts in surface growth. Cambridge University Press; Barabasi AL, Araujo M, Stanley HE (1992) Phys Rev Lett 68:3729

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

83

20. Schrder A, Klppel M, Schuster RH, Heidberg J (2001) Kautschuk Gummi Kunstst 54:260 21. Witten TA, Rubinstein M, Colby RH (1993) J Phys II (France) 3:367 22. Klppel M, Heinrich G (1995) Rubber Chem Technol 68:623 23. Klppel M, Schuster RH, Heinrich G (1997) Rubber Chem Technol 70:243 24. Heinrich G, Straube E, Helmis G (1988) Adv Polym Sci 85:33 25. Brown D (1987) PhD thesis, University of Cambridge, UK 26. Donnet JB, Bansal RC, Wang MJ (eds) (1993) Carbon black: science and technology. Marcel Decker, New York Hongkong 27. Kraus G (ed) (1965) Reinforcement of elastomers. Interscience Publ, New York London Sydney 28. Payne AR (1962) J Appl Polym Sci 6:57 29. Payne AR (1963) J Appl Polym Sci 7:873 30. Payne AR (1964) J Appl Polym Sci 8:2661 31. Payne AR (1964) Trans IRI 40:T135 32. Payne AR (1965) In: Kraus G (ed) Reinforcement of elastomers. Interscience Publ, New York London Sydney 33. Payne AR (1965) J Appl Polym Sci 9:2273,3245 34. Payne AR (1972) J Appl Polym Sci 16:1191 35. Payne AR (1963) Rubber Chem Technol 36:432 36. Medalia AI (1973) Rubber Chem Technol 46:877 37. Medalia AI (1974) Rubber Chem Technol 47:411 38. Voet A, Cook FR (1967) Rubber Chem Technol 40:1364 39. Voet A, Cook FR (1968) Rubber Chem Technol 41:1215 40. Dutta NK, Tripathy DK (1989) Kautschuk Gummi Kunstst 42:665 41. Dutta NK, Tripathy DK (1992) J Appl Polym Sci 44:1635 42. Dutta NK, Tripathy DK (1990) Polym Test 9:3 43. Ulmer JD, Hergenrother WL, Lawson DF (1998) Rubber Chem Technol 71:637 44. Wang MJ, Patterson WJ, Ouyang GB (1998) Kautschuk Gummi Kunstst 51:106 45. Freund B, Niedermeier W (1998) Kautschuk Gummi Kunstst 51:444 46. Mukhopadhyay K, Tripathy DK (1992) J Elastomers Plast 24:203 47. Wang MJ (1998) Rubber Chem Technol 71:520 48. Bischoff A, Klppel M, Schuster RH (1998) Polym Bull 40:283 49. Vieweg S, Unger R, Heinrich G, Donth E (1999) J Appl Polym Sci 73:495 50. Payne AR, Watson WF (1963) Rubber Chem Technol 36:147 51. Amari T, Mesugi K, Suzuki H (1997) Prog Org Coat 31:171 52. Payne AR, Wittaker RE (1970) Rheol Acta 9:91 53. Payne AR, Wittaker RE (1970) Rheol Acta 9:97 54. Kraus G (1984) J Appl Polym Sci Appl Polym Symp 39:75 55. van de Walle A, Tricot C, Gerspacher M (1996) Kautsch Gummi Kunstst 49:173 56. Lin CR, Lee YD (1996) Macromol Theory Simul 5:1075; (1997) Macromol Theory Simul 6:102 57. Heinrich G, Klppel M (2002) Adv Polym Sci 160:1 58. Mullins L (1948) Rubber Chem Technol 21:281 59. Mullins L, Tobin RN (1957) Rubber Chem Technol 30:355 60. Mullins L (1965) In: Kraus G (ed) Reinforcement of elastomers,. Interscience Publ, New York London Sydney 61. Medalia AI (1978) Rubber Chem Technol 51:437 62. Edwards SF, Vilgis TA (1988) Rep Prog Phys 51:243; (1986) Polymer 27:483 63. Guth E, Gold O (1938) Phys Rev 53:322 64. Huber G (1997) PhD thesis, University of Mainz, Germany 65. Huber G, Vilgis TA (1998) Euro Phys J B3:217; (1999) Kautschuk Gummi Kunstst 52:102 66. Heinrich G, Vilgis TA (1993) Macromolecules 26:1109 67. Eisele U, Mller HK (1990) Kautschuk Gummi Kunstst 43:9 68. Bueche F (1960) J Appl Polym Sci 4:107; (1961) J Appl Polym Sci 5:271

84 69. 70. 71. 72. 73. 74. 75. 76. 77. 78. 79. 80. 81. 82. 83. 84. 85. 86. 87. 88. 89. 90. 91. 92. 93. 94. 95. 96. 97. 98. 99. 100. 101. 102. 103. 104. 105. 106. 107. 108. 109. 110. 111.

Manfred Klppel Govindjee S, Simo J (1991) J Mech Phys Solids 39:87; (1992) J Mech Phys Solids 40:213 Dannenberg EM (1974) Rubber Chem Technol 47:410 Rigbi Z (1980) Adv Polym Sci 36:21 Hamed GR, Hatfield S (1989) Rubber Chem Technol 62:143 Haarwood JA, Mullins L, Payne AR (1965) J Appl Polym Sci 9:3011 Haarwood JA, Payne AR (1966) J Appl Polym Sci 10:315, 1203 Klppel M, Schramm J (1999) In: Dorfmann A, Muhr A (eds.) Constitutive models for rubber. Balkema, Rotterdam, p 211 Klppel M, Schramm J (2000) Macromol Theory Simul 9:742 Kaliske M, Heinrich G (1999) Rubber Chem Technol 72:602 Heinrich G, Kaliske M (1997) Comput Theor Polym Sci 7:227 Schrder A (2000) PhD thesis, University of Hannover, Germany Schrder A, Klppel M, Schuster RH (1999) Kautschuk Gummi Kunstst 52:814 Schrder A, Klppel M, Schuster RH (2000) Kautschuk Gummi Kunstst 53:257 Schrder A, Klppel M, Schuster RH, Heidberg J (2002) Carbon 40:207 Klppel M, Schrder A, Schuster RH, Schramm J (2000) Paper No XLI, ACS Rubber Division Meeting, Dallas, USA Klppel M, Schrder A, Heinrich G, Schuster RH, Heidberg J (2000) Proceedings: Kautschuk-Herbst-Kolloquium, Hannover, Germany, p 193 Schuster RH, Klppel M, Schramm J, Heinrich G (1998) Paper No 56, ACS Rubber Division Meeting, Indianapolis, USA Klppel M, Schuster RH, Schaper J (1999) Rubber Chem Technol 72:91 Schuster RH, Meier J, Klppel M (2000) Kautschuk Gummi Kunstst 53:663 Schuster RH, Klppel M, Frh T (1997) Paper No 53, ACS Rubber Division Meeting, Anaheim, USA Klppel M, Meier J (2001) In: Besdo D, Schuster RH, Ihlemann J (eds.) Constitutive models for rubber II. Balkema, Lisse Abingdon Exton Tokyo, p 11 Raab H, Frhlich J, Gritz D (2000) Kautschuk Gummi Kunstst 53:137 Niedermeier W, Stierstorfer J, Kreitmeier S, Metz O, Gritz D (1994) Rubber Chem Technol 67:148 Niedermeier W, Raab H, Stierstorfer J, Kreitmeier S, Gritz D (1994) Kautschuk Gummi Kunstst 47:799 Hjelm RP, Wampler WA, Serger PA (1991) Paper No 5, ACS Rubber Division Meeting, Toronto, Canada Rieker TP, Misono S, Ehrenbourger-Dolle F (1999) Langmuir 15:914 Rieker TP, Hindermann-Bischoff M, Ehrenbourger-Dolle F (2000) Landmuir 16:5588 Frhlich J, Kreitmeier S, Gritz D (1998) Kautschuk Gummi Kunstst 51:370 Zerda TW, Yang H, Gerspacher M (1992) Rubber Chem Technol 65:130 Isamail JMK, Pfeifer P (1994) Langmuir 10:1532 Isamail JMK (1992) Langmuir 8:360 Pfeifer P, Obert M, Cole MW (1989) Proc R Soc Lond A423:169 Pfeifer P, Cole MW (1990) New J Chem 14:221 Lippens BC, Linsen BG, De Boer JH (1964) J Catalysis 3:32 Adamson AW, Ling L (1961) Adv Chem 33:51 Langmuir I (1918) J Am Chem Soc 40:1316. Fowler RH, Guggenheim EA (1952) Statistical thermodynamics. Cambridge University Press, Cambridge, UK Douglas JF (1989) Macromolecules 22:3707 Vilgis TA, Heinrich G (1994) Macromolecules 27:7846 Herd CR, McDonald GC, Hess WM (1992) Rubber Chem Technol 65:107 Gerspacher M, OFarrell CP (1992) Kautschuk Gummi Kunstst 45:97 Le Mehaute A, Gerspacher M, Tricot C (1993) In: Donnet JB, Bansal RC, Wang MJ (eds) Carbon black: science and technology. Marcel Decker, New York Hongkong, p 245 Medalia AI (1967) J Colloid Interface Sci 24:393

The Role of Disorder in Filler Reinforcement of Elastomers on Various Length Scales

112. 113. 114. 115. 116. 117. 118. 119. 120. 121. 122. 123. 124. 125. 126. 127. 128. 129. 130. 131. 132. 133. 134. 135. 136. 137. 138. 139. 140. 141. 142. 143. 144. 145. 146. 147. 148. 149. 150. 151. 152. 153.

85

Medalia AI, Heckman FA (1996) Carbon 7:567 Viswanathan R, Heaney MB (1995) Phys Rev Lett 75:4433 Ehrburger-Dolle F, Tence M (1990) Carbon 28:448 Oppermann B (1994) PhD thesis, University of Hannover, Germany Heckman FA, Medalia AI (1969) J Inst Rubber Ind 3:66 Hess WM, Chirico VE, Burgess KA (1973) Proceedings: International Rubber Conference, Prague, CR Gessler M (1970) Rubber Chem Technol 43:943 Sgodzaj U (2001) PhD thesis, University of Karlsruhe, Germany Jger KM, McQueen DH (2001) Polymer 42:9575 Medalia AI (1986) Rubber Chem Technol 59:432 Boettger H, Bryksin UV (1986) Hopping conduction in solids. Verlag Akademie, Berlin Miyasaka K (1985) Nippon Gomu Kyokaishi 58:561 OFarrell CP, Gerspacher M, Nikiel L (2000) Kautschuk Gummi Kunstst 53:701 Probst N, Grivei E (2000) Proceedings: Kautschuk-Herbst-Kolloquium, Hannover, Germany, p 205 Balberg I (1998) Trends Stat Phys 2:39; (1987) Phys Rev Lett 59:1305 Rubin Z, Sunshine A, Heaney MB, Bloom I, Balberg I (1999) Phys Rev B59:12,196 Stauffer D, Aharoni A (1992) Introduction to percolation theory. Taylor and Francis, London Ayala JA, Hess WM, Dotson AO, Joyce GA (1990) Rubber Chem Technol 63:747 Hess WM, Chirico VE (1975) Proceedings: Plast Rubber Inst 1st Eur Conf, Brussels, Belgum van Beek LKH (1967) In: Birks JB (ed.) Progress in dielectrics. vol 7. Heywood, London, p. 69 Ouyang GB (2000) Proceedings: Kautschuk-Herbst-Kolloquium, Hannover, Germany, p 183 Schwartz G, Cerveny S, Marzocca AJ (2000) Polymer 41:6589 Kremer F, Ezquerra TA, Mohamadi M, Bauhofer W, Vilgis TA, Wegner G (1988) Solid State Commun 66:153 Jger KM, McQueen DH, Tchmutin IA, Ryvtina NG, Klppel M (2001) J Phys D Appl Phys 34:2699 Gefen Y, Aharony A, Alexander S (1983) Phys Rev Lett 50:77 Havlin S, Bunde A (1991) In: Bunde A, Havlin S (eds) Fractals and disordered systems. Springer, Berlin Heidelberg New York, p 115 Kastner A, Alig I, Heinrich G, Klppel M (In preparation) Klppel M (1997) Kautschuk Gummi Kunstst 50:282 Georg G, Bhm A, Nguyen M (1995) J Appl Polym Sci 55:1041 Frhlich J, Niedermeier W (2000) Proceedings: German Rubber Conference, Nrnberg, Germany, p 107 Frhlich J, Luginsland HD (2000) Proceedings: Kautschuk-Herbst-Kolloquium, Hannover, Germany, p 13 Wang T, Wang MJ, Shell J, Tokita N (2000) Kautschuk Gummi Kunstst 53:497 Schuster RH (1989) Verstrkung von Elastomeren durch Ruß, WDK-Grnes Buch Nr 40 Cotten GR (1975) Rubber Chem Technol 48:548 Kraus G, Gruver JT (1968) Rubber Chem Technol 41:1256 Meissner B (1974) J Appl Polym Sci 18:2483 Brennan JJ, Jermyn TE, Boonstra BB (1965) Gummi Asbest Kunstst 18:266 Boonstra BB (1967) J Appl Polym Sci 11:389 Sircar AK, Voet A (1970) Rubber Chem Technol 43:973 Wolff S, Wang MJ, Tan EH (1993) Rubber Chem Technol 66:163 Chapman AV, Fulton WS, Tinker AJ (2000) Proceedings: Kautschuk-Herbst-Kolloquium, Hannover, Germany, p 23 Kida N, Ito M, Yatsunyanagi F, Kaido H (1996) J Appl Polym Sci 61:1345

86 154. 155. 156. 157. 158. 159. 160. 161. 162. 163. 164. 165. 166. 167. 168. 169. 170. 171. 172. 173. 174. 175. 176. 177.

Manfred Klppel Sircar AK, Lamond TG (1975) Rubber Chem Technol 48:79, 89 Kantor Y, Webman I (1984) Phys Rev Lett 52:1891 Friedlander SK, Jang HD, Ryu KH (1998) Appl Phys Lett 72:173 Friedlander SK, Ogawa K, Ullmann M (2001) J Polym Sci Polym Phys 38:2658 Mller M (2002) PhD thesis, University of Hannover, Germany Mller M, Schuster RH (2000) Proceedings: German Rubber Conference, Nrnberg, Germany, p 77 Tschoegl NW (1989) The phenomenological theory of linear viscoelastic behavior. Springer, Berlin Heidelberg New York van Dongen PGJ, Ernst MH (1985) Phys Rev Lett 54:1396; (1985) J Phys A18:2779 Ziff RM, McGrady ED, Meakin P (1985) J Chem Phys 82:5269 Heinrich G, Straube E (1984) Acta Polym 35:115 Heinrich G, Straube E (1987) Polym Bull 17:247 Rubinstein M, Panyukow S (1997) Macromolecules 30:8036 Straube E, Urban V, Pyckhout-Hintzen W, Richter D, Glinka CW (1995) Phys Rev Lett 74:4464 Klppel M (1994) Macromolecules 27:7179 Klppel M, Menge H, Schmidt H, Schneider H, Schuster RH (2001) Macromolecules 34:8107 Edwards SF, Vilgis TA (1988) Rep Prog Phys 51:243; (1986) Polymer 27:483 Klppel M, Heinrich G (1994) Macromolecules 27:3569 Fetters LJ, Lohse DJ, Richter D, Witten TA, Zirkel A (1994) Macromolecules 27:4639 Klppel M (1992) Prog Colloid Polym Sci 90:137 Klppel M (1993) J Appl Polym Sci 48:1137 Meier J (2002) PhD thesis, Technical University of Clausthal, Germany Meier J, Giebeler E, Klppel M, Schuster RH (2001) Paper No. XX, ACS Rubber Division Meeting, Provicence, USA Brown JD (1997) PhD thesis, Rensselaer Polytechnic Institute, Troy, New York, USA Chazeau L, Brown JD, Yanyo LC, Sternstein SS (2000) Polym Compos 21:202

Adv Polym Sci (2003) 164:87–210 DOI 10.1007/b11055

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM) and their Application to Polymers and Polymer Composites Martin Munz · Brunero Cappella · Heinz Sturm · Markus Geuss · Eckhard Schulz Federal Institute for Materials Research and Testing (BAM), Unter den Eichen 87, 12205 Berlin, Germany E-mail: [email protected] Abstract Beyond measuring the topography of surfaces, scanning force microscopy (SFM) has proved to be valuable both for mapping of various materials properties and for modifying surfaces via lithography techniques. Thus, SFM has gained relevance as a surface analysis technique as well as a tool for nanoscale engineering purposes. Different kinds of tipsample interactions are exploitable, e.g. mechanical, thermal and electrical ones. Owing to its versatility, SFM has found plenty of applications in polymer science. Among others, the examples reported on in this review article encompass issues related to commodity polymers, various polymer-based composites, polymer blends, or ferroelectric polymers. For instance, stiffness imaging is elucidated as a technique for detecting interphases occurring in composites with inorganic fillers. The described applications are mainly related to mechanical and electrical tip-sample interactions. The respective fundamentals are outlined as well as some aspects of the measurement of materials contrasts. The presented techniques of nano-scale modification are a dynamical sort of plowing lithography and electrical poling, both performed by means of SFM-probes. Keywords Contact mechanics · Electrical properties · Interface/interphase · Nanolithography · Polymer-matrix composites (PMC) · Scanning/atomic force microscopy (SFM/AFM) · Thermal diffusivity

1

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

93

2

Fundamentals of Scanning Probe Microscopy and Basic Instrumentation . . . . . . . . . . . . . . . . . . . . . . . . .

96

3

Nanomechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 105

3.1 3.1.1 3.1.2 3.1.3 3.1.4

Fundamentals of Tip-Sample Interactions Normal Loading . . . . . . . . . . . . . . . . . Micro-Indentation Testing . . . . . . . . . . Shear Loading . . . . . . . . . . . . . . . . . . Sliding Friction . . . . . . . . . . . . . . . . .

4

Stiffness Mapping for the Characterisation of Heterogeneous Polymer Systems . . . . . . . . . . . . . . . . . . . . 121

4.1

Characterisation of Crosslinked Polymer Films. . . . . . . . . . . . . 121

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

107 107 112 115 117

Springer-Verlag Berlin Heidelberg 2003

88

Martin Munz et al.

4.2

Constant Dynamic Indentation Mode (CDIM) as Demonstrated on a PS/PMMA Composite Sample. . . . . . . . . . . . . . . . . . . . . 4.3 Imaging the Surface Layer of Injection-Moulded Polymer Parts . . 4.4 The Sub-Macroscopic Diffusional Profile of OsO4 in Polyamide6 (PA6) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5 Interphases in Polymer Based Composites. . . . . . . . . . . . . . . . 4.5.1 The Mesoscopic Stiffness Profile Characterising the Interphase Between Copper(oxide) and Amine-Cured Epoxy . 4.5.2 The Microscopic Stiffness Profile Characterising the Interphase Between C-Fibres and Polyphenylenesulfide (PPS) 4.5.3 Discussion of the Detected Stiffness Profiles . . . . . . . . . . . . . .

122 124 126 128 129 137 141

5

Mapping of Mechanical and Thermal Properties of a Model Brake Pad . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 145

5.1 5.2

Combined Measurement of Friction and Stiffness on a Model Brake Pad . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 145 Thermal Diffusivity Measurements on a Model Brake Pad. . . . . . 149

6

Nanolithography . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 152

6.1 6.2 6.2.1 6.2.2 6.2.3 6.3

Mechanical Lithography on Polymer Surfaces . . . . . Dynamic Plowing Lithography . . . . . . . . . . . . . . . State of the Art . . . . . . . . . . . . . . . . . . . . . . . . . Experimental . . . . . . . . . . . . . . . . . . . . . . . . . . . Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Force-Displacement Curves and Force-Displacement Curves Indentation (FDI) . . . . . . . . . . . . . . . . . . . 6.3.1 State of the Art . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.2 Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Insights into the Process of Surface Modification . . . 7 7.1 7.2 7.3 7.4 7.4.1 7.4.2 7.4.3 7.4.4 7.4.5 7.4.6

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

152 153 153 154 154

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

160 160 160 163

Materials Contrasts of Electric Properties. . . . . . . . . . . . . . . . 169

Motivation and Introduction . . . . . . . . . . . . . . . . . . . . . . . . Literature Overview . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Technical Aspects and Technological Problems. . . . . . . . . . . . . A.C. Conductivity in the SFM Contact Mode . . . . . . . . . . . . . . Graphite . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Electrically Conductive Ion Tracks . . . . . . . . . . . . . . . . . . . . . Carbon Fibre Surfaces . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Polyaniline, a Conductive Polymer. . . . . . . . . . . . . . . . . . . . . Plasma Polymerized Iodothiophene . . . . . . . . . . . . . . . . . . . . Barium Tetratitanate and Yttrium Doped Barium Titanate: A Partially Conductive and a Partially Semiconductive Ceramic. . 7.5 Materials Contrasts in the SFM Non-Contact Mode . . . . . . . . . . 7.5.1 Industrial Polypropylene with Two Different Technical Additives . 7.5.2 Surface Charges on a Polymer Electret . . . . . . . . . . . . . . . . . . 7.5.3 Dewetting of an Incompatible Polymer Blend on a Gold Surface: Polyacryl-co-Styrene and Polybutadiene . . . . . . . . . . . . . . . . .

169 170 174 176 177 177 179 181 181 182 185 186 186 187

89

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

7.5.4 Liquid Crystalline Polysiloxane: Surfaces and Edges of a Smectic Layered Ferroelectric . . . . . . . . . . . . . . . . . . . . . 7.6 Piezoresponse Force Microscopy (PFM) . . . . . . . . . . . . . . . . . 7.6.1 Polarising Small Domains in Ferroelectric Polymer Films . . . . . . 7.6.2 Domain Growth Kinetics and Piezoelectric Hysteresis for Thin P(VDF-co-TrFE) Films . . . . . . . . . . . . . . . . . . . . . . . 7.6.3 Poling DPL Fabricated Sub-m Ferroelectric Polymer Structures . 8

188 190 192 193 195

Concluding Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 196

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 199

List of Abbreviations and Symbols ABS AFAM AFM ATR CDIM CFRP CPM c-SFM DC-EFM DGEBA DLC DMA DMT DPL EBL EDX EFM EP ESEM FDI FEP FFM FMM HIPS HM HOPG IRRAS JKR LB MALDI-MS

Poly(acryl-co-styrene)/polybutadiene blend Atomic force acoustic microscopy Atomic force microscopy Attenuated total reflectance infrared spectroscopy Constant dynamic indentation mode Carbon fibre reinforced polymers Colloidal probe microscopy Conductivity SFM Dynamic contact mode electrical force microscopy Diglycidylether of bisphenol-A Diamond-like carbon Dynamic-mechanical analysis Derjaguin-Muller-Toporow model Dynamic plowing lithography Electron beam lithography Energy dispersive X-ray analysis Electrostatic force microscopy Ethylene-propylene Environmental scanning electron microscope Force-distance curve indentation Fluoroethylenepropylene Friction force microscopy Force modulation microscopy High-impact polystyrene High modulus Highly oriented pyrolitic graphite Infrared-reflection-absorption spectroscopy Johnson-Kendall-Roberts model Langmuir-Blodgett Matrix-assisted laser desorption/ionisation mass spectrometry

90

M-D MD MEMS M-LFM MPDA MWNT oLED P(VDF-TrFE) PAN PBD PE PFM PMC PMMA PP PPS PR PS PVDF PVE SAM SCM SEM SFA SFM SK(F)M SLAM SNOM SPM SSPM SSRM SThM STM TEI TEM TGS TM TPE UFM UHV UV VM-SFM VUV XPS a

Martin Munz et al.

Maugis-Dugdale model Molecular-dynamics Micro-electro-mechanical systems Modulated lateral force microscopy Metaphenylenediamine Multiwall carbon nanotube Organic light emitting diodes Polyvinylidenefluoride/trifluorethylene Polyacrylonitrile Polybutadiene Polyethylene Pulsed force mode Polymer matrix composites Polymethylmethacrylate Polypropylene Polyphenylenesulfide Phenolic resin Polystyrene Polyvinylidenedifluoride Polyvinylethylene Self-assembled monolayers Scanning capacitance microscopy Scanning electron microscopy Surface force apparatus Scanning force microscopy Scanning Kelvin (force) microscopy Scanning local-acceleration microscopy Scanning near field optical microscopy Scanning probe microscopy Scanning surface potential microscopy Scanning spreading resistance microscopy Scanning thermal microscopy Scanning tunnelling microscopy Thermoelastic instability Transmission electron microscopy Triglycine sulfate Tapping mode Thermoplastic elastomeric materials Ultrasonic force microscopy Ultra high vacuum Ultraviolet Voltage modulated SFM Vacuum-ultraviolet X-ray photoelectron spectroscopy Contact radius

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

A Ad Ae Ai(h) Ao Ap Ar Aw Arf Awf b bdyn B c cth C gc d d33 D DDPL, DFDI Dn(N) Dth DT d ddyn dx g E Ec Eel e fscan F Fkfr Fsfr F G G* h hr H H(t) kc

Contact area Domain area Recovered work; work of elastic deformation Indenter area function Minimum domain area Dissipated work; work of plastic deformation; hysteresis of the contact lines “Reading” oscillation amplitude “Writing” oscillation amplitude “Reading” free oscillation amplitude “Writing” free oscillation amplitude Effective radius of contact Bending amplitude Amplitude of the oscillations Concentration Specific heat capacity Charge capacity Critical shear strength Width of the dead zone of the interface height step Converse piezoelectric constant Dielectric displacement Depth of the holes in DPL and in FDI, respectively Profile of the network structure of the thermoset Penetration depth of the thermal wave Diffusion coefficient Deformation Deformation amplitude Lateral displacement Surface energy Youngs modulus Coercitive field Electrical field Dielectric constant Scan rate Force Kinetic friction force Static friction force Phase Shear modulus Reduced shear modulus Penetration depth Remaining plastic deformation at zero load Hardness Relaxation-time spectrum Elastic constant of the cantilever

91

92

keff kts klatts K jw J I IC IT L l lth M33 n p P Pad Pdyn Pel Prel Psel Psatel Q Q33 Qx r r1 r2 R S Sbp Sw SH sc td tr T TC TG t U V Vneg Vpos

Martin Munz et al.

Effective force constant Stiffness of the contact Lateral stiffness of the tip-sample contact Reduced elastic modulus Heat current density Creep compliance Electrical current Electrical current via mechanical contact Electrical tunnelling current Scan velocity Maugis parameter Thermal conductivity Electric field dependent electrostrictive constant Friction coefficient Poisson ratio Contact pressure External load Adhesion force Force amplitude in force-modulation mode Electrical polarisation Remanent polarisation Spontaneous polarisation Saturation polarisation Exothermic reaction heat Polarisation dependent electrostrictive constant Lateral force Mass density Radius of curvature of the liquid meniscus Radius of the liquid bridge Radius of curvature of the tip Stiffness Bulk polymer stiffness Amount of stiffness change at the position N=N0 Side of the hole Yield stress Characteristic time of diffusion Characteristic time of the crosslinking reaction Temperature Curie temperature Glass temperature Characteristic response time Voltage Crack propagation velocity Volume of the hole Volume of the border-wall

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

Vr Vw vscan W w yv zdyn z w wres

93

“Reading” voltage amplitude “Writing” voltage amplitude Scan velocity W idth of the hole Adhesion energy per unit area Plasticity factor Modulation amplitude Thermal conductance Frequency Resonance frequency of the cantilever

1 Introduction In scanning force microscopy (SFM) [1] microscopic cantilevers with a sharp tip positioned close to the free end of the cantilever are employed. Alongside with the piezoelectric transducers for high-resolution movement, the cantilever represents one of the core elements of microscopes of the SFM type. If not consisting of silicon nitride (Si3N4), which is an insulating ceramic, in the vast majority of cases these cantilevers consist of silicon, which belongs to the class of semiconducting materials. Hence, when investigating surfaces of macromolecular materials by means of SFM, two different classes of materials are involved, namely polymers and inorganic semiconductors. Undoubtedly, these materials are ever-present in our daily lives and are playing more and more an increasing role. Among others, their great success can be traced back to a common trait, namely a kind of versatility, that is the potential of a material to exhibit wide ranges of different properties which are accessible technically by dedicated but similar fabrication techniques and which can be exploited for manifold applications. For instance, in the case of semiconductors the electrical and optical properties can easily be changed by means of doping techniques. Similarly, the stiffness for tensile loading of polymers can be enhanced significantly by techniques such as blending of two or more polymers complementing one another in their mechanical properties or by stretching. Moreover, electrical and optical properties of polymer materials are increasingly being studied and are paving the way for polymers to be used as active elements, such as organic light emitting diodes (oLED). One trait that obviously seems to be common to the two materials classes, i.e. polymers and semiconductors, as well as to the microscopy technique SFM, is versatility. That is, without significant changes to the basic experimental set-up of the SFM type microscope, many different properties of the surface under investigation can be measured and recorded in the form of an image. Consequently, based on the SFM principle, plenty of different measurement techniques have been developed and have largely driven the widespread dissemination of SFM-type microscopes one may find nowadays in many research labs. Re-

94

Martin Munz et al.

ferring to the various existing modifications of the SFM principle as well as to some techniques where microscopic probes are being employed which are completely different from the cantilevers typical for SFM (namely in scanning tunnelling microscopy, STM [2], and often also in scanning near-field optical microscopy SNOM [3]), the more general term scanning probe microscopy (SPM) has been coined. In the particular case of an SFM-type microscope, the probe consists of a cantilever and a tip. Essentially, the versatility of SFM results from the numerous tip-sample interactions which can be exploited for characterising the surface under investigation. For instance, when operating in immediate mechanical contact between tip and sample and when having applied an electrical voltage between an electrically conductive cantilever and an electrode at the backside of the sample, the current flowing across the tip-sample contact may be used for mapping variations of the electrical conductivity. In an analogue manner, variations of the thermal conductivity of the surface under investigation may be mapped. Whatever the particular set-up, material of the tip surface, and sample material, the force acting between tip and sample can be used for controlling the tip-sample distance. Simultaneously, other interactions such as the electrical tip-sample current can be recorded and used for characterising the sample surface. These kind of imaging techniques reflecting the lateral variations of a particular physical property are often referred to as materials contrasts. They may be used for contrasting different components, differing in their composition or their structure. Similarly, a materials contrast may be used for mapping changes of the measured physical quantity as occurring along a certain direction, but within the same material. Obviously, careful interpretation of the gathered materials contrast requires some knowledge on the tip-sample interaction being exploited. Owing to the operation of the tip in the near-field of the sample, that is within rather small a distance from the sample surface (<100 nm), the magnitude of the effective tip-sample interaction area is affected generally by the surface topography. Consequently, the potential cross-talk from topography via the tip-sample interaction area should always be borne in mind when analysing materials contrast images. The ability to characterise various physical properties on a highly local scale may provide valuable information not available by means of more conventional microscopy techniques. Whatever the particular issue why a (macromolecular) material is being investigated, imaging its structure is in many cases a straightforward approach and may provide plenty of information on its morphology, texture, the effects of the particular production technique, or the mechanism of failure of a part made up of that material. Structureproperty relationships are being studied widely in order to learn how to deduce materials properties from the materials structure, and in what ways the materials properties may be improved by well-aimed modifications to the materials structure. Alongside with the spatial organisation of a material, compositional heterogeneities are being present in most materials and can play a major role for certain properties such as the mechanical strength. Consequently, sampling of concentration profiles or concentration mapping

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

95

are valuable techniques in materials science. The required spatial resolution can be provided by scanning a focused probe across the area under investigation, e.g. like in scanning electron microscopy (SEM). Since compositional heterogeneities are in many cases related to corresponding variations in local physical properties, the recorded concentration profiles can be translated into property profiles provided that some knowledge of the respective concentration-property-relationship is given. For instance, this knowledge can be gathered from reference measurements performed on materials with a well-defined chemical composition, so-called reference materials. If performing the reference measurements by means of a macroscopic measurement technique, however, it should be borne in mind that the resulting macroscopic concentration-property-relationship does not hold necessarily on the length scale of the concentration gradient of interest. For instance, the macroscopic tensional strength of a material may be impaired significantly by the presence of mesoscopic flaws such as voids, whereas on the local scale the probability of finding flaws within the sampling volume is reduced and the tensional strength can be enhanced. Hence, microscopic measurements are highly desirable which provide information on the physical property of immediate interest. For instance, when dealing with fibre-reinforced composites, in general, there exists an interphase present between fibre and matrix with mechanical properties deviating from those of the bulk matrix and of the bulk filler material, respectively. The shape of the corresponding radial stiffness profile shows some impact on the stress distribution occurring around the fibre and, hence, on the overall mechanical performance of the composite material [4]. The stiffness profile may arise either from corresponding gradients of the composition or from structural gradients. Instead of profiling these variations and translating them into a stiffness profile by means of reference data or a model, it seems to be more straightforward to map the stiffness variations themselves. Several examples of stiffness mapping as applied to heterogeneous polymer systems are given in Sect. 4. An application of thermal and combined mechanical SFM measurements as performed on a polymer-matrix composite referring to brake pad materials is be elucidated in Sect. 5. The potential benefits which can be taken from electrical materials contrasts as well as particular measurement techniques and their limits are described in Sect. 7. Rather than aiming to sampling the sample surface in a non-destructive manner, the directness of the tip-sample interactions may be exploited deliberately for modifying the sample surface. Thus, by addressing particular tip-sample interactions promising for inducing surface modifications and by variation of the strength of the tip-sample interaction, the transition from reading to writing can be made. This capability has opened up new routes towards manipulation of materials on the nanoscale. Alongside with the need for small-scale lithography, this potential capability of SPM-based techniques has propelled a now world-wide rush into nanotechnology. Beyond the new tools for nanoscale modification of materials, operation of the SFM in the writing regime may be used for studying the high-strain behaviour

96

Martin Munz et al.

of polymers on a highly local scale. As, in general, physical laws holding on the macroscale are implying some statistics, simple scaling down to sampling volumes encompassing only a small number of molecules may lead to erroneous results. Small is different and promising materials properties may be expected on the nanoscale. Moreover, when considering future information storage technologies based on nanoscale modifications of polymer surfaces [5], issues related to the long-term stability of the nanostructures seem to be of paramount interest. In general, it may be stated that the functionality of polymers is being extended to micro- and nanoscale. These kinds of approaches are expected to open up new ways to micro- or nanoscale devices and their future employment will increase even further the present degree of versatility of macromolecular materials. An SFM based lithography technique by means of mechanical interactions as applied to surfaces of polystyrene (PS) and polymethylmethacrylate (PMMA) is described in Sect. 6. Similarly, some results of SFM-based poling experiments performed on a piezoelectric polymer are elucidated in Sect. 7.6. In the following Sects. 2 and 3 some fundamentals of SFM are outlined as well as some basics of nanomechanics relevant to tip-sample interactions, respectively.

2 Fundamentals of Scanning Probe Microscopy and Basic Instrumentation The general principle of scanning probe microscopy (SPM) is to scan a very sharp probe over the surface under investigation. With probe and sample being so close to each other that their mutual interaction occurs via the near-field instead of the far-field, the tip-sample interaction is very local and a high lateral resolution can be achieved. In fact, atomic resolution was accomplished by means of scanning tunnelling microscopy (STM) and scanning force microscopy (SFM) on metals and ionic crystals. Depending on the particular tip-sample interaction being employed, different physical properties of the sample surface can be mapped. In the case of STM, the current tunnelling between a sharpened metal wire and the electrically conductive sample is measured. Owing to the pronounced distance dependence of the tunnelling current, an extraordinary sensitivity for tip-sample distance changes is given. Provided a finely adjustable actuator for movements in direction vertical to the sample surface, the vertical probe position can be adapted to the topography of the sample surface by using the magnitude of the tunnelling current as control variable of a feedback loop. When scanning the STM probe across the sample surface a topographic map can be recorded with the vertical displacements of the probe representing the height changes of the sample surface. In a similar manner to STM, in SFM the mechanical forces acting between a sharp tip and the sample surface are being exploited for recording topography images. Owing to the ever-present van der Waals forces, SFM measurements can be performed on arbitrary materials without special requirements for electrical conductivity. The total tip-

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

97

sample interaction may also include other forces such as electrostatic or magnetic ones, or solvation forces. The force sensitivity is achieved by means of a microscopic cantilever the tip is attached to. Usually, the bending of the cantilever upon attractive or repulsive tip-sample forces is sensed by means of laser beam reflected off the rear side of the cantilever. The angle of reflection of the focused laser beam changes with the bending of the cantilever. A segmented photodiode may be used for detecting the position changes of the reflected laser beam. Depending on the geometrical and electronic amplification of this detection scheme, which is adapted from the operation principle of a light pointer, a vertical resolution of the order of ~0.01 can be achieved. In a similar manner, the torsional flexure of the cantilever due to lateral forces acting on the tip can be detected. This requires sensitivity of the photodiode for positional shifts of the reflected laser beam along a second axis aligned perpendicular to the first one. Hence, fourfold segmented photodiodes are often used for accomplishing that. Beyond imaging the sample topography, the SFM set-up can be exploited for imaging further sample properties, such as local stiffness, adhesion, friction, or thermal conductivity. In principle, information related to the mechanical properties of the tip-sample contact are accessible without special modifications of the cantilever. The force changes upon approaching the cantilever to the sample surface and the subsequent retracting are generally recorded in the form of force-distance curves and can provide a wealth of information about the particular tip-sample interactions and the mechanical properties of the tip-sample contact [6]. Measuring and analysing force-distance curves is a specialised field and discussing the details is beyond the scope of this article. Essentially, the force-distance curve encompasses an attractive range including the jump-to-contact in the approaching part, a nonlinear repulsive range in both the approaching and the retracting part, and a pull-off range in the retracting part. Special-purpose set-ups were devised for probing specific tip-sample interactions like electric, magnetic, thermal or optical ones. The basic set-up of SFM microscopes is depicted in Fig. 1a. The cantilever is scanned across the surface along lines parallel to the x-axis (axis of fast scanning). Successive scan lines are shifted along the y-axis (axis of slow scanning). Usually, the axis of fast scanning is chosen perpendicular to the length axis of the cantilever. The scan range may range from some nanometres to some tens of micrometres. The tip-sample interaction can be sensed in contact, in intermittent contact, or in non-contact mode. In contact mode the tip touches the sample surface permanently and the overall force on the tip is repulsive. The resulting bending of the cantilever is concave. The repulsive tip-sample interaction changes fast with penetration depth which allows a high z-resolution. During scanning lateral forces act between tip and sample, either due to shear deformation of the tip-sample contact or due to frictional forces. Both of them can be a matter of interest, but the shear forces can result in some modification of the sample surface. In non-contact mode no intimate contact between tip and sample is established but the tip is close enough to the sample surface to sense the vertical gradient of surface

98

Martin Munz et al.

Fig. 1 a Schematic representation of the basic components of a standard SFM detection system. The sample surface under investigation is scanned by means of a very fine tip which is located near the free end of a microscopic cantilever. The vertical forces acting between tip and surface result in a bending of the cantilever which is detected by means of an optical detection system strongly resembling a light pointer. b According to the regime of the force-distance curve where the tip is operated during imaging, three basic operation modes can be distinguished. In non-contact and in intermittent contact operation, the vertical cantilever position is subjected to a periodical displacement modulation with a frequency close to the resonance frequency of the cantilever. In non-contact mode the tip is moving solely in the regime of purely attractive forces, whereas in contact mode the tip-surface forces are repulsive. In intermittent contact mode during each modulation period the tip senses both attractive and repulsive forces with the time of repulsive interaction being only a fraction of the modulation period

forces. The stiffness of the free cantilever is diminished by the vertical gradient of attractive surface forces. The corresponding reduction of the resonance frequency of the cantilever can be exploited for driving the topography feedback. In intermittent contact mode the tip moves both in the attractive and the repulsive regime of the force-distance curve. At the lower point of the vertical displacement modulation of the cantilever base the tip touches the sample surface. In a more figurative way, this mode is also referred to as tapping mode (TM). Pulling-off the tip from the adhesive surface requires a certain minimum amplitude of displacement modulation. The closer the cantilever approaches the sample surface, the more its oscillation amplitude is diminished. Thus, the amplitude signal is generally exploited as input variable to the topography feedback loop. The phase shift of the cantilever oscillation to the driving signal can be related to stiffness and adhesion properties of the surface under investigation. Extensive research work has been performed in order to characterise the potential and the limits of each of the three basic modes of operation. Since

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

99

these issues are beyond the scope of this article we may refer to some more dedicated articles and the references given therein [7–15]. The intermittent contact mode has gained great importance for studying thin films of compliant materials and clusters only slightly adhered to the underlying substrate. Since the tip is in contact with the sample surface only for a fraction of the oscillation period (typically, ~6–20 ms) of the cantilever, the scanning-induced shearing forces imposed onto the tip-sample contact are negligible and even the most compliant polymers can be imaged in a non-destructive manner. The interpretation of the phase signal, however, is still a matter of vivid debate. Without claiming completeness, we may refer to some exemplary publications [8, 16–24]. Although the permanent tip-sample contact imposes to some extent lateral forces on the sample surface upon scanning, the contact mode operation is frequently used in studies where the film-substrate adhesion is strong enough, or thick films or even bulk samples are being investigated [25–31]. Mapping a certain area of the sample surface by scanning with the topography feedback being switched on essentially means that the total force acting on the tip is kept rather constant. Presuming that the surface forces acting between tip and sample do not exhibit significant changes, the adjustments of the vertical cantilever position necessary for keeping the preset value of the cantilever bending are equal to the height changes of the scanned topographic profile. Conversely, the scan velocity can be set to zero and the whole force-distance curve can be driven through. For given environmental conditions and a given cantilever, recording the whole force-distance curve provides the maximum amount of information available on a certain site of the surface under investigation. Frequently, the acquisition of force-distance curves is referred to as point spectroscopy. Several approaches have been developed for combining these two opposing acquisition techniques. One obvious approach is to scan the same area several times with the setpoint of the topography feedback being varied successively. However, only a rather limited force range is accessible by this method due to the instabilities of the feedback occurring at small loads. Instead of scanning continuously, the cantilever can successively be moved to different sites of an array and complete force-distance curves can be driven through and recorded on each site of the array. In this way a volume is mapped with each discrete lateral site being represented by a force-distance curve. The lateral translation can be performed either with tip and sample being in intimate contact or at the point of maximum distance between tip and sample. Owing to the fact that no lateral forces are imposed on the tip-sample contact, the latter approach may considered advantageous. In an approach described by Cappella et al. [32], the tip is moved towards the sample surface until a certain preset maximum total force (i.e. concave cantilever bending) is reached. All equidistant points of the force-distance curve are referred to this point. The spatial variation of force-distance curves can be visualised by displaying for each site of the array the force measured at some vertical distance from the reference point. Thus a whole series of that kind of force slice is available with each image representing a certain vertical distance from the point of maximum

100

Martin Munz et al.

Fig. 2 Schematic representation of the basic detection elements of the scanning force microscope and of the piezoelectric transducers generating the displacement modulations for purposes of dynamic mechanical measurements. The dynamic components of the tip-sample forces resulting from the normal/lateral displacement modulations are detected via the torsion/bending of the microscopic cantilever and the deflection of the laser beam reflected off the rear side of the cantilever. The positional shift of the latter is registered by means of a segmented photo-diode

cantilever bending. However, the rigorous approach of recording complete force-distance curves for an array of surface sites is rather consumptive both in storage space and in time. Whilst storage space is nowadays no more an issue of major concern, the acquisition time still matters. For instance, presuming an acquisition time per force-distance curve of 1 s, the total acquisition time for a 6060 array takes 1 h. Thus the achievable lateral resolution is rather limited. In a more pragmatic approach the force-distance curve is driven through comparatively rapid while the cantilever is being scanned laterally in a continuous manner (pulsed force mode) [33, 34]. Instead of saving the complete force-distance curve, only some characteristics such as the slope of the contact branch and the pull-off force are being extracted. In a similar approach the lateral translation is performed only when the tip is retracted from the sample surface (jumping mode) [35]. Low-amplitude displacement modulation can be superimposed to either the sample position or the position of the cantilever base; see Fig. 2. Via the stiffness of the cantilever for bending and torsion, the displacement modulation translates to force modulation. More precisely, out-of-plane (i.e. in the z-direction) displacement modulation results in modulated compressive loading of the tip-sample contact [36], whereas in-plane (i.e., in the x- or y-directions) displacement modulation results in modulated shear loading

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

101

[37]. Generally, these measurement techniques are called force modulation microscopy (FMM) and modulated lateral force microscopy (M-LFM), respectively. The dynamic response of the cantilever reflects the respective stiffnesses of the tip-sample contact. The highly sensitive lock-in technique can be employed for signal recovery. When using dual-channel lock-in amplifiers, both amplitude and phase of the response signal are available. Moreover, via variation of the modulation frequency, rate-dependent behaviour of the surface material can be investigated. As an alternative to the amplitude of dynamic cantilever deformation, the tip-sample stiffness can be calculated from the shift of the resonance frequencies of the cantilever [38]. Instead of indirect force modulation by means of displacement modulation, direct force modulation was accomplished by applying alternating magnetic fields. Producing a corresponding force on the cantilever requires a magnetisation in the field direction which can be achieved by gluing an appropriately oriented magnetic particle on its rear side [39]. Instead of the particle a magnetic film can be deposited [40]. Especially when operating in a liquid, the systems response is much less obscured by mechanical interferences than in the case of acoustic excitation [40]. By means of a set-up where the SFM cantilever is replaced, Syed Asif et al. [41] implemented a force-modulation technique using a three-plate capacitive load-displacement transducer. The transducer allows both electrostatic force actuation and displacement sensing. Owing to the vertical arrangement of the tip, upon loading there should not occur any appreciable lateral force component. Thus, the amplitude of displacement modulations needs not to be kept small in order to avoid slipping within the tip-sample contact. In SFM-based force modulation experiments, however, the cantilever tilt of ~10–15 with respect to the horizontal causes a lateral force component when loading the tip-sample contact. For minimising this effect, the modulation amplitude should be limited to the nanometre range [42]. When applying the modulation during scanning, amplitude and phase maps can be recorded simultaneously to the image of topography. Alternatively, on selected sites force-distance curves can be driven with simultaneous recording of the dynamic cantilever response signals [43]. With the scanning velocity being set to zero, the tip-sample contact is not affected by sliding. However, when applying in-plane displacement modulations, at high modulation amplitudes sliding of the tip sets in and the lateral forces acting on the tip are due to friction forces rather than shear deformation of the tipsample contact [44]. Owing to the anisotropy of most of the SFM-cantilevers, the lateral displacement modulation is mostly applied in direction perpendicular to the cantilever length axis, similarly to the scanning motion. Recently, a symmetric probe design has been devised in order to allow measuring lateral forces in arbitrary in-plane directions [45]. FMM was successfully applied in order to image local stiffness variations occurring on surfaces of polymer samples. For instance, Overney et al. [46] and Bar et al. [47] demonstrated by means of FMM that the frictional properties of lubricating monolayers not only depend on their adhesion properties but also on their compression stiffness. Consequently, stiffness should

102

Martin Munz et al.

be considered as a major parameter, e.g. when performing friction experiments with systematic variation of the adhesive forces by means of chemically modified tips (chemical force microscopy). Valuable information can be gained from the combined measurement of properties complementing one another. More recently, a combination of the pulsed force mode with FMM was proposed [48]. Thus the low frequency and large amplitude modulation of the vertical cantilever position (responsible for driving through the force-distance curve) is superimposed onto a second vertical modulation of high frequency and low amplitude. In a similar manner pulsed force mode can be combined with lateral vibrations of high frequency and low amplitude, i.e. with M-LFM [48]. Yet another promising combination is studying changes of local mechanical properties upon systematic variation of the sample temperature. Temperature variation was combined with phase imaging in intermittent contact mode [49], FMM [50], or pulsed force microscopy [34, 51]. When heating the total sample, some complications arise due to thermal drift effects. In particular, the stiffness of the cantilever may change upon temperature variation. Instead of applying a macroscopic heating stage, local heating can be achieved by special-purpose micro-cantilevers (scanning thermal microscopy, SThM). A thin thermoresistive filament located at the very end of the micro-cantilever can be used both as a local heating element and a thermal probe [52]. Instead of applying thin filaments, pronounced Joule heating may also be induced at the locus of geometric restrictions of the cantilever cross-section, where the electrical current density is increased [53]. The geometric restrictions can be a part of the cantilever design. When the tip encounters material exhibiting high thermal conductivity, the heat flow into the sample will increase and, consequently, for a given heating current the temperature of the probe itself will decrease. In contrast, by means of a special feedback loop, the probe temperature can be kept constant by adapting appropriately the magnitude of the heating current. As in a standard SFM, the bending of the cantilever upon topographic height changes is used as a control variable of the topography feedback loop. Alternatively to a d.c. heating current, application of a.c. heating currents allows use of the lock-in technique. Beyond the gain in sensitivity, via the frequency of temperature modulation the sensing depth can be varied in a systematic manner [54]. More detailed outlines of the emerging field of SThM can be found in the dedicated reviews by Majumdar [55] and Pollock and Hammiche [56]. Essentially, the sensitivity of FMM for stiffness variations is governed by the ratio of the cantilever stiffness to the stiffness of the tip-sample contact. Moreover, for strong disproportions between these two stiffnesses, the dynamic cantilever response was shown to be affected by frictional forces [57]. For typical cantilevers with bending stiffness, kc, of ~0.1–50 N/m this condition is easily met when dealing with compliant polymers. In the case of isotactic polypropylene (PP) with the Youngs modulus value E1.5 GPa, a tip radius of curvature R10 nm and an imaging force of 50 nN, the effective tip-sample stiffness is of the order of 30 N/m [26]. Accordingly, stiffness measurements on stiff materials such as metals or ceramics require much

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

103

stiffer cantilevers. On the other hand, a high cantilever stiffness is equivalent to a low force sensitivity. Especially when investigating materials that are very heterogeneous from the mechanical point of view, conflicting requirements on the cantilever stiffness arise from the presence of both stiff and soft components. For instance, when investigating mechanically heterogeneous materials such as carbon fibre reinforced polymers (CFRP), rather soft cantilevers are necessary for characterising the compliant polymer matrix surface without inducing any unintended surface modification, whereas stiff cantilevers are needed for characterising the stiff fibres. This dilemma can be sidestepped when noting that, for a given cantilever, the range of sufficient stiffness sensitivity can be extended to more stiff materials by operating at frequencies higher than its fundamental resonance frequency. In this regime the cantilever mass behaves like an inertial mass, i.e. the mass of the cantilever cannot move fast enough to keep up with the imposed ultrasonic excitation [58]. Owing to this effect, the cantilever becomes dynamically rigid and even on comparatively stiff materials a soft cantilever can induce elastic surface deformations. For excitation frequencies just above the resonance frequency where the amplitude response decreases like w2 (where w denotes the circular frequency of the imposed displacement modulation), FMM was referred to as scanning local-acceleration microscopy (SLAM) [58]. Similar experiments performed above the frequency of the fundamental eigenmode or higher ones are referred to as atomic force acoustic microscopy (AFAM) [59], ultrasonic force microscopy (UFM) [60] or overtone SFM [61]. For operating in the frequency range between ~100 kHz and several MHz and in the acoustic near-field, these techniques may be subsumed under the term near-field acoustic microscopy. At sufficiently high excitation amplitudes the non-linearity of the force-distance curve comes into play and the force averaged over one modulation period is non-vanishing. In a heterodyne approach both the cantilever and the sample were subjected to vertical displacement modulations at adjacent ultrasonic frequencies. Owing to mixing in the tip-sample contact, the cantilever vibrates at the beat (difference) frequency, and the corresponding detection signal can be analysed in terms of amplitude and phase [62]. This approach allows one to monitor phase shifts on the ultrasonic time scale. This feature may be exploited for studying fast relaxation processes. In the inertial regime the spatial distribution of the cantilever mass is of major importance. Thus, simple spring-mass models where the total cantilever mass is supposed to be concentrated within one point do not hold. Instead, the particular mass-distribution of the cantilever has to be taken into account, e.g. by means of analytical continuum mechanics models [63, 64] or by numerical finite element modelling [53, 61]. As demonstrated by Rabe et al. [63], the continuum mechanical theory of flexural waves of elastic beams applies quite convincingly to SFM-cantilevers made up of single-crystal Si. One of the most striking discrepancies between the continuum mechanics model taking into account the particular shape of the cantilever and the point-mass model is the change of the contact resonance upon increasing stiffness of the tip-sample contact. Whilst the latter predicts diverging

104

Martin Munz et al.

contact resonance frequencies, according to the continuum mechanics description the resonance frequencies are bound between the resonance frequencies of the free and of the fully clamped cantilever [63]. Furthermore, in the point-mass model there exists only one eigenmode, namely the resonance of the harmonic oscillator. Consequently, excitations well above the respective resonance frequency are strongly suppressed which is conflicting with the pronounced systems response observable at higher eigenmodes [65]. With increasing amplitude of the ultrasonic excitation, a broader part of the force-distance curve is being sensed, and new effects may be observed owing to its non-linearity. The resonance peaks become increasingly asymmetric, their maxima shift to lower frequencies, and the contact resonances show a hysteresis when the direction of the frequency scan is inverted [66]. Moreover, depending on the adhesion hysteresis the time-averaged force exhibits a discontinuity [60] which is generally referred to as mechanical diode effect. Quantitative evaluation of the resonance spectra in terms of Youngs modulus of tip and sample surface requires knowledge of the exact geometry of the cantilever. However, the cross-section of the cantilever beam may not be constant and the tip of the cantilever is quite often not located perfectly symmetric to the central length axis of the beam [59]. As well as the beam shape the shape of the apex of the tip also shows a non-negligible impact on the resonant behaviour. As shown by Dinelli et al. [67], a blunt tip gives no dependence of the contact stiffness on the normal force. Finally, a satisfying description of the dynamics of the tip-sample contact requires the finite lateral stiffness of the tip-sample contact to be taken into account [64, 68]. In general, when performing nanomechanical experiments using a tip-like probe, the overall shape of the tip, its micro-roughness, its chemical composition, and its surface chemistry are as important for the measurement as the topography, roughness, mechanics and surface chemistry of the surface under investigation. Unambiguous characterisation of this surface requires well-defined properties of the probing tip. Thus the conditions of tip preparation should be well-controlled and dedicated techniques are necessary for characterising the tip itself. Essentially, this can be achieved either by employing high-resolution microscopic techniques, such as scanning electron microscopy (SEM) and transmission electron microscopy (TEM), or by calibration procedures. Usually, the latter rely on inert reference samples with quite exactly known properties. Tip characterisation is rendered more and more difficult when the size of the tip reaches nanoscale dimensions. Therefore, despite the reduction in achievable lateral resolution, somewhat blunt tips are often used where the discreteness of matter is considered negligible and the essential parameters such as the radius of curvature of the apex can be determined with sufficient precision. For instance, initially blunt tips may be deliberately worn or covered with a thick coating. In a more rigorous approach, instead of the tip a small sphere-shaped particle attached to the cantilever may be employed for the nanomechanical experiments. This approach is generally referred to as colloidal probe microscopy (CPM) [69]. Micron-size beads of several materials such as glass [70], silica [71, 72], silicon nitride [73], polyethylene [74], polystyrene [75], cross-linked poly-

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

105

dimethylsiloxane [76] or cellulose [77, 78] were applied for measuring specific interaction forces. For studying the influence of surfactants or boundary layers, the bead may even be covered with a thin film [71]. Strongly deviating from the sphere-like shape of the attached particle, more recently another kind of nanosize probe technique was proposed, employing a multiwall carbon nanotube (MWNT) [79–81]. When being attached to the end of an SFM-tip with its length axis more or less parallel to that of the tip, the very end of the nanotube may serve as a well-defined nanosized probe (diameter 2–20 nm). The technique is expected to benefit from the extraordinary aspect ratio and the outstanding mechanical properties of carbon nanotubes.

3 Nanomechanics With increasing surface-to-volume ratio, surface forces play an increasing role, whereas volume forces such as the gravitational force become rather unimportant. In addition to the ever-present van der Waals force, hydrogen bonding forces, capillary forces, or long-range electrostatic forces may give further contributions to the total surface force. For instance, the different surface forces were outlined by Lee [82] and Fr berg et al. [83]. Owing to the adhesive forces, the atoms of the nearby tip and sample may rearrange and the contact area is nonzero even at vanishing external load. When being in contact, the adhesion-driven increase of the contact area between SFM-tip and sample impairs the achievable lateral resolution. Moreover, the SFMmeasurement may suffer from fluctuations of the atom positions. Given strong interactions between tip and sample, nanoscale welding can be observed [84]. Specifically, this is the case when bringing uncovered metals into mutual contact. Due to cohesive bonding a connective neck is formed. Upon retracting the tip, the connective neck elongates and finally disrupts at some pull-off force. The neck deforms through a series of structural deformations involving elastic and yielding stages [85]. Molecular dynamics simulations suggest that plastic yielding of nanometre sized contacts under tensile stress involves a series of structural transformations between ordered and disordered states of a small number of atomic layers adjacent to the constriction [86]. The adhesion forces are dramatically reduced when the surface is covered by low-surface energy monolayers such as hydrocarbons and fluorocarbons. Essentially, the coverage with a low surface energy film results in a kind of passivation of the tip-sample contact. In micro-electro-mechanical systems (MEMS) engineering, deposition of low surface energy coatings and chemical surface modification are considered as effective techniques for minimising plastic deformations as well as reducing friction forces and wear [87]. Furthermore, hydrophobisation of the surfaces allows one to alleviate the problem of adsorption of moisture at narrow gaps [88, 89]. Liquid bridging leads to stiction, the unintended sticking of moveable or bendable machine parts to nearby surfaces. Originally, the term stiction was introduced to

106

Martin Munz et al.

characterise the failures of hard disk drives in which the available accelerating force is insufficient to overcome local static friction due to adhesion forces among disk, slider and intervening lubricant [90]. In addition to the application of low surface energy coatings, the propensity for stiction may be reduced by minimising the apparent contact area. This can be achieved either by introducing regular microbumps/microdimples or by systematic modification of the microscale surface roughness [88, 89]. Beyond MEMS applications of molecular surface layers, biocompatibilisation of artificial microelectronic interfaces in order to provide reliable operational conditions for biochips under conditions of natural chemical or biological environment is another issue of growing importance [87]. The finite size of nanoscale contacts has strong implications on their mechanical properties. Recalling that plastic deformation in macroscopic crystals usually occurs by motion of dislocations, it is self-evident that the probability of nanoscale plastic flow being affected by dislocations is quite low. The concentration of dislocations in a crystal varies strongly, but even in an annealed single crystal the average separation between two nearby dislocations is small as compared to traditional engineering length scales, namely ~1 mm [91]. In the case of nanoscale mechanical contacts, however, (pre-existing) dislocations are rather unlikely to contribute to plastic deformations and the yield stress, sc, may approach the ideal value G·(2p)1, where G=E(2(1+n))1 is the shear modulus [91] with n denoting the Poisson ratio, i.e. the negative ratio of the relative deformations as measured in lateral and in normal direction. Similarly, the probability of the measurement to be affected by flaws decreases with decreasing sampling volume. Experimentally, the yield stress was found to be ~1/30 of the Youngs modulus, which is ~80 times larger than the macroscopic yield stress [85]. As shown by Bhushan [92], the hardness values decrease with increasing depth of indentation. For a sliding interface exhibiting near-zero friction and wear, surfaces should be free of nanoscratches and contact stresses should be below the hardness of the softer material to minimise plastic deformation. Consistently with the improved hardness, on the micro- to nanoscale the wear rates were observed to be smaller [92]. Beyond the size of the sampling volume, finite size effects may also affect the behaviour of the lubricant. With increasing contact pressure the lubricant is squeezed out of the contact up to several molecular layers. Structure and physical properties of the lubricant molecules are governed by their specific interactions with the confining rigid surfaces rather than by hydrodynamic quantities such as bulk viscosity. Owing to the predominance of surface forces and the finite size effects, the mechanical behaviour of nanoscale junctions is in many aspects strongly different from that of macroscopic contacts. The improved hardness and wear characteristics are promising for nano- and microscale mechanical devices. In contrast, nanomechanics and nanotribology cannot be predicted by simple down-scaling of the respective laws known from the macroscopic regime. Although the mechanical models neglecting the discrete structure of matter must break down at the atomic scale, continuum mechanics models

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

107

taking into account surface forces have proved to hold to rather small length scales. Providing analytical expressions, the various classical contact models have found widespread application in micro- and nanoscale mechanical experiments. And being approved on the micrometre scale, it seems quite natural to apply them to some extent to downscaled experiments. 3.1 Fundamentals of Tip-Sample Interactions

Several well-established mechanical contact models are available that are based on concepts from continuum elasticity. In general, the purpose of these models is to describe the deformation of two contacting spheres upon loading. Within the frame of these models, the case of a tip indenting a plane can be considered when setting the radius of curvature of one of the spheres to infinity and approaching the apex of the tip by a sphere of radius R. Despite the fact that these models originate from traditional macroscopic concepts, their use for describing the mechanical contact between SFM-tip and sample surface is rather common and has delivered a considerable number of reasonable results. Taking into account the nano-scale extension of the tip-sample contact, this is somewhat surprising as effects such as spontaneous rearrangements of single atoms are not contained in models that start from averaging over atomic length scales. Results from molecular dynamics simulations, however, corroborated the applicability of classical contact mechanics to nanoscale contacts, at least in a semi-quantitative manner [93]. Via contact mechanics the vital parameter contact area may be estimated, which cannot be directly measured by SFM or related nanoscale indentation techniques. Rather detailed overviews of classical contact mechanics were given in several review articles dealing with nanomechanics [6, 94–96]. This review shall be restricted to the essentials of contact mechanics necessary for grasping the basic ideas and for understanding related SFM experiments. 3.1.1 Normal Loading

Within the widely accepted Hertz-model [97] the mutual deformation of two contacting spheres is described, but without considering attractive surface forces. With increasing surface-to-volume ratio, however, surface forces play an increasing role. Given the same external load, models allowing for surface forces do provide different values of the contact area, the indentation depth and the stored elastic deformation energy. The Johnson-Kendall-Roberts (JKR) model [98] presumes short-range surface forces acting exclusively within the contact area. Owing to these surface forces, the same contact area is achieved for lower values of the external load than in the case of the Hertz model. The area density, w, of the thermodynamic adhesion energy is given by Dupr s equation:

108

w ¼ g ¼ g1 þ g2 g12

Martin Munz et al.

ð1Þ

where g1 and g2 denote the surface energies of the two contacting materials and g12 is the respective interfacial energy. w represents the energy per unit area necessary for separating the two materials and to increase their mutual distance to infinity. In the limit w=0 the JKR equations are identical to those of the Hertz model. The reduced modulus K of the mechanical contact is given by 1 1 n22 4 1 n21 K¼ þ ð2Þ 3 E1 E2 Denoting the radius of curvature of the tip with R and the external load with P, according to JKR theory the contact radius a is given by qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ R 3 P þ 3pwR þ 6pwRP þ ð3pwRÞ2 a ¼ ð3Þ K With P=0 we get a30=6pwR2K1. Hence a is finite even for zero external load P, owing to the adhesion forces. The detachment of tip and sample, the so-called pull-off, requires a tensile force Pad which characterises the adhesion force Pad=(3/2)pwR. With d denoting the deformation of the tip-sample contact as measured in the vertical direction, the corresponding stiffness kts=@P/@d of the contact is given by 3 kts ¼ aK 2

(3a)

The presumption of short-range surface forces underlying the JKR model is violated when dealing with comparatively stiff materials where the extent of elastic surface deformations is small compared to the range of surface forces. Instead the model according to Derjaguin, Muller and Toporow (DMT) is valid in this case. Following the DMT model [99], surface forces are limited to a ring-shaped area (annulus) enclosing the central contact area where the compressive forces are acting. In the annulus a

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

109

on the reFig. 3a,b Dependence of the reduced contact area Aand the reduced loadP duced deformation d, respectively, as calculated by means of the Maugis-Dugdale theory for different values of the transition parameter l. The JKR, DMT and Hertz limits are ¯ P and d are dimenindicated. Negative deformations d occur only in the JKR limit.A, sionless parameters given by a(pwR2K1)1/3, P/pwR and d(p2w2RK2)1/3, respectively. The JKR curves are characterised by nose-like regions; at the extremal point of the nose-like region instability occurs. Adapted from [6]

action between two parallel planar surfaces separated by the same distance. In case of violation of the constraint a<

110

Martin Munz et al.

Fig. 4 Map of the validity regimes of the several contact mechanics models (adhesion map). Pad/P denotes the ratio between the adhesive component of the load and the total one. d1 is the elastic compression, whereas dad is the deformation due to adhesion. h0 is the effective range of action of adhesive forces (h0=0.97z0, whereby z0 denotes the equilibrium interatomic distance). Adapted from [108]

A map is commonly used for displaying the regimes of validity of the particular contact models (Fig. 4). The coordinates of the map are given by the ¼ P=pwR. Here, transition parameter l as given by Eq. (4) and the ratio P P denotes the external load and pwR denotes a representative adhesive pulloff force Pad. The Hertz model applies in the majority of engineering situations where high loads allow for neglecting adhesive forces. In the rigid zone (Bradley regime) all elastic deformation is small compared with the range of the surface forces [108]. The force-deformation relation of the DMT model includes the transition parameter l which indicates that the DMT model does not encompass the rigid Bradley limit [109]. The DMT model was shown to be valid, in particular when a large meniscus of condensed liquid is present [110, 111]. Similar to Muller et al. [103], several authors performed self-consistent numerical computations of the non-linear equations based on the LennardJones potential instead of dealing with analytical approaches. Greenwood [108, 109] and Feng [112] calculated the dependence of the pull-off force on the transition parameter l. For fixed g and R, softer spheres require less force to separate, though they deform more significantly. At the extreme limits of small and large values of l, however, the pull-off force becomes virtually independent of l. On a local scale, this is consistent with the prediction of the JKR and the DMT model that the pull-off force is independent of elastic moduli of spheres [112]. The errors made by using the Dugdale approximation may be assessed by comparing with the Lennard-Jones potential [108] which embodies the essential features absent in the Dugdale model, namely the finite repulsive compliance and continuously decreasing attraction. As shown by Johnson and Greenwood [108], the effect of the Dugdale approximation only becomes significant at low values of the transition parameter l. Similarly, nu-

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

111

merical calculations by Barthel [113] indicate that the nature of the interaction has a very moderate influence on the solution. The transition from DMT to JKR is only slightly delayed if a very short-range interaction like a linear one is replaced by a longer-range interaction like van der Waals. The adhesion energy and the geometry of the contact are considered as the dominant parameters. The low modulus of elastomers generally ensures that l>80, so that such materials fall well into the JKR regime [108]. In the case of the surface force apparatus (SFA), the compliance of the glue along with high adhesion results in l40, indicating the applicability of the JKR equations. The SFM, however, employs stiff and sharp tips, providing in the case of UHV conditions 0.2l1.1 [114, 115] and meeting the condition for the transition region. Upon variation of the vapour pressure, the pull-off force may change either due to the adhesion energy w or due to the transition parameter l [113]. From their measurements with Si3N4 tips on high-density polyethylene, Pi trement and Troyon [106] receive from their data evaluation procedure the l-values 0.045 and 0.143, respectively, measured both under ambient conditions and in vacuum. The models outlined above are based on the presumption of perfectly elastic behaviour. When dealing with viscoelastic materials such as polymers, however, the rate dependency of the Youngs modulus has to be taken into account. Beyond the contact situation of dry viscoelastic materials, some viscous dissipation occurs when tip or sample are covered by thin liquid layers, e.g. thin lubricating films. Given the viscoelastic correspondence principle, stresses and strains of the viscoelastic material can be calculated by replacing the Youngs modulus with the creep compliance function J(t), respectively, the stress relaxation function E(t). For very short times (t!0) the value of E(t) is equal to the instantaneous value E0, whereas in the opposite limit t!1 the relaxed value E1 is attained. The ratio E0/E1 is of the order of 104 for elastomers. Furthermore, adhesion hysteresis is a major feature of indentation experiments performed on viscoelastic materials. The energy necessary for separation is larger than the energy returned when bringing indenter and sample into contact. In general, adhesion hysteresis is governed by the deformation rate. The fundamental contributions to the description of contact mechanics of viscoelastic materials were made by Ting [116], Roberts and Thomas [117], Schapery [118], Maugis and Barquins [119] and Greenwood and Johnson [120]. Beyond the contact radius a the second significant length is the length l along which the surface forces act. The problem is usually described in terms of fracture mechanics and the velocity of the advancing or receding circumferential line enclosing the contact area pa2 is referred to as crack propagation velocity V=da/dt. Thus, the periphery of the contact is viewed as the tip of a crack. Essentially, the deformation rates are given by V/a and V/l. They are the characteristic rates for creep effects and crack effects, respectively. The latter will be dominant when V/l is comparable to the characteristic relaxation rate of the viscoelastic material. For l<

112

Martin Munz et al.

of the adhesion behaviour is governed by the creep compliance function J(l/V). Glassy behaviour is expected in the limit of rapid tip-sample separation, i.e. in the limit l/V!0. At higher loading rates creep effects play an increasing role and their being neglected is no longer justified. A continuum mechanics model including both creep and crack effects was presented by Hui et al. [121]. Essentially, the problem is broken down into an outer problem of viscoelastic contact mechanics and an inner problem of adhesion mechanics. Giri et al. applied this model for analysing their nanoindentation experiments performed on films of tempered styrene-butadiene copolymer latexes [122]. Similar data recorded under low-loading conditions [123], however, were shown to be appropriately described by a model due to Johnson [124] where creep effects are neglected. Along with the loading rate Vakarelski et al. [125] observed some increase of the adhesion force with the holding time at the position of maximal load. Similar to the results of Deruelle et al. [126], as derived from macroscopic measurements, this result suggests that it takes some time for interdiffusion of polymer chains or for establishing bonds across the interface, especially in the case of rough surfaces. 3.1.2 Micro-Indentation Testing

When applying larger indentation depths the presumption d<

Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)

113

Fig. 5a,b Schematic representation of: a the tip-sample contact upon high loading; b the according compliance curve. In the case of perfectly plastic response the unloading curve is identical to the vertical line intersecting with the abscissa at hmax. In general, some viscoelastic recovery occurs and the residual impression depth hg is smaller than hmax. The difference hchg represents the extent of viscoelastic recovery. Ap and Ae denote the dissipated and the recovered work, respectively. Ap=0 for perfect elastic behaviour, whereas Ae=0 for perfect plastic behaviour. The viscoelastic-plastic properties of the material may be described by the parameter Ap(Ap+Ae)1. The contact strain increases with the attack angle q. Adapted from [138]

Additionally, when dealing with viscoelastic materials such as polymers some time-delayed viscoelastic recovery occurs. The residual impression in the sample surface indicates plastic deformation. Both loading and unloading curves are recorded. From the slope of the initial elastic recovery, the contact stiffness can be calculated. Evaluation of the compliance curve in terms of moduli needs knowledge of the area of contact. Hence, tips with rather well-defined geometry are used for performing indentation experiments. The most important indenters are of the Berkovich-type (three-sided pyramidal), Vickers-type (four-sided pyramidal), sphere-like indenters and cone-like indenters. The basic features of compliance curves are depicted in Fig. 5. The most frequently used method of analysis of depth-sensing indentation testing was developed by Oliver and Pharr and is described in great detail in [131]. More recently, a review of the different analysis methods was given by Fischer-Cripps [132]. For any indenter geometry it has been found that the relationship between stiffness S and elastic modulus K may be defined as follows [133]: @P 3 b pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð5Þ Sjhmax ¼ jhmax ¼ pﬃﬃﬃ Amax K @h 2 p where Amax denotes the projection of the contact area between the indenter and the material at Pmax, and K denotes the reduced modulus as defined in Eq. (2). For distinguishing from purely elastic deformations, d, in the case of high-strain indentation experiments exceeding the elastic limit, the penetration depth is referred to as h. b is a parameter dependent on the indenter

114

Martin Munz et al.

geometry (1**
Pmax Aðhc Þ
ð6Þ
Here, hc denotes the vertical distance along which contact is made. For soft metals, the hardness is directly proportional to the flow stress, with the constant of proportionality being ~3. This constant is material-specific and depends on the state of strain underneath the indenter. For a fully plastic indentation, this constant is approximately equal to 2.8 for polymethylmethacrylate (PMMA) [134]. It is worth noting that hardness and elasticity are rather unrelated to each other. Whilst the physical origin of elasticity is the stretching/compression of bonds or it may have an entropic origin as for rubber, plasticity has its origin in the creation and motion of imperfections. Accordingly, the concentration of imperfections shows a rather small impact on the Youngs modulus, but it affects the plastic flow stress [91]. The correlation between the cross-sectional area of the indenter and the distance from its tip is given by the so-called indenter area function Ai(h). Usage of Ai(h) is based on the observation that, at peak load, the material conforms to the shape of the indenter to some depth hc [131]. From Fig. 5 the relation S=ePmax(hmaxhc)1 is obvious. hc can be deduced from the loaddisplacement data, and the projected area of contact can be estimated directly from the area function Ai(h). The constant e is related to the geometry of the indenter. For perfect Berkovich indenters the area function Ai(h) is given by Ai(h)=24.5·h2. The area function Ai(h) is usually calibrated from indentations on hard and plastic materials such as fused silica [131]. Alternatively, corresponding images of the indenter may be recorded via scanning electron microscopy (SEM) or SFM. Vickers and Berkovich pyramidal indenters are presumed to have point-like tips, whilst usually tip regions are more or less blunted due to fabrication tolerance and wear. These deviations play an increasing role with decreasing indentation depths. Scanning of the indenter tip by means of SFM was used for characterising changes of its shape due to wear [135]. As shown by Oliver and Pharr [131] by careful examination of indentation load-displacement data, the unloading curve can be accurately described by the power law relation P=m(hhr)n, where m and n are fitting parameters and hr denotes the remaining plastic deformation at zero load. The initial unloading slope is found by differentiating analytically this expression and evaluating the derivative at the peak load and the corresponding displacement. The procedure of data evaluation outlined above works well only when the key quantities unloading stiffness, indenter area function and load frame compliance are known with some precision. The latter is important especially for large indentations made in high-modulus materials. Imaging the residual impression is not required when applying the indenter area function Ai(h). However, effects such as piling-up, sinking-in or cracking of material around the indenter can occur which lead to inaccuracies in the
Materials Contrasts and Nanolithography Techniques in Scanning Force Microscopy (SFM)
115
evaluation scheme as outlined above. Thus imaging of the residual indent seems to be useful for detecting such irregularities [134, 136]. Again, SEM or SFM may be used for imaging the residual indent. SFM allows the recording of a true topographic map with calibrated height data; however, it should be borne in mind that the SFM topography image is a convolution of the true topography with the shape of the SFM tip. This effect may only be neglected if the tip used for imaging is considerably sharper than the tip used for indenting. Calculating the hardness from the ratio of maximum applied load and the contact area as deduced from the image of the residual impression is a more simple approach than the compliance method. However, this is not applicable for materials exhibiting a considerable amount of viscoelastic recovery as no residual impression will be visible [137]. Micron-indentation measurements on polymers revealed creeping effects, resulting in a rounding of the loading-unloading peak [138]. The rounding can be circumvented by holding the maximum load for a certain time long enough to settle down creeping. Moreover, a significant strain-rate hardening effect was observed (e.g. for polymethylmethacrylate (PMMA)), that is, at higher strain rates the polymer accommodates a lower displacement at a constant maximum applied load [138]. Another effect to be borne in mind is work hardening, either due to high strain rates imposed during the indentation experiment or as a result of stresses imposed during the polishing procedure. Surface oxidation or contamination may lead to deviations of the surface properties from those of the bulk. As the regularity of the indenter-surface contact area is impaired by surface roughness, flat surfaces are desirable for running indentation experiments. Last but not least, indentation size effects are an issue of concern. With increasing sampling volume the probability of encountering flaws rises [136]. When investigating thin films, the depth of indentation should be no more than one-tenth of the film thickness in order to avoid the measurement being influenced by the underlying substrate [139]. Failure mechanisms and wear behaviour of thin coatings are increasingly being studied by means of micro-/nanoindentation and micro-/nanoscale scratching [92, 140]. 3.1.3 Shear Loading
The tip-sample contact will deform elastically if a lateral force smaller than the force of limiting friction is applied. In fact, microslip occurs at the contact periphery even for very small lateral forces, and upon increasing lateral forces microslip spreads throughout the interface [141]. Consistently, contact area measurements by Savkoor and Briggs [142] during the static friction phase revealed a decreasing contact size with increasing values of the tangential force. When surmounting the force of limiting friction, the entire contact slips and the tip begins to slide. For lateral forces well below the force of limiting friction, however, microslip effects may be neglected [143]. Presuming a lateral force Qx acting on the contact, the lateral displacement dx between different points in the tip and the sample may be written as
116
Martin Munz et al.
Qx=8bG*·dx=klatts·dx [144]. Here, b denotes the effective radius of contact and G* the reduced shear modulus of tip and sample: 2 n1 2 n2 1 G ¼ þ ð7Þ G1 G2 klat ts ¼ 8bG
ð8Þ
is the lateral stiffness of the tip-sample contact for small lateral forces. Owing to its definition b=a+n(ca) with 0**

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close